# Polymer Reaction & Colloid Engineering

Institute for Chemical and Bioengineering Department of Chemistry and Applied Biosciences ETH Zurich 8093 Zurich,Switzerland

LECTURE NOTES (intended to complete but not to substitute the lectures)

POLYMER REACTION & COLLOID ENGINEERING

Prof.Dr. M. Morbidelli

Prof.Dr. P. Arosio

November 17, 2016

AUTUMN SEMESTER 2016 Contents

1 Free-Radical Polymerization 6 1.1 Chemical Reactions ...... 6 1.1.1 Initiation ...... 6 1.1.2 Propagation ...... 7 1.1.3 Chain Transfer ...... 7 1.1.4 Bimolecular Termination ...... 9 1.2 Diﬀusion Control of Chemical Reactions ...... 9 1.3 Polymerization Processes ...... 11 1.3.1 Bulk Polymerization ...... 11 1.3.2 Solution Polymerization ...... 11 1.3.3 Suspension Polymerization ...... 11 1.3.4 Emulsion Polymerization ...... 11 1.4 Kinetics of Free-Radical Polymerization ...... 12 1.4.1 Involved Chemical Reactions ...... 12 1.4.2 Population Balance Equations in a Batch Reactor ...... 12 1.4.3 Rate of Monomer Consumption ...... 14 1.5 Pseudo Steady State Approximation ...... 15 1.5.1 Stiﬀness Ratio ...... 18

2 Chain Length Distribution of Polymers 20 2.1 Population Balance Equations ...... 20 2.1.1 Active Chains ...... 20 2.1.2 Dead Chains ...... 22 2.2 Instantaneous Chain Length Distribution ...... 24 2.2.1 Number Distribution and Number Average ...... 24 2.2.2 Weight Distribution and Weight Average ...... 25 2.2.3 Polydispersity ...... 26 2.2.4 Summary ...... 27

3 Cumulative Properties of Polymers 28 3.1 Cumulative Chain Length Distribution, Moments, and Properties ...... 28 3.1.1 Width of the Cumulative Distribution ...... 30 3.2 Designing Polymerization Processes with Respect to Desired CLDs . . . . . 31 3.2.1 Case I: Termination by Combination is Negligible ...... 31

2 Contents

3.2.2 Case II: Termination by Combination Dominates ...... 33

4 Copolymerization 35 4.1 Kinetics of Copolymerization ...... 35 4.1.1 Involved Chemical Reactions ...... 35 4.1.2 Long-Chain Approximation ...... 36 4.1.3 Rate of Monomer Consumption ...... 37 4.2 Chain Length Distribution of Copolymers ...... 38 4.2.1 Population Balance Equation ...... 38 4.2.2 Pseudo-Homogeneous Approach ...... 38 4.2.3 Kinetics of Multi-Monomer Polymerization ...... 39 4.3 Chain Composition Distribution of Copolymers ...... 41 4.3.1 Instantaneous Chain Composition ...... 41 4.3.2 Composition Drift ...... 43 4.3.3 Chain Composition Control ...... 44 4.3.4 Reactor Monitoring and Control ...... 50

5 Heterogeneous Free-Radical Polymerization 53 5.1 Concept of Micellar Particle Nucleation ...... 53 5.2 Radical Segregation ...... 54 5.3 Phase Partitioning ...... 56 5.3.1 Monomer ...... 57 5.3.2 Emulsiﬁer ...... 57 5.4 Colloidal Stability ...... 58 5.5 Kinetic Mechanism of Emulsion Polymerization (Smith & Ewart, 1954) . . . . 58 5.6 Kinetics of Micellar Particle Nucleation ...... 61 5.7 Distribution of Active Radicals in the Polymer Particles ...... 63

6 Stability of Colloidal Suspensions 67 6.1 Kinetic Stability of Colloidal Suspensions ...... 67 6.2 Interaction between two Charged Bodies ...... 68 6.2.1 van der Waals Forces ...... 68 6.2.2 Electrostatic Forces ...... 72 6.2.3 Total Interaction Energy ...... 84 6.2.4 Simple Manifestation of Electrical Double Layers: Soap Films . . . . 85 6.3 Coagulation of Colloidal Suspensions ...... 86 6.3.1 Aggregation by Potential Control ...... 86 6.3.2 Aggregation by Electrolyte Addition ...... 88 6.4 Steric Interactions ...... 91

3 Contents

7 Kinetics and Structure of Colloidal Aggregates 95 7.1 Diﬀusion Limited Cluster Aggregation – DLCA ...... 95 7.1.1 Aggregation Rate Constant – DLCA ...... 95 7.1.2 Cluster Mass Distribution – DLCA ...... 97 7.1.3 Role of Aggregate Morphology – DLCA ...... 98 7.2 Reaction Limited Cluster Aggregation – RLCA ...... 100 7.2.1 Aggregation Rate Constant – RLCA ...... 100 7.2.2 Role of Cluster Morphology – RLCA ...... 103 7.2.3 Cluster Mass Distribution – RLCA ...... 105 7.3 Comparison of Aggregation Regimes – DLCA vs. RLCA ...... 105 7.3.1 Aggregation Rate Constant – DLCA vs. RLCA ...... 105 7.3.2 Cluster Mass Distribution – DLCA vs. RLCA ...... 106 7.3.3 Aggregate Morphology – DLCA vs. RLCA ...... 109 7.3.4 Comparison to Experimental Data ...... 110 7.4 Cluster Coalescence ...... 111 7.5 Solid Suspensions under Shear ...... 116 7.5.1 Shear induced Aggregation ...... 116 7.5.2 Shear induced Breakage ...... 121 7.6 Gelation of Colloidal Suspensions ...... 122 7.6.1 The Gelation Process ...... 122 7.6.2 Brownian-Induced Gelation ...... 124 7.6.3 Shear-Induced Gelation ...... 125 7.7 Experimental Characterization of Colloidal Suspensions ...... 128 7.7.1 Light Scattering ...... 128 7.7.2 Static Light Scattering ...... 129 7.7.3 Dynamic Light Scattering ...... 135 7.8 Zeta Potential, Electrophoretic Mobility, and Surface Charge Density . . . . . 137

8 Proteins and Bioprocesses 142 8.1 Proteins and Biomolecules ...... 142 8.2 Enzyme Kinetics ...... 146 8.2.1 Michaelis-Menten Equation ...... 146 8.2.2 Engineering of enzyme kinetics ...... 147 8.3 Bioprocessing ...... 149 8.3.1 Microbial growth ...... 149 8.3.2 Reactor design ...... 150 8.3.3 Product recovery, formulation and delivery ...... 153 8.3.4 Choice of the reactor conﬁguration ...... 153 8.3.5 Biopharmaceuticals ...... 154

9 Protein Aggregation 162 9.1 Proteins and Colloids ...... 162

4 Contents

9.2 Experimental biophysical techniques ...... 164 9.3 Kinetic Model and PBE ...... 167 9.3.1 Case Study: aggregation of a monoclonal antibody (mAb-1) . . . . . 168 9.4 Protein Misfolding and Aggregation in the Biomedical Context ...... 173 9.4.1 Functional role of protein self-assembly and aggregation in biology . 173 9.4.2 Role of aberrant protein aggregation in pathology: amyloid ﬁbrils . . 174 9.4.3 Kinetic and thermodynamic stability of amyloid ﬁbrils ...... 175 9.4.4 Aggregation mechanism of amyloid ﬁbrils ...... 177 9.4.5 Role of chemical kinetics in drug discovery ...... 178

5 Chapter 1 Free-Radical Polymerization

1.1 Chemical Reactions

1.1.1 Initiation

The initiation reaction produces free radicals. There are several ways to do this:

• Chemical initiation The decomposition of the initiator (e.g. AIBN) forms free radicals:

CH3 CH3 CH3

kd NCCN N C CN N2 + 2 NC C

CH3 CH3 CH3

kd • • I2 −→ I + I (rd = kdI2) • kI • I + M −→ R1

dI• = 2 f k I − k I• M ≈ 0 (1.1) dt d 2 I

• ⇒ kII M = 2 f kdI2 ≡ RI (1.2) where f is the initiator eﬃciency, typically f = [0.5, 1]. Note that in order to ensure

a continuous production of radicals all over the process, 1/kd should be larger than the characteristic time of the polymerization reaction. Examples of the decomposition

characteristic time, τd for some commercial initiators are:

6 CHAPTER 1. FREE-RADICAL POLYMERIZATION

τd T

Acetyl peroxide 2 h 80 ◦C Cumyl peroxide 12 h 110 ◦C t-Butyl hydroperoxide 45 h 150 ◦C

Since this is a ﬁrst order process, τd = 1/kd.

• Thermal initiation: thermal decomposition of the monomer (e.g. styrene). This represents a danger, for example during monomer transportation, since it may lead to undesired polymerization of the monomer. For this reason, inhibitors (scavengers of radicals) are usually added to the monomers before storage. This causes the occurrence of a non reproducible induction period when such monomers are polymerized.

• Initiation by radiation The decomposition of the initiator is caused by light or another source of radiation. Since this method is quite expensive, it is only applied to polymerization systems oper- ating at very low temperatures.

1.1.2 Propagation

Propagation is the addition of a monomer molecule to a radical chain.

R R k + p

n-1 n

k • p • • Rn + M −→ Rn+1 rp = kpRn M

1.1.3 Chain Transfer

• Chain transfer to monomer

• kfm • • Rn + M −→ Pn + R1 r = kfmRn M

The reactants are the same as for the propagation reaction, but the activation energy is 3 much larger. Accordingly, kfm is usually at least 10 times smaller than kp. This reaction

7 CHAPTER 1. FREE-RADICAL POLYMERIZATION

R R k + fm +

n-1 n-1

leads to the formation of a polymer chain with a terminal double bond. This can induce chain branching through the terminal double bond propagation reaction.

• Chain transfer to chain transfer agent

• kfs • • Rn + S −→ Pn + R1 r = kfsRnS

A chain transfer agent, S is a molecule containing a weak bond that can be broken to

lead to radical transfer, similarly as in the case of monomer above (e.g. CCl4, CBr4, mercaptans).

• Chain transfer to polymer

k • fp • • Rn + Pm −→ Pn + Rm r = kfpRn (mPm)

• In this reaction the growing radical chain, Rn extracts a hydrogen from the dead chain,

Pm. Since this extraction can occur on any of the m monomer units along the chain, the

rate of this reaction is proportional to the length of Pm.

General observations on the role of chain transfer reactions:

- The concentration of radicals is not aﬀected and therefore the rate of monomer con- sumption is also unchanged.

- The growth of polymer chains is stopped and therefore shorter chains are produced.

- Each transfer event leaves a diﬀerent end-group on the chain that can be detected (NMR, titration) so as to identify and quantify the corresponding chain transfer reaction.

- Nonlinear (branched) polymer chains are produced: directly by chain transfer to poly- mer or indirectly through the propagation of the terminal double bond left by a chain transfer to monomer event.

8 CHAPTER 1. FREE-RADICAL POLYMERIZATION

1.1.4 Bimolecular Termination

Bimolecular termination occurs according to two diﬀerent mechanisms: termination by com- bination and termination by disproportionation. Their relative importance depends upon the speciﬁc polymerization system.

• Termination by combination

R R R k + tc R m-1

n-1 m-1

n-1

• • ktc • • Rn + Rm −→ Pn+m r = ktcRnRm

This reaction results in an increase of the chain length.

• Termination by disproportionation

R R R R k + td +

n-1 m-1 n-1 m-1

• • ktd • • Rn + Rm −→ Pn + Pm r = ktdRnRm

The chain length remains constant during the termination reaction. Note that also in this case chains with terminal double bond are produced, which can therefore lead to the occurrence of branching.

1.2 Diffusion Control of Chemical Reactions

When dealing with macromolecules we can regard the reaction event as constituted by two steps in series:

9 CHAPTER 1. FREE-RADICAL POLYMERIZATION

• a relative motion or diﬀusion of the two molecules in order to overlap their active centers (note that the centers of gravity of the two macromolecules already overlap, i.e., we have no mass transport involved)

• the reaction event per se, i.e., breakage and formation of chemical bonds.

Since the two steps are in series, the slowest one deﬁnes the rate of the overall process, that is the reaction rate.

In the case of termination by combination, the reaction step is very fast, while the diﬀusion step is slow due to the diﬃculty of the two macromolecules to ﬁnd their respective active centers (the two chains exhibit strong entanglements). The result is that diﬀusion is the rate determining step. Accordingly the rate constant of termination by combination, ktc has the following characteristics:

• decreases with viscosity (and therefore with conversion)

• increases very mildly with temperature

• is substantially independent of the chemical nature of the radicals.

This eﬀect is usually referred to as Trommsdorf or gel eﬀect. This is responsible for the accumulation of radicals during the reaction which can also lead to thermal runaway of the reactor.

Let us now consider the other involved reactions. It is found that in most cases they are not diﬀusion controlled for the following reasons:

• termination by disproportionation: the reaction step is slower (can still be diﬀusion controlled)

• chain transfer to polymer: reaction is slower and diﬀusion is faster since we have many reactive points along the chain.

• propagation: reaction is slower and diﬀusion much faster due to the small dimension of the monomer (this reaction stops below the glass transition temperature)

10 CHAPTER 1. FREE-RADICAL POLYMERIZATION

1.3 Polymerization Processes

1.3.1 Bulk Polymerization

• ingredients: monomer and initiator only

• products: high purity

• disadvantage: poor temperature control at high conversion (thermal runaway!)

1.3.2 Solution Polymerization

• ingredients: solvent, monomer and initiator

• guarantees an eﬃcient heat transfer

• disadvantage: low productivity because of low solubility of the produced polymer

1.3.3 Suspension Polymerization

• ingredients: water, monomer, initiator and stabilizer

• size of formed polymer particles approx. 0.01 − 0.5 cm

• initiator is solubilized in monomer phase

• polymerization occurs within the monomer droplets

• high productivity (> 40 % solid)

• heat production is under control

1.3.4 Emulsion Polymerization

• ingredients: water, monomer, initiator and stabilizer

• size of formed polymer particles approx. 0.05 − 1 µm

• initiator is solubilized in water phase

• polymerization occurs mainly within the polymer particles

11 CHAPTER 1. FREE-RADICAL POLYMERIZATION

• high productivity (> 40 % solid)

• heat production is under control

• advantage: high molecular weight as well as high polymerization rate can be achieved simultaneously

1.4 Kinetics of Free-Radical Polymerization

1.4.1 Involved Chemical Reactions

• Initiation I2 −→ 2 R1 r = 2 f kdI2 ≡ RI k • p • • Propagation Rn + M −→ Rn+1 r = kp MRn • kfm • • Chain Transfer Rn + M −→ R1 + Pn r = kfm MRn • kfs • • Rn + S −→ R1 + Pn r = kfsSRn k • fp • • Rn + Pm −→ Rm + Pn r = kfpRn (mPm) • • ktc • • Termination Rn + Rm −→ Pn+m r = ktcRnRm • • ktd • • Rn + Rm −→ Pn + Pm r = ktdRnRm

where n, m = [1...∞]

Note that all reaction rate constants are assumed to be chain length independent, i.e., we use the Terminal Kinetic Model.

1.4.2 Population Balance Equations in a Batch Reactor

• n=1: dR• 1 = R − k MR• dt I p 1 ∞ X • + (kfm M + kfsS ) Rn n=2 ∞ ∞ X X k ( P ) R• − k (nP ) R• + fp 1 1 n fp n 1 n=1 n=1 ∞ X − (k k ) R• R• tc + td n 1 (1.3) n=1

12 CHAPTER 1. FREE-RADICAL POLYMERIZATION

• n ≥ 2: dR• n = k MR• − k MR• dt p n−1 p n • − (kfm M + kfsS ) Rn ∞ ∞ X • X • +kfp (nPn) Rm − kfp (mPm) Rn m=1 m=1 ∞ X − (k k ) R• R• tc + td m n (1.4) m=1 Let us deﬁne ∞ • X • R ≡ Rn (1.5) n=1 and sum up equations (1.3) and (1.4) from n = 1 to ∞. In this way we obtain: dR• dR• X∞ dR• = 1 + n dt dt dt n=2 ∞ ∞ • X • X • = RI − kp MR1 + kp M Rn−1 − kp M Rn n=2 n=2 ∞ ∞ X • X • + (kfm M + kfsS ) Rn − (kfm M + kfsS ) Rn n=2 n=2 ∞ ∞ X X k ( P ) R• − k (nP ) R• + fp 1 1 n fp n 1 n=1 n=1 ∞ ∞ ∞ ∞ X X X X k nP R• − k R• (mP ) + fp [ n] m fp n m n=2 m=1 n=2 m=1 ∞ ∞ ∞ X X X − (k k ) R• R• − (k k ) R• R• tc + td 1 n tc + td n m (1.6) n=1 n=2 m=1

dR• X∞ = R − k MR• + k M R• dt I p p n n=1 ∞ ∞ ∞ X X X k R• P (nP ) − k (nP ) R• R• + fp 1 + n fp n 1 + n n=2 n=1 n=2 ∞ X − (k k ) R• R• R• tc + td 1 + n (1.7) n=2 dR• ⇒ = R − (k + k ) R•2 (1.8) dt I tc td

13 CHAPTER 1. FREE-RADICAL POLYMERIZATION

1.4.3 Rate of Monomer Consumption

Under the assumption of pseudo steady state for the concentration of active chains (see 1.5) we can write: dR• = R − (k + k ) R•2 = 0 (1.9) dt I tc td and obtain: r R R• = I (1.10) (ktc + ktd)

Let us now consider the rate of monomer consumption, Rp. Neglecting the chain transfer to monomer reaction we have: ∞ r X R R = k M R• = k M I (1.11) p p n p (k + k ) n=1 tc td The mass balance for the monomer can be written as follows (still in the case of a batch reactor): dM = −R = −k MR• (1.12) dt p p • Considering kpR as the pseudo-ﬁrst order reaction rate constant for monomer consumption, we can conclude that the characteristic time for the process of monomer consumption is τM = 1 • . Using the conversion instead of the concentration, X = (M0 − M) /M0, and combining kpR equation (1.11) and (1.12) we get: r dX 1 dM Rp RI = − = = (1 − X) kp (1.13) dt M0 dt M0 (ktc + ktd)

r dX RI = kp dt (1.14) (1 − X) (ktc + ktd) where the initial condition is X(t = 0) = 0. Therefore we can write:

Z t r RI X = 1 − exp − kp · dt (1.15) 0 (ktc + ktd) As long as the temperature in the reactor remains constant, i.e., before the onset of the so- called gel eﬀect, ktc and ktd are independent of the conversion X. Moreover, if the half-life of the initiator is much larger than the characteristic time of the monomer consumption process,

τM, τd τM, the solution to equation (1.15) is: r RI X = 1 − exp −kp · t (1.16) (ktc + ktd)

14 CHAPTER 1. FREE-RADICAL POLYMERIZATION

X

1

equation (1.16) gel effect (Trommsdorf)

t

• Which kinetic parameter(s) can be estimated from the plot of the monomer conversion vs. time?

1.5 Pseudo Steady State Approximation

In this section we introduce an important concept often used in chemical reaction engineer- ing, the so-called pseudo steady state approximation (PSSA). Therefore, let us consider two consecutive ﬁrst-order reactions occurring in a batch reactor:

I −→ R (r1 = k1I)

R −→ P (r2 = k2R) with initial conditions I(0) = I0, R(0) = R0 and P(0) = 0. The mass balances are: dI = −k I (1.17) dt 1 dR = k I − k R (1.18) dt 1 2 The solution of equation (1.17) is:

I = I0 exp (−k1t) (1.19) which substituted in equation (1.18) leads to a linear non-homogeneous ODE. We consider the solution of the homogeneous associated equation:

H R = A exp (−k2t) (1.20)

15 CHAPTER 1. FREE-RADICAL POLYMERIZATION and then the particular solution having the form:

P R = K exp (−k1t) (1.21)

Substituting in equation (1.18) we get:

−k1K exp (−k1t) = k1I0 exp (−k1t) − k2K exp (−k1t) (1.22)

⇒ k1K + k1I0 − k2K = 0 (1.23)

k I ⇒ K = 1 0 (1.24) k2 − k1 Thus the general solution is:

H P k1I0 R = R + R = A exp (−k2t) + exp (−k1t) (1.25) k2 − k1 which using the initial condition to compute A reduces to: ! k1I0 k1I0 R = R0 − exp (−k2t) + exp (−k1t) (1.26) k2 − k1 k2 − k1

Let us now consider the case where R is a very reactive species, that is k2 k1, then equation (1.26) reduces to: k1I0 k1 R = exp (−k1t) = I (1.27) k2 k2

This means that R starts at R0 and after a short time of the order of 1/k2 the term exp (−k2t) vanishes and R = k1I/k2 as shown in the ﬁgure. We see two time scales in the process:

• 1/k2: characteristic time of disappearance for R ⇒ fast

• 1/k1: characteristic time of disappearance for I ⇒ slow

Since the dynamics of R is faster than that of I, we can assume that R is at any given time at steady state with respect to I, i.e., R is so fast to reach steady state before I can change signiﬁcantly. This is the PSSA, which means that we can assume dR/dt = 0 in equation (1.18), and compute the PSSA value of R: k Rss = 1 I (1.28) k2 which is the same value given by equation (1.27).

16 CHAPTER 1. FREE-RADICAL POLYMERIZATION

o kI1

k2 kI R=ss 1 k2

Ro

t 1/k2 1/k1

Note

In the PSSA we do not mean that dR/dt = 0, and in fact in the case above we see that:

ss 2 2 dR k1I0 k1 = − exp (−k1t) = − I (1.29) dt k2 k2 Actually we simply mean that

dRss dRss k I and k Rss (1.30) dt 1 dt 2 as it is readily seen by comparison noting that k1/k2 1.

Another Point of View

Let us rewrite equation (1.18) as follows: ! dR k1 ss = k2 I − R = k2 (R − R) (1.31) dt k2

We can observe that: if R > Rss ⇒ dR/dt < 0 ⇒ R decreases if R < Rss ⇒ dR/dt > 0 ⇒ R increases which means that R remains always “around” Rss. Note that this is not true in general, but only ss in the case where k2 is very large we have that the “force” attracting R to R increases up to the point where R cannot diﬀer signiﬁcantly from Rss.

17 CHAPTER 1. FREE-RADICAL POLYMERIZATION

Conclusion

The PSSA can be applied when we have very diﬀerent characteristic times, typically when the intermediate species is very reactive, i.e., k2 k1. The obtained solution is valid for most of the process time, with the exception of a short initial transient. We have two characteristic times:

• the fast one (1/k2) which belongs to R and where I does not change signiﬁcantly

• the slow one (1/k1) which belongs to I and determines the process time, that is the time needed by the slowest species to complete its dynamics.

With respect to numerical integration this has important implications:

• the integration time is given by the process time, i.e., τp ≈ 1/k1

• the integration step is proportional to the characteristic time of the fastest dynamics that

we want to follow, i.e., ∆τ ≈ 1/k2

• the number of integration steps is proportional to τp/∆τ ≈ k2/k1 which means that the

larger is k2/k1 the more we are entitled to use PSSA ... and the more integration steps we have to compute if we fail to use it.

1.5.1 Stiffness Ratio

In general, for a system of ODEs the ratio between the largest and the smallest eigenvalue is referred to as the stiﬀness ratio of the system. This gives a measure of the diﬃculty in integrating a system of ODEs numerically. The coeﬃcient matrix of the system of ODEs, deﬁned as: dx = A x (1.32) dt in our case is given by:

−k1 0 I A = with x = (1.33) k1 −k2 R The eigenvalues of A are given by:

(−k1 − λ)(−k2 − λ) = 0

⇒ λ1 = −k1 , λ2 = −k2

18 CHAPTER 1. FREE-RADICAL POLYMERIZATION and the stiﬀness ratio is then given by: λ k 2 = 2 (1.34) λ1 k1 which, as discussed above, is proportional to the integration steps to be used in the numerical integration of the system of ODEs.

19 Chapter 2 Chain Length Distribution of Polymers

2.1 Population Balance Equations

In the following we concentrate on linear chains only which means kfp = 0 and no propagation of the terminal double bond.

2.1.1 Active Chains

• Under the assumption of pseudo steady state for species R1, dR• 1 = 0 (2.1) dt we can set equation (1.3) equal to zero:

• • • • • RI + (kfm M + kfsS ) R − R1 = kp MR1 + (ktc + ktd) R R1 (2.2)

• Solving for R1 we obtain: • • RI + (kfm M + kfsS ) R R1 = • (2.3) kp M + (ktc + ktd) R + (kfm M + kfsS )

Since RI is given by equation (1.10):

•2 RI = (ktc + ktd) R (2.4) we can simplify equation (2.3) as follows: α R• = R• (2.5) 1 1 + α where α is the summation of various characteristic time ratios: k R• k R• k M k S α = tc + td + fm + fs kp M kp M kp M kp M τp τp τp τp = + + + (2.6) τtc τtd τfm τfs

20 CHAPTER 2. CHAIN LENGTH DISTRIBUTION OF POLYMERS

where τp is the characteristic time of the addition reaction of a single monomer unit, while the τ at the denominator are the characteristic times of the chain transfer and the termination reac- tions involved in the system. The order of magnitude of these characteristic times, which refer to second-order processes, can be computed using pseudo-ﬁrst order reaction approximation. • So far the monomer addition reaction, r = kp MRn and the pseudo-ﬁrst order rate constant is 1 −3 kp M, so that τp = . In most applications, we have that τp ≈ 10 s while termination kpM 0 reactions (or at least the dominating one) has τf or τt ≈ 10 s. This means that a polymer chain leaves about 1 s and in this time it adds about 103 monomer units. Note that the characteristic 1 3 time of the process is that of monomer consumption, τM = • which is of the order of 10 kpR s. These are the three time scales dominating the process under examination. From equation • • (2.5) we can see that for α 1 ⇒ R1 R , as expected. • If we apply the pseudo steady state assumption now to the species Rn (n ≥ 2), we can write:

dR• n = 0 (2.7) dt

• h •i • kp MRn−1 = kp M + kfm M + kfsS + (ktc + ktd) R Rn (2.8)

• • ⇒ Rn = Rn−1Φ (2.9) where 1 Φ = (2.10) 1 + α Therefore we obtain:

• • • 2 • n−1 Rn = Rn−1Φ = Rn−2Φ = ... = R1Φ (2.11) and using equation (2.5):

1 α α R• = R• = R• (2.12) n (1 + α)n−1 1 + α (1 + α)n

Thus, we can consolidate the two cases (n = 1 and n ≥ 2) and write the general expression for n ≥ 1: α R• = R• (2.13) n (1 + α)n

21 CHAPTER 2. CHAIN LENGTH DISTRIBUTION OF POLYMERS

Note

• equation (2.13) can be simpliﬁed if α 1:

1 ≈ exp (−αn) for α 1 (2.14) (1 + α)n

R• ⇒ n ≈ α exp (−αn) (2.15) R•

Rn R

a increases

n

Z ∞ R• Z ∞ exp (−αn) ∞ • n − − • dn = α exp ( αn) dn = α = 1 0 R 0 α 0

To summarize, we can state that the distribution of active chains is normalized and, moreover, it is characterized by only one kinetic parameter α deﬁned by equation (2.6).

2.1.2 Dead Chains

dP 1 Xn−1 n = (k M + k S + k R•) R• + k R•R• (2.16) dt fm fs td n 2 tc j n− j j=1 Here we can write: 1 R•R• + R•R• = R•R• (n = 3) Xn−1 2 1 2 2 1 1 2 1 • • 1 • • •2 • • • • 1 •2 ktc R R = R R + R + R R = R R + R (n = 4) (2.17) 2 j n− j 2 1 3 2 3 1 1 3 2 2 j=1 1 • • • • • • • • • • • • 2 R1R4 + R2R3 + R3R2 + R4R1 = R1R4 + R2R3 (n = 5)

22 CHAPTER 2. CHAIN LENGTH DISTRIBUTION OF POLYMERS

• If we use equation (2.13) to express Rn, we obtain for the sum term: n−1 n−1 " ! !# X • • X • α • α ktc R j Rn− j = ktc R j R n− j j=1 j=1 (1 + α) (1 + α) R•2α2 Xn−1 = k (1) tc (1 + α)n j=1 α2 (n − 1) = k R•2 (2.18) tc (1 + α)n Therefore we can rewrite equation (2.16) as follows: dP α 1 α2 (n − 1) n = (k M + k S + k R•) R• + k R•2 (2.19) dt fm fs td (1 + α)n 2 tc (1 + α)n where we see that α alone is not anymore suﬃcient to fully describe the distribution, and we have to introduce further parameters:

" • ! • ! 2 # dPn • kfm kfsS ktdR α ktcR 1 α (n − 1) = kp MR + + n + n (2.20) dt kp kp M kp M (1 + α) kp M 2 (1 + α) The introduced parameters are deﬁned as follows: • k k S k R τp τp τp γ = fm + fs + td = + + (2.21) kp kp M kp M τ f m τ f s τtd

• k R τp β = tc = (2.22) kp M τtc where α = β + γ (2.23) Finally, we obtain for n ≥ 1: " # dP α 1 n = R γ + (n − 1) αβ (2.24) dt p (1 + α)n 2 Comparing equations (2.13) and (2.24) it is easy to see that in the case of active chain distribu- tion only the ratio between the characteristic times of propagation and termination is relevant. On the other hand, dealing with the dead chain distribution we have to distinguish between two diﬀerent types of chain reactions: chain transfers and disproportionation on one side, and combination on the other side. The question is: what is the conceptual diﬀerence between these reactions which makes them to play a diﬀerent role in determining the chain length distribution?

23 CHAPTER 2. CHAIN LENGTH DISTRIBUTION OF POLYMERS

2.2 Instantaneous Chain Length Distribution

In the following section we consider the instantaneous CLD of polymer chains. Diﬀerent distributions can be introduced.

2.2.1 Number Distribution and Number Average

The instantaneous CLD or number distribution is deﬁned as follows:

dPn polymer chains of length n dt fN(n) = = ∞ (2.25) total number of polymer chains X dPn dt n=1 Note that this is an instantaneous property, that is it represents the CLD of the inﬁnitesimal amount of polymer produced at a given time. Using equation (2.24) we obtain:

1 − γ + 2 (n 1) β (β + γ) (1 + α)n f n N( ) = ∞ 1 (2.26) X γ + (n − 1) β (β + γ) 2 (1 + α)n n=1 Since the following equality holds for geometric series

X∞ aq bq (a + nb) qn = + for |q| < 1 (2.27) (1 − q) 2 n=1 (1 − q) we can rewrite the denominator in equation (2.26) as follows:

∞ " # !n ∞ " # !n X 1 1 X 1 1 γ − β (β + γ) + n β (β + γ) 2 1 + α 2 1 + α n=1 n=1 " # ! ! 1 1 1 1 + α = γ − β (β + γ) + β (β + γ) (2.28) 2 α 2 α2 and since α = β + γ ! ! ! 1 1 1 1 + α 1 1 = γ − β + β = γ + β (2.29) α 2 2 α α 2 Finally, we obtain for equation (2.26):

γ + 1 (n − 1) β (β + γ) α 2 fN(n) = (2.30) (1 + α)n 1 γ + 2 β

24 CHAPTER 2. CHAIN LENGTH DISTRIBUTION OF POLYMERS

By deﬁnition holds: X∞ fN(n) = 1 (2.31) n=1 Let us focus now on the moments of this distribution. In particular, the j-th order moment of fN(n) is deﬁned as follows: ∞ X j µ j = n fN(n) (2.32) n=1 From the ﬁrst two moments we can calculate the number average of the CLD: µ 1 n = 1 ≈ for α 1 (2.33) N µ 1 0 γ + 2 β which, when multiplied by the molecular weight of the monomer, MM, leads to the so-called number average molecular weight:

µ1 MN = MM (2.34) µ0

2.2.2 Weight Distribution and Weight Average

Another way to characterize the distribution of the polymer chains is the so-called instanta- neous weight distribution:

n · dPn number of monomer units in the chains of length n dt fW(n) = = (2.35) total amount of consumed monomer Rp or expressed in terms of fN:

n fN(n) n fN(n) fW(n) = P∞ = (2.36) 1 n fN(n) µ1

If we compute the mean of this distribution we obtain the weight average of the CLD:

1 X∞ µ n = n2 f (n) = 2 (2.37) W µ N µ 1 1 1

Note that the moments used in the last two expressions refer to fN. Using equations (2.30) and (2.36) we obtain: 3 2 γ + 2 β nW ≈ for α 1 (2.38) (γ + β)2

25 CHAPTER 2. CHAIN LENGTH DISTRIBUTION OF POLYMERS

n n N W

) f W n

( f

W N f ) , n ( N f

n

which, when multiplied by the molecular weight of the monomer, MM, leads to the so-called weight average molecular weight: µ2 MW = MM (2.39) µ1

To summarize, we deﬁned two diﬀerent means nN and nW of only one distribution fN. The reason for this is given in the following subsection.

2.2.3 Polydispersity

The polydispersity index (PDI) is a widely used quantity to characterize distributions in gen- eral and the CLD in particular. This is deﬁned as follows: n σ = W ≥ 1 (2.40) nN

µ /µ µ µ ⇒ 2 1 2 0 σ = = 2 (2.41) µ1/µ0 µ1 Thus, σ = 1 means that all chains have exactly the same length. The polydispersity index describes the width of a distribution and is therefore an alternative way to represent its variance v: ∞ X 2 2 v = (n − nN) fN(n) = µ2 − 2µ1nN + nNµ0 n=1 µ2 µ2 µ2 − 1 1 − 1 = µ2 2 + 2 µ0 = µ2 µ0 µ0 µ0 µ2 = 1 (σ − 1) (2.42) µ0

26 CHAPTER 2. CHAIN LENGTH DISTRIBUTION OF POLYMERS

Note that v = 0 corresponds to σ = 1. The usage of the polydispersity to characterize the width of CLD of polymers is justiﬁed by the fact that equation (2.40) is particularly convenient in practice. We have in fact various techniques available that can measure either the number average or the weight average of polymer chains.

2.2.4 Summary

For the reaction scheme of the free-radical polymerization system described in section 1.4.1 we can write the following relationships for the instantaneous properties of the CLD (if α 1): 1 nN = β (2.43) γ + 2

3 2 γ + 2 β nW = (2.44) (γ + β)2 2 γ + 3 β γ + 1 β σ = 2 2 (2.45) (γ + β)2

27 Chapter 3 Cumulative Properties of Polymers

3.1 Cumulative Chain Length Distribution, Moments, and Properties

c In order to compute the cumulative number-CLD, fN(n) from the instantaneous one, fN(n) we use the following relation:

number of polymer chains of length n produced per unit time z }| { Z t ! c 1 dP fN(n, t) = fN(n, t) dt (3.1) P(t) 0 dt | {z } total number of polymer chains of length n produced until time t which multiplying both sides by n j and summing for n = 1 to ∞ gives the following expression for the moments of the cumulative distribution: ∞ ∞ ! X 1 Z t X dP n j · f c(n, t) = n j · f (n, t) dt (3.2) N P(t) N dt n=1 0 n=1 which leads to: Z t ! Z P(t) c 1 dP 1 µ j = µ j dt = µ j dP (3.3) P(t) 0 dt P(t) 0 Note that since P represents the total number of dead polymer chains per unit volume, from equation (2.24) we have:

X∞ X∞ γ + 1 (n − 1) αβ dP dPn 2 = = αRp (3.4) dt dt (1 + α)n n=1 n=1

28 CHAPTER 3. CUMULATIVE PROPERTIES OF POLYMERS which using equation (2.29) reduces to: dP 1 β β = αR γ + = R γ + (3.5) dt p α 2 p 2 The total number of chains per unit volume produced at time t, is then given by: Z t β P(t) = Rp γ + dt (3.6) 0 2

Examples

Let us calculate now a few moments:

c • µ0 Z P(t) c 1 P(t) µ0 = µ0 dP = = 1 (3.7) P(t) 0 P(t) c c • µ1 and µ2 Z P(t) c 1 µ1 = µ1 dP (3.8) P(t) 0

Z P(t) c 1 µ2 = µ2 dP (3.9) P(t) 0 In both cases we get the weighted average of the instantaneous properties.

c • cumulative number average of the MWD, nN

c Z P(t) Z P(t) Z P(t) c µ1 1 1 µ1 1 nN = c = µ1 dP = dP = nN dP (3.10) µ0 P(t) 0 P(t) 0 µ0 P(t) 0 Again we obtain the weighted average of the instantaneous property.

c • cumulative weight average of the MWD, nW

R P(t) c Z P(t) Z P(t) µ µ2 dP 1 µ 1 nc 2 0 2 P n P W = c = R P(t) , d = W d (3.11) µ1 µ dP P(t) 0 µ1 P(t) 0 0 1

• polydispersity index, σc

R P(t) c c µ dP Z P(t) c µ2µ0 0 2 1 σ = 2 = 2 , σ dP (3.12) c R P(t) P(t) µ 1 µ dP 0 1 P(t) 0 1

29 CHAPTER 3. CUMULATIVE PROPERTIES OF POLYMERS

c c Note that nW and σ are not anymore the weighted averages of the corresponding instantaneous quantities. To obtain them, the integrals in equations (3.11) and (3.12) have to be solved. In conclusion, when computing the averages of a cumulative CLD it is convenient to inte- grate the following ODE to get the cumulative moments

c d µ jP dP = µ (3.13) dt j dt and from this compute the desired averages.

3.1.1 Width of the Cumulative Distribution

The width of the cumulative CLD can be regarded as determined by two factors:

• the width of the instantaneous CLD which is given by the kinetics of the process

• the shifting of the instantaneous average chain length with time.

cumulated at time t3 (not normalized)

n·f(n)

inst. at time t2

inst. at time t3 inst. at time t1

log(n)

If the instantaneous CLD is constant in time, so as its average n, then the cumulative CLD su- perimposes the instant one and the two have the same polydispersity. However, if the instanta- neous n changes in time the cumulative polydispersity is certainly larger than the instantaneous one, that is: σc ≥ σ (3.14)

30 CHAPTER 3. CUMULATIVE PROPERTIES OF POLYMERS

3.2 Designing Polymerization Processes with Respect to Desired CLDs

3.2.1 Case I: Termination by Combination is Negligible

If termination by combination is negligible with respect to at least one of the other chain termination reactions we have β γ, and then from equations (2.43) to (2.45): 1 n = (3.15) N γ

2 n = (3.16) W γ

σ = 2 (3.17)

For fN(n) we obtain: γ f (n) = ≈ γ exp (−γn) (3.18) N (1 + γ)n This result corresponds to the so-called most probable or Flory distribution. The expression for fW(n) is then: 2 n fN(n) nγ 2 fW(n) = = n ≈ nγ exp (−γn) (3.19) µ1 (1 + γ) Thus, in order to control the CLD we have to play with the parameter γ.

Chain Transfer to Monomer Dominates

Let us assume that chain transfer to monomer is the dominating chain termination in the entire polymerization system. In this case we have:

τp τp τp τp k γ = + + ≈ = fm (3.20) τfm τfs τtd τfm kp

⇒ γ = f temp. (3.21) For an isothermal batch reactor we obtain therefore:

γ = const. ⇒ nN = const. (3.22) and σc = σ = 2 (3.23)

31 CHAPTER 3. CUMULATIVE PROPERTIES OF POLYMERS

. -4 n 10 W

10 nN

5

t

A typical example for this case is the polymerization of vinyl chloride to PVC. It we want to produce the narrowest possible CLD, the only problem is therefore to control the temperature during the entire process. In addition, we note that:

• in order to increase nN, the temperature has to be reduced ⇒ γ decreases

• in order to decrease nN, the temperature has to be increased ⇒ γ increases.

This follows from the observation that the activation energy is typically larger for chain trans- fer to monomer than for propagation, so that γ = kfm/kp is an increasing function with tem- perature. Note that since the temperature can only be changed to a certain extent, only modest changes in the average chain length can be achieved. In order to achieve a signiﬁcant reduc- tion in the average chain length it is more eﬀective to add a chain transfer agent which results in a new dominating termination step, i.e., τfs τfm. On the other hand a signiﬁcant increase in the average chain length would be diﬃcult to achieve.

Termination by Disproportionation Dominates

In the case where termination by disproportionation is the dominating chain termination reac- tion, γ becomes: √ • τp k R k R γ ≈ = td = td I (3.24) τtd kp M kp M In order to keep γ constant, we have to keep the constant monomer concentration, M, the temperature, T, as well as the rate of radical production, RI. This is obviously diﬃcult in batch systems. Therefore, the value of nN will most likely decrease with M and therefore

σc > σ = 2 (3.25)

32 CHAPTER 3. CUMULATIVE PROPERTIES OF POLYMERS

nW

nN

t

A typical example for this case is the polymerization of methyl methacrylate to PMMA where σc ≈ 5. To obtain a lower value of σc we have two possibilities:

• work in semi-batch reactors where monomer is continuously added in order to keep constant its concentration in the reactor

• use emulsion polymerization.

Industrially, PVC is produced mainly in suspension whereas PMMA is usually produced in emulsion.

3.2.2 Case II: Termination by Combination Dominates

In the case where bimolecular combination is the dominating chain termination reaction we have β γ and therefore from equations (2.43)-(2.45) we have:

2 n = (3.26) N β

3 n = (3.27) W β

σ = 1.5 (3.28)

Note that termination by combination potentially leads to the narrowest CLD. √ • τp k R k R β = = tc = tc I (3.29) τtc kp M kp M

33 CHAPTER 3. CUMULATIVE PROPERTIES OF POLYMERS

nW

nN

t

Thus, we can draw the same conclusion as in the previous case (section 3.2.1). As a typical example the low-temperature polymerization of styrene can be mentioned (T = 50◦C).

In a batch system we would again expect a decreasing nN with conversion. However, experi- mentally the opposite is observed. This is due to the fact that, although M decreases, because of the gel eﬀect ktc decreases even more, resulting in a decreasing value of β.

34 Chapter 4 Copolymerization

4.1 Kinetics of Copolymerization

4.1.1 Involved Chemical Reactions

• Initiation I2 + M −→ 2 R1 r = 2 f kdI2 ≡ RI k • pAA • • Propagation Am,n + A −→ Am+1,n r = kpAAAAm,n k • pAB • • Am,n + B −→ Bm,n+1 r = kpABBAm,n k • pBA • • Bm,n + A −→ Am+1,n r = kpBAABm,n k • pBB • • Bm,n + B −→ Bm,n+1 r = kpBBBBm,n • kfsA • • Chain Transfer Am,n + S −→ R1 + Pm,n r = kfsASAm,n • kfsB • • Bm,n + S −→ R1 + Pm,n r = kfsBSBm,n • • ktAA • • Termination Am,n + Ar,q −→ Pm+r,n+q or Pm,n + Pr,q r = ktAAAm,nAr,q • • ktAB • • Am,n + Br,q −→ Pm+r,n+q or Pm,n + Pr,q r = ktABAm,nBr,q • • ktBB • • Bm,n + Br,q −→ Pm+r,n+q or Pm,n + Pr,q r = ktBBBm,nBr,q

where n, m, r, q = [1...∞] and kt = ktc + ktd

Note that a similar notation as for homopolymerization has been used above with, for example, • Am,n indicating the concentration of active chains containing m units of monomer A and n units of monomer B, and terminating with a monomer A unit. The latter unit, where the radical is located, deﬁnes the reactivity of the active chains, and accordingly determines the rate constant of all the reactions above. This is usually referred to as the terminal kinetic model. So for example, kpAB represents the rate constant for the propagation of radical chain of type A and any length with a monomer B.

35 CHAPTER 4. COPOLYMERIZATION

4.1.2 Long-Chain Approximation

The long-chain approximation (LCA) starts from the observation that the following equality holds along a polymer chain:

(number of transitions A → B) = (number of transitions B → A) ± 1 (4.1)

These geometrical considerations lead to the following condition on reaction rates:

• • kpABA B = kpBAB A (4.2)

Let us deﬁne R• = A• + B• (4.3) where A• represents the total concentration of radicals of type A, that is radicals terminating with a monomer of type A: ∞ ∞ • X X • A = Am,n (4.4) m=1 n=1 Therefore we obtain: • • • kpABA B = kpBA (R − A ) A (4.5)

• kpBAA • • ⇒ A = R = pAR (4.6) kpABB + kpBAA

• kpABB • • ⇒ B = R = pBR (4.7) kpABB + kpBAA where pA is the probability of having a radical of type A. Now, let us write the mass balance for A• and B•: dA• = R + k B•A − k A•B − k A•2 − k A•B• (4.8) dt IA pBA pAB tAA tAB

dB• = R + k A•B − k B•A − k B•2 − k A•B• (4.9) dt IB pAB pBA tBB tAB The rates of initiation for the monomers A and B are deﬁned as the product of the overall rate of initiation and the respective monomer mole fractions in the monomer phase, i.e., RIA =

RIXA and RIA = RIXB, where A B X = and X = (4.10) A A + B B A + B

36 CHAPTER 4. COPOLYMERIZATION

The summation of equation (4.8) and (4.9) gives:

dR• dA• dB• = + = R + R − k A•2 − k B•2 − 2k A•B• (4.11) dt dt dt IA IB tAA tBB tAB

• Applying the pseudo steady state assumption to R and using RI = RIA + RIB we obtain:

2 •2 2 •2 •2 RI − ktAA pAR − ktBB pBR − 2ktAB pA pBR = 0 (4.12) and therefore s • RI R = ∗ (4.13) kt

∗ where kt is deﬁned as follows:

∗ 2 2 kt = ktAA pA + 2ktAB pA pB + ktBB pB (4.14)

To conclude, we obtain the same result as in the case of homopolymerization with a pseudo- ∗ termination rate constant, kt deﬁned by equation (4.14) replacing the actual termination rate constant, kt.

4.1.3 Rate of Monomer Consumption

Since propagation reactions dominate monomer consumption, we have:

• • • RpA = kpAAA A + kpBAB A = kpAA pA + kpBA pB AR (4.15)

• • • RpB = kpBBB B + kpBAA B = kpBB pB + kpAB pA BR (4.16)

( ∗ • ∗ RpA = kpAAR • ⇒ ∗ • ⇒ Rp,tot = RpA + RpB = kp M R (4.17) RpB = kpBBR

∗ • ⇒ Rp,tot = RpA + RpB = kp M R (4.18)

∗ ∗ Introducing the pseudo-propagation rate constants kpA and kpB we obtain again a similar ex- pression as in the case of homopolymerization.

37 CHAPTER 4. COPOLYMERIZATION

4.2 Chain Length Distribution of Copolymers

4.2.1 Population Balance Equation

In this section we calculate the CLD in the case of a copolymerization process. Let us therefore consider the population balance of chain radicals terminating with a monomer unit A and containing r units of any type (A or B): dA• r = k · A · A• + k · A · B• dt pAA r−1 pBA r−1 • − kpAA · A + kpAB · B Ar • • • • −kfsA · S · Ar − (ktAA · A + ktAB · B ) Ar (4.19) and similarly for the radicals terminating with a B unit: dB• r = k · B · B• + k · B · A• dt pBB r−1 pAB r−1 • − kpBB · B + kpBA · A Br • • • • −kfsB · S · Br − (ktBB · B + ktBA · A ) Br (4.20)

• • • Applying the long-chain approximation and using Rr = Ar + Br we obtain: dR• h i r = k · p + k · p · A + k · p + k · p · B · R• dt pAA A pBA B pBB B pAB A r−1 h i • − kpAA · pA + kpBA · pB · A + kpBB · pB + kpAB · pA · B · Rr • − (kfsA · pA + kfsB · pB) · S · Rr 2 2 • • − ktAA · pA + 2ktAB · pA · pB + ktBB · pB · Rr · R (4.21)

A further simpliﬁcation can be achieved when using the pseudo-homopolymerization rate constants: • dR ∗ ∗ r = k M R• − k M R• − k∗ SR• − k∗R•R• (4.22) dt p r−1 p r fs r t r This expression is identical to the population balance equation (PBE) for a homopolymer containing r monomer units. We can extrapolate this result to all PBEs involved in computing the CLD for copolymers. This method is the so-called pseudo-homogeneous approach, it will be discussed in the next section.

4.2.2 Pseudo-Homogeneous Approach

From the results above we can conclude as follows:

38 CHAPTER 4. COPOLYMERIZATION

When using the long chain approximation, the PBE for the CLD of a copolymeriza- tion process can be reduced to the corresponding ones of a homopolymerization pro- cess, where the actual polymerization rate constants are replaced by suitable averages (pseudo-kinetic parameters) of the actual copolymerization rate constants.

These averages are diﬀerent depending upon the reaction order with respect to the radical species:

• zero-order processes

RI = RIA + RIB (4.23)

• ﬁrst-order processes

∗ kp M = kpAA pA + kpBA pB · A + kpBB pB + kpAB pA · B (4.24)

∗ kfs = kfsA pA + kfsB pB (4.25)

• second-order processes

∗ 2 2 kt = ktAA pA + 2ktAB pA pB + ktBB pB (4.26)

This implies that in order to compute the CLD of a copolymer we can use the same equations developed above for a homopolymer, by simply replacing the actual homopolymerization con- stants with the pseudo-homopolymerization ones (function of the actual copolymerization rate constants). This procedure is referred to as the pseudo-homopolymerization approach. Note that all rate constants of the pseudo-homopolymerization are functions of the composition of the monomer phase which in principle changes during the reaction.

4.2.3 Kinetics of Multi-Monomer Polymerization

The current polymer technology requires, for applications of increasing complexity, the pro- duction of chains containing two or more monomer. As the long chain assumption cannot be extended to the case where more than two monomers are involved one has to take a diﬀerent approach. Let us consider the case of three monomer polymerization, and write the molar balances of the radical chains with the same terminal unit and any chain length. Since the cross propaga- tion reactions dominate these balances we consider the following reactions:

39 CHAPTER 4. COPOLYMERIZATION

k • pAB • • A + B −→ B r = kpABA B k • pAC • • A + C −→ C r = kpACA C k • pBA • • B + A −→ A r = kpBAB A k • pBC • • B + C −→ C r = kpBCB C k • pCA • • C + A −→ A r = kpCAC A k • pCB • • C + B −→ B r = kpCBC B The following balances follow: dA• = k B•A + k C•A − k B + k C A• (4.27) dt pBA pCA pAB pAC

dB• = k A•B + k C•B − k A + k C B• (4.28) dt pAB pCB pBA pBC

R• = A• + B• + C• (4.29) Note that the last equation has been introduced to replace the molar balance of C• which would have been a linear combination of the ﬁrst two. We cannot compute the absolute values of A•, B• and C• but only their ratios. Thus, introducing the probabilities (or mole fractions):

• • • • • • pA = A /R , pB = B /R , pC = C /R we get: kpBAApB + kpCAApC − kpABB + kpACC pA = 0 kpABBpA + kpCBBpC − kpBAA + kpBCC pB = 0 (4.30) pA + pB + pC = 1 which is a linear system with three unknowns. Note that in the case of binary copolymeriza- tion, the system above reduces to: ( k Ap − k Bp = 0 pBA B pAB A (4.31) pA + pB = 1 which leads to the same solution

kpBAA pA = (4.32) kpBAA + kpABB obtained earlier using LCA. Which means that LCA is simply a short-cut form of the pseudo steady state approximation in the case of binary copolymers. This procedure can be general- ized to any number of monomer species greater or equal than three.

40 CHAPTER 4. COPOLYMERIZATION

Note that in equation (4.27) and (4.28) we have assumed that the cross propagation reactions are much faster than all terminations. This is generally the case in polymerization systems, with the only exception of block polymerization. The pseudo-homopolymerization rate constants are then computed using the same rules indicated above:

• zero-order average

RI = RIA + RIB + RIC + ... (4.33)

• ﬁrst-order average ∗ kfs = kfsA pA + kfsB pB + kfsC pC + ... (4.34)

∗ kpA = kpAA pA + kpBA pB + kpCA pC + ... (4.35)

∗ kpB = kpAB pA + kpBB pB + kpCB pC + ... (4.36)

... (4.37)

• second-order average

∗ 2 2 2 kt = ktAA pA + ktBB pB + ktCC pC

+2ktAB pA pB + 2ktAC pA pC + 2ktBC pB pC +... (4.38)

4.3 Chain Composition Distribution of Copolymers

4.3.1 Instantaneous Chain Composition

The mole fraction of A in the diﬀerential amounts of polymer produced at a given instant of time is given by: RpA FA = (4.39) RpA + RpB where the rate of polymerization of A and B can be computed using equation (4.17): kpAA pA + kpBA pB · A FA = (4.40) kpAA pA + kpBA pB · A + kpBB pB + kpAB pA · B

41 CHAPTER 4. COPOLYMERIZATION

As seen in equation (4.6) and (4.7) the probability of having a radical of type A or B is given by: kpBAA pA = kpBAA + kpABB

kpABB pB = kpBAA + kpABB If we now introduce the reactivity ratios, which are deﬁned as the ratio between the direct and the cross propagation rate constant for a given radical,

kpAA kpBB rA = and rB = (4.41) kpAB kpBA we can rewrite equation (4.40) as follows:

(rAA + B) · A FA = (rAA + B) · A + (rBB + A) · B (r X + X ) · X = A A B A (4.42) (rAXA + XB) · XA + (rBXB + XA) · XB Equation (4.42) is the so-called Mayo-Lewis equation which contains only two kinetic pa- rameters, rA and rB. In order to understand the eﬀect of the reactivity ratios on the Mayo-Lewis equation we will derive the expression for dFA/dXA. Therefore we rewrite equation (4.42) us- ing the expression XB = 1 − XA

2 (rA − 1)X + XA F = A (4.43) A 2 2 (rA − 2)XA + 2XA + rB(1 − XA) and then diﬀerentiate with respect to XA dFA 2(rA − 1)XA + 1 den − nom 2(rA − 2)XA + 2 − 2rB(1 − XA) = 2 (4.44) dXA den where den and nom are the denominator and nominator of equation (4.43), respectively. Now we will consider the limits of dFA/dXA for XA → 0 and XA → 1:

dFA 1 = (4.45) dXA XA→0 rB

dFA 1 = (4.46) dXA XA→1 rA In the following we want to distinguish three diﬀerent cases:

42 CHAPTER 4. COPOLYMERIZATION

! ! dFA dFA I(rA > 1) ∧ (rB < 1) : > 1 ∧ < 1 dXA XA→0 dXA XA→1 both radicals ”prefer” to propagate with A (A is more reactive)

! ! dFA dFA II (rA < 1) ∧ (rB > 1) : < 1 ∧ > 1 dXA XA→0 dXA XA→1 both radicals ”prefer” to propagate with B (B is more reactive)

! ! dFA dFA III (rA < 1) ∧ (rB < 1) : > 1 ∧ > 1 dXA XA→0 dXA XA→1 both radicals ”prefer” to propagate with the other monomer

The Mayo-Lewis plot represents the instantaneous composition of a polymer, FA produced from a given monomer phase composition, XA and it can be represented by the following plot.

1

I

III FA

II

0 XA 1

4.3.2 Composition Drift

Let us analyze the behavior of the chain composition distribution in a batch reactor using the Mayo-Lewis diagram. Suppose that we charge initially in the reactor a monomer mixture 0 where the molar fraction of A is XA. As soon as the reaction starts we produce polymer 0 chains with mole fraction of A equal to FA. However, since FA > XA the monomer phase

43 CHAPTER 4. COPOLYMERIZATION

0 becomes poorer of A, and XA decreases below the initial value XA. With the progress of the polymerization the XA value decreases further, leading to the production of polymer chains continuously poorer in A, as indicated by the arrow in the plot.

1

FA

o X A

o 0 X A 1

Note that the composition drift produces substantial variations in the chain compositions. This can be appreciated by noting that complete monomer conversion, the average composition of all chains has to be equal to the initial monomer composition.

4.3.3 Chain Composition Control

In order to avoid the composition drift we have to use a semibatch reactor, where we introduce a ﬂow rate N˙ of the two monomers in order to keep constant the monomer phase mole fraction,

XA and consequently also the composition of the produced polymer chains.

NA NB

For this we consider the mass balances in a semibatch reactor where N˙ A and N˙ B are the molar

44 CHAPTER 4. COPOLYMERIZATION

ﬂow rates of the two monomers: dN A = N˙ − R V (4.47) dt A pA

dN B = N˙ − R V (4.48) dt B pB where Ni represents the moles of the i-th monomer in the reactor, V is the volume of the ∗ • reactor content, and RpA and RpB the monomer polymerization rate given by RpA = kpAAR ∗ • and RpB = kpBBR , respectively, so that: dN A = N˙ − k∗ R•N (4.49) dt A pA A

dN B = N˙ − k∗ R•N (4.50) dt B pB B where NA = AV and NB = BV. Let us now introduce the dimensionless time τ = t/tf, where tf is the duration of the process. So that we get: dN A = t N˙ − k∗ R•N (4.51) dτ f A pA A

dN B = t N˙ − k∗ R•N (4.52) dτ f B pB B 0 0 with the initial conditions NA(0) = NA and NB(0) = NB. Assuming that the pseudo kinetic propagation rate constants do not change during the process we can integrate the equations above to obtain: N˙ N˙ N = N0 − A exp −k∗ R•t τ + A (4.53) A A ∗ • pA f ∗ • kpAR kpAR N˙ N˙ N = N0 − B exp −k∗ R•t τ + B (4.54) B B ∗ • pB f ∗ • kpBR kpBR The question is now how to operate the reactor in order to keep the monomer phase composi- tion constant, i.e., NA/NB = const. There are two possible operation modes.

Starved Operation

This operation modus, which is frequent in reaction engineering, is based on the observation that the reactor under consideration is a self-regulated system, in the sense that it admits only

45 CHAPTER 4. COPOLYMERIZATION one stable pseudo-steady state. Accordingly, as τ → ∞ the system autonomously approaches such a steady state, deﬁned as follows:

˙ ∗ • pss NA = kpAR NA = RpAV (4.55)

˙ ∗ • pss NB = kpBR NB = RpBV (4.56) This means that the system adjusts itself in order to satisfy the above pseudo-steady state condition, which means that the monomer amounts inside the reactor change from the initial 0 0 pss pss values NA and NB, to the values NA and NB deﬁned by the equations above which are such that the rate of of consumption of each monomer by the polymerization process is equal to the rate of monomer feed to the reactor which we can of course control. Accordingly, in order to produce a copolymer with composition FA, in these conditions, we simply need to take N˙ A/(N˙ A + N˙ B) = FA constant in time so as to have RpA/ RpA + RpB = FA and than produce a copolymer with instantaneous composition equal to the desired value. Note that the values pss pss pss pss pss pss NA and NB are such that the monomer mole fraction XA = NA / NA + NB is equal to the value that according to the Mayo-Lewis plot leads to the desired copolymer composition, FA. This is done autonomously by the system, we do not need to know this plot for the particular copolymer under examination. The problem is that this condition is satisﬁed only at the pseudo-steady state, i.e., at τ → ∞, while during the transient period the copolymer composition is not equal to the desired value. However, by looking at the exponential functions in equations (4.53) and (4.54), we see that the pseudo-steady state condition is achieved at the time

1 1 τ = ∗ • and ∗ • (4.57) kpAR tf kpBR tf for the two monomers. Thus, if we take a very long process time, i.e.,

1 1 tf ∗ • or ∗ • (4.58) kpAR kpBR we have that the pseudo-steady state conditions are achieved after a very short fraction of the process time, i.e., τ 1, so that the amount of polymer produced in the transient condition is small, and we can actually make it negligible by increasing tf at will. The starved equation made is then based on the second condition, that is the feed time should be suﬃciently long,

46 CHAPTER 4. COPOLYMERIZATION in particular such as to satisfy the condition above. A more intuitive explanation of the mech- anism of this operation mode can be obtained by looking directly at the mass balances (4.51) and (4.52). By considering the ﬁrst one in the form dN h i A = t k∗ R• Npss − N (4.59) dτ f pA A A pss ˙ ∗ • we see that if we have NA < NA = NA/ kpAR then dNA/dτ > 0 and NA increases, while if pss NA > NA then dNA/dτ < 0 and NA decreases. This means that NA is always attracted towards pss the pseudo-steady state value NA (auto regulated system) with a ”speed” which is higher the ∗ • larger is the value of tfkpAR . A similar argument holds true for B. Q

M

qout

A simple example of an auto regulated system, which admits only one stable steady state is that of a tank with a hole, where feed the volumetric ﬂow rate, Q of water. The mass balance leads to: dM A = Q − q (4.60) dt out where M is the level of the liquid, A the cross section and the outlet ﬂow rate is given by p Bernoulli equation as qout = Ah 2gM, where Ah is the cross section of the hole. The mass balance above can be rewritten as follows: dM Q A p = − h 2gM (4.61) dt A A Introducing the steady state value √ Q Mss = p (4.62) Ah 2g this reduces to: p dM Ah 2g √ √ = Mss − M (4.63) dt A

47 CHAPTER 4. COPOLYMERIZATION which indicates that whatever is the initial level in the tank, this changes in order to reach the steady state value, which is the one that makes qout = Q. This is in perfect analogy with the starved reactor, which is however a semibatch and not a continuous system, and therefore does not admit a real steady state. ∗ • ∗ • Note that by taking the feed time tf 1/ kpAR or 1/ kpBR we are imposing to the system a dynamics much slower than its intrinsic one, which is the dynamics of monomer ∗ • ∗ • consumption (whose characteristic times are 1/ kpAR and 1/ kpBR for the two monomers). Accordingly, we do not allow the monomer accumulation in the reactor, and this is the reason why this operation modus is referred to as starved. The time evolutions of conversion (solid line) and amount of monomer introduced in the reactor (dashed line) are shown in the ﬁgures below.

Batch Semibatch

100% 100%

time time

In other words we are forcing the reactor to produce much less than its potential in order to have a narrow chain composition distribution.

Power Feed Operation

In this operation modus we try to realize two objectives simultaneously:

• narrow chain composition distribution

• maximum productivity of the reactor

We can consider that we have two scalar and two reactor optimization variables, that is the 0 0 amounts of the two monomers initially introduced in the reactor, NA and NB, and the two ﬂow rates as a function of time, i.e., N˙ A(t) and N˙ B(t) for t > 0. We need to deﬁne them in order to satisfy the two objectives above. For the ﬁrst objective function, i.e., chain composition equal to FA, we can ﬁrst impose to have initially in the reactor the monomer phase composition,

48 CHAPTER 4. COPOLYMERIZATION

XA which leads to the desired polymer composition, FA. For this we need ﬁrst to know the

Mayo-Lewis relation to compute XA and then we impose:

0 NA 0 0 = XA (4.64) NA + NB

Next we operate on the ﬂow rates N˙ A and N˙ B in order to keep the monomer phase composition constant during the entire process, that is: d (N /N ) A B = 0 , for t > 0 (4.65) dt or: dN dN N A = N B , for t > 0 (4.66) B dt A dt which from the mass balances (4.49) and (4.50) leads to: ˙ ∗ • ˙ ∗ • NB NA − kpAR NA = NA NB − kpBR NB , for t > 0 (4.67)

This constraint allows keeping constant the composition of the produced polymer. A third constraint is on the total weight of the polymer produced in one batch, WP which is imposed by the volume of the reactor: Z ! Z ! 0 ˙ m 0 ˙ m NA + NAdt MA + NB + NBdt MB = WP (4.68)

We can now use the last degree of freedom to reach the second objective, that is maximum polymerization rate at any time during the process. This is a complex problem of demanding calculations whose simple solution is that the less reactive monomer (B in our case) should all be introduced at the beginning of the process, that is

N˙ B = 0 , for t > 0 (4.69) which introduced in equation (4.67)leads to: ˙ ∗ ∗ • NA = kpA − kpB R NA , for t > 0 (4.70) which indicates that we have to add to the reactor the amount of A needed to equilibrate the change in composition induced by its higher reactivity with respect to B.

Thus, summarizing, if we need to produce a total amount of polymer WP with uniform chain w composition FA, we proceed as follows. Using the corresponding weight fractions FA and

49 CHAPTER 4. COPOLYMERIZATION

w FB, we compute the total amounts (weights) of the two monomers needed WA and WB. From

Mayo-Lewis relation we compute the monomer phase mole fraction XA which corresponds to

FA. From this we compute the total moles of the two monomers to be initially introduced in the reactor: 0 WB NB = m (4.71) MB

0 NA 0 0 = XA (4.72) NA + NB m 0 The remaining amount of A, given by WA/MA − NA, is fed during the process according to the

N˙ A value given by equation (4.70). This operation modus is economically more convenient than the starved operation but it requires to know the kinetics of the process (cf. Mayo-Lewis) and to be able to implement the condition (4.65) which requires either to measure on-line or to model the kinetic of the process. An additional problem which often arises with this procedure is that the very high productivity leads to a very large heat production which may be diﬃcult to handle with a given heat exchange area. If the reactor cooling capacity is insuﬃcient and ﬁxed, one should reconsider the above optimization process and substitute the maximum productivity objective with the condition that the heat production rate should never exceed the potential heat cooling of the reactor, so as to be able to maintain isothermal operating conditions. This would be of the following form:

RpA (−∆HA) + RpB (−∆HB) ≤ US (T − Tc) (4.73) where ∆Hi is the polymerization enthalpy of the i-th monomer, U and S are the reactor heat transfer coeﬃcient and surface, respectively and Tc is the temperature of the cooling medium.

4.3.4 Reactor Monitoring and Control

The composition control problem can be solved with a closed-loop controller, provided that we have a reliable on-line sensor for the monomer phase composition. The measured composition could be compared to the set-point XA and then a proper action taken on the manipulated variables N˙ A and N˙ B. Such a sensor could be a gas chromatograph for the liquid phase or for the phase in the head space. The second is probably faster and more robust, but deﬁnitely not suﬃciently for its routine use in a production environment. More easy is to measure on-line the global rate of polymerization in the reactor. For this we can use the reactor heat balance

50 CHAPTER 4. COPOLYMERIZATION

as follows: ˙ out in (−∆H) RpV = Nccpc Tc − Tc (4.74) where N˙ c and cpc are the ﬂow rate and the heat capacity of the cooling medium, and ∆H is the global reaction enthalpy. From this equation, by measuring on-line the outlet and inlet temperatures of the cooling medium, we can compute the instantaneous global rate of poly- merization. Clearly, we have no way to distinguish the individual contribution of the two monomers from this energy balance. The above equation is approximate and in applications we should account for heat losses and for the heat accumulations. In addition, it is generally out in diﬃcult to use a reactor as a calorimeter. On one hand in fact we need Tc and Tc to be very close so as to have a uniform cooling of the reactor. On the other hand, we need to have an out in appreciable diﬀerence of Tc and Tc in order to avoid an excessive propagation of the tem- perature measurement error in the estimated value of the global rate of polymerization. Other equivalent sensors are used in applications which estimate the rate of reaction from density measurements which are obtained by measuring the ultrasound propagation velocity in the re- acting system. The complementary information needed to compute the rate of polymerization of the two individual monomers can be obtained using a kinetic model. The rate of monomer consumption is in fact given by:

dN A = −R = −k∗ R•AV (4.75) dt pA pA In practice, the diﬃculty in using this equation is the evaluation of R• which is the source of many irreproducibilities, due to unpredictable impurities, inhibitors or others. On the other hand, the polymer composition

∗ RpA kpAA FA = = ∗ ∗ (4.76) RpA + RpB kpAA + kpBB

51 CHAPTER 4. COPOLYMERIZATION does not depend on R• and therefore can be evaluated a priori with much higher reliability. The best way to monitor the reactor behavior is therefore to combine a sensor for measuring on-line the global polymerization rate with the equation above to split the total monomer consumption into the contributions of the two monomers.

52 Chapter 5 Heterogeneous Free-Radical Polymerization

We refer in particular to suspension and emulsion polymerization. In both cases we start from a suspension of monomer droplets (dd = 100 − 1000 µm) in an aqueous solution obtained by rigorous stirring with the addition of some surfactant or emulsiﬁer. We then add an initiator which is monomer soluble for suspension and water soluble for emulsion polymerization. Suspension Polymerization: At the end of the reaction we obtain a suspension of polymer particles with the same size as the original monomer droplets, i.e., dp ≈ 100 − 1000 µm. The radicals produced inside the particles promote the polymerization which proceeds just like in a bulk, thus following the kinetics described earlier for homogeneous polymerization.

Emulsion Polymerization: In this case the ﬁnal size of the polymer particles is dp ≈ 100 nm, that is much smaller than the original monomer droplets. The mechanism of this process and the corresponding kinetic behavior are more complex and have to be treated separately.

5.1 Concept of Micellar Particle Nucleation

Emulsiﬁer molecules form in water solution aggregates called micelles, when the total con- centration of emulsiﬁer tends to exceed a given concentration, the so-called critical micellar concentration (cmc). This can be seen from surface tension measurements or from measurements of the free emulsiﬁer concentration in the water phase, Ew. The radicals produced in solution are initially hydrophilic, but after adding a few monomer units by solution polymerization, become enough hydrophobic to diﬀuse into the organic phase. There are two possibilities, the monomer droplets or the micelles, which in their core

53 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

surface tension

EW

cmc added amount of E per unit volume

solubilize some monomer. The choice depends upon the surface area available for transport:

6 6 −1 monomer droplets ⇒ φM ≈ 0.50 · ≈ 0.03µm dd 100 6 6 ⇒ φ ≈ . · ≈ µ −1 micelles E 0 01 −2 6 m dm 10 It follows that most of the radicals enter the micelle, and there start the polymerization with the monomer. At this point we say that a new polymer particle has been formed (nucleated).

5.2 Radical Segregation

The very small size of the polymer particles leads to the radical segregation which is the characteristic feature of emulsion polymerization. Let us consider the minimum possible radical concentration in an emulsion polymer particle where bimolecular termination can occur: 2 2 R• ≈ . · −5 = = −18 23 0 3 10 mol/L (5.1) vpNA 10 · 6 · 10

7 By considering a typical value for the termination rate constant, kt = 5 · 10 L/mol/s, leads to a characteristic time for termination equal to:

1 −2 τt = • = 10 s (5.2) ktR

−3 Comparing this with the characteristic time for propagation, τp ≈ 10 s we conclude that the two radicals can add only a few monomer units before terminating. We can now consider the number of radicals in a particle, n as a function of time:

54 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

n

t t 2 t t

t t 1 e e

t t 0 e e time

We see that this follows a periodic evolution, where τe represents the characteristic time of en- try of a radical from water phase in the polymer particle. We can then compute an approximate value of time average number of radicals per particle:

0 · τ + 1 · τ + 2 · τ τ + 2 · τ n = e e t = e t (5.3) 2 · τe + τt 2 · τe + τt which since τt τe, leads to: n ≈ 0.5 (5.4)

Note that most of the propagation of the radicals occurs when the radical is alone in the par- ticle, and this lasts for a time equal to τe. Thus, in order to have suﬃciently high molecular weights the initiator concentration is adjusted so that τe τp. From this it follows that

τe τt. The radical segregation has an important consequence on the quality of the produced poly- mer:

• Non-segregated system (homogeneous)

k M k R•2 ∝ p rate of termination = t nN • • ⇒ ktR rate of propagation = kp MR • Rp ∝ kp MR

• We have a conﬂict: in order to have high molecular weights, nN we need low R , but

this leads to low rate of polymerization, Rp. This is because of the coupling between ter- mination and propagation through the radical concentration, the ﬁrst one having larger reaction order.

55 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

• Segregated system (emulsion)

nN = (rate of monomer addition) · τe 1 · = kp Mp • keRw spNA • n n Rp = kp MpRpvpNp = kp Mp vpNp = kp Mp Np vpNA NA

• where ke is the mass transfer coeﬃcient of the radicals in the water phase, Rw into the • polymer particles with surface sp and volume vp; Mp and Rp are the monomer and radical

concentrations in the polymer particles, and Np is their number per unit volume of water.

It is seen that the quantities are now decoupled, and we can obtain high molecular weights with high productivity.

5.3 Phase Partitioning

During an emulsion polymerization process we have polymer particles, micelles and monomer droplets dispersed in the water phase. Monomer and free emulsiﬁer are partitioned among these phases according to equilibrium. Since the external surfaces are very large (very small particles) the transport kinetics is in fact much faster than the polymerization reaction.

monomer droplets micelles

polymer particles

56 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

5.3.1 Monomer

sat As long as monomer droplets are present, Mw+Md > Mw (where the indices refer to water and sat to the monomer droplets and Mw is the concentration at saturation conditions), three phases are present, namely water, polymer particles, and monomer droplets. In this case we have:

M M M aw = ap = ad (5.5)

M where a j is the activity of the monomer in phase j. Since the monomer droplets consist of M pure monomer ad = 1. Therefore the activity and concentration in the water and the polymer,

Mw and Mp, remain constant, as long as monomer droplets are present. As the monomer is hardly soluble in water and its amount in the core of the micelles is usually negligible, most of the monomer is partitioned between the monomer droplets as well as in the swollen polymer particles (up to 60% in volume). When the monomer droplets are consumed we have:

M M aw = ap (5.6)

The activities can be computed using suitable thermodynamic models (Flory Huggins,Uni- quac, equation of states), to provide the concentration of the monomer in the two phases, Mw and Mp.

5.3.2 Emulsiﬁer

Similarly, as in the previous case we have:

E E aw = ap (5.7)

If Ew > cmc, then we have the formation of a third phase, the micelles. As long as micelles are present, the value of Ew does not change and we have Ew = cmc. The above activity equality is in general represented by the Langmuir isotherm, which better describes the adsorption of the emulsiﬁer on the surface of the polymer particles. ΓE, the adsorbed emulsiﬁer concentration [mol/vol] is given by:

∞ KEEw ΓE = ΓE (5.8) 1 + KEEw ∞ where KE is the adsorption equilibrium constant and ΓE is the saturation concentration, which is achieved when the entire surface of the particle per unit volume, ap = sp/vp is covered by

57 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

the emulsiﬁer. By deﬁning aE the surface area covered by a single emulsiﬁer molecule we get:

∞ ap ΓE = (5.9) aENA The emulsiﬁer amount adsorbed on the monomer droplets is usually negligible.

5.4 Colloidal Stability

Besides its role in the nucleation process, the emulsiﬁer is also very important in providing colloidal stability to the polymer particles. Let us consider an ionic surfactant (steric surfac- tants can also be used) where the surfactant molecule carries a net charge on the polymer particles, thus making them to repel each other and prevent coagulation. As a rule of thumb, in order to avoid coagulation we have to keep most of the particle surface covered by the surfactant. Since the particles grow during polymerization, this can be achieved by adding the emulsiﬁer during reaction and proportionally to the increase of the total polymeric surface.

5.5 Kinetic Mechanism of Emulsion Polymerization (Smith & Ewart, 1954)

The process is typically divided in three intervals.

Interval I: Nucleation

As soon as the radicals produced by the initiator enter the micelles we have the formation of new polymer particles. Other nucleation mechanisms are possible, but we now restrict only to the micellar one. In principle, we have that some of the radicals can terminate in the aqueous solution, some may enter the monomer droplets and some the previously formed polymer particles. However, particularly for fast nucleation the vast majority of radicals produced by the initiator enter the micelles, and therefore as a ﬁrst approximation we have:

dNp = R (5.10) dt I The nucleated polymer particles (increasing in number) grow by taking monomer from the aqueous solution (and eventually from the monomer droplets), their surface grows and adsorbs more and more surfactant. The surfactant available in the water phase decreases until all

58 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

micelles disappear and the concentration of emulsiﬁer Ew starts dropping below cmc. This indicates the end of the nucleation interval, and the number of particles will thereafter remain constant.

Interval II: Growth

In this stage of the process the number of particles remains constant but their volume grows over time. The volume of a single particle, vp, consist of polymer and monomer, vp = vmon + vpol. The volume fraction of the monomer and the polymer in the particle can be written as follows: v φ = mon (5.11) vp and vpol 1 − φ = (5.12) vp As long as monomer droplets are present (interval I and II) the volume fraction of monomer dissolved in the particle stays constant, φ = const. ≡ φ∗ (can reach values up to 0.6). First we will consider the volume growth of polymer in a single particle, vpol:

m dvpol • Mmon = kp MpRpvp (5.13) dt ρpol with ρ M φ∗ mon p = m Mmon and • n Rp = NAvp one obtains dv ρ n Mm pol k φ∗ mon v mon = p m p dt Mmon vpNA ρpol ∗ n ρmon = kpφ (5.14) NA ρpol where the ﬁrst three factors represents the moles of monomer reacted per unit time and per unit m volume, Mmon is the monomer molecular weight and ρmon and ρpol the monomer and polymer densities respectively. From this, the volumetric growth of a single particle can be derived as

59 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION follows: ! dvp d vpol dvpol 1 = = dt dt 1 − φ∗ dt 1 − φ∗ ∗ φ n ρmon = kp ∗ (5.15) 1 − φ NA ρpol

Note that vpol is always increasing, whereas vp is only increasing, when φ = const. (interval I and II). Since n = 0.5 and φ∗ is kept constant by the presence of the monomer droplets, it follows that: dvp = const. ≡ c (5.16) dt The overall reactor productivity

d dvp R ∝ v N = N = N c (5.17) p dt p p p dt p remains also constant during this interval. This interval continuous as long as monomer droplets are present, after this the monomer concentration in the water phase drops below its saturation value, indicating the end of the growth interval.

Interval III: Monomer Depletion

The polymerization process continues in the polymer particles. The monomer concentrations

Mw and Mp decrease in parallel, and the rate of polymerization consequently decreases up to the end of the process.

I II III monomer conversion Rp

Vpol

time

60 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

Comments

• The rate of polymerization increases in interval I due to the increase of Np:

dvp R ∝ N = (R t) c (5.18) p p dt I while it remains constant in interval II and decreases to zero in interval III. This leads to the sigmoidal behavior of the monomer conversion curve, whose derivative is propor-

tional to Rp.

• We assumed that the polymer particles do not coagulate, since they are kept colloidally stable through the addition of surfactant during the polymerization. If we add all the emulsiﬁer at the beginning we make a lot of micelles, therefore many small particles with a large surface that most likely leads to coagulation.

5.6 Kinetics of Micellar Particle Nucleation

During intervals I and II, the growth of the volume of a single particle, vp is given by 5.15:

∗ dvp φ n ρmon = kp ∗ dt 1 − φ NA ρpol Since in these intervals φ∗ = const. and we can assume n = 0.5, the quantity above is equal to a constant: dvp = c (5.19) dt

61 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

If we assume that the nucleation interval is very short, we can approximate that all the radicals produced by the initiator, RI enter the micelles, so that:

dNp = R (5.20) dt I where neglecting the initiator consumption we have that RI is constant. The nucleation stops when the micelles disappear, that is when all emulsiﬁer is adsorbed on the polymer particles. By taking KE 1, the emulsiﬁer adsorption isotherm simpliﬁes to ∞ ΓE = ΓE and the condition for the end of the nucleation interval reduces to:

∞ 0 0 NpfvpfΓE = E − cmc ≈ E (5.21) where E0 is the overall concentration of emulsiﬁer originally introduced in the reactor while

Npf is the ﬁnal value of the number of polymer particles per unit volume of water, Np, and tf is ∞ the time at the end interval I. Since ΓE = ap/aENA we obtain:

0 Npfvpfapf = Npf spf = E aENA (5.22)

Using equations (5.19) and (5.20) we have:

Npf = RItf vpf = ctf (5.23)

Note that 2 ) sp = 4πr 1 2 p 3 3 4 3 ⇒ sp = (36π) vp (5.24) vp = 3 πrp

1 2 3 3 0 ⇒ Npf (36π) vpf = E aENA (5.25)

Npf vpf = ctf = c (5.26) RI

2 ! 3 1 2 Npf 0 Npf (36π) 3 c 3 = E aENA RI 2 5 R 3 1 ⇒ 3 0 I Npf = E aENA 1 c (36π) 3 ! 2 3 R ρ N 5 1 ⇒ N E0a N 5 I p A pf = E A m 1 (5.27) kpnMp Mmon (36π) 5 We conclude that the ﬁnal number of particles per unit volume of water grows with the power of 0.6 of the initial emulsiﬁer concentration, E0 and the power 0.4 of the initial initiator con- centration, I0.

62 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

5.7 Distribution of Active Radicals in the Polymer Particles

The following physicochemical steps are involved in the process:

r knd

ct n(n-1)

• Radical entry from the aqueous phase:

rad. • = keR spNA ≡ ρ (5.28) time × part. w

where ke is the mass transfer coeﬃcient of the radicals from the water into the polymer particles.

• Radical desorption from the polymer particles:

rad. n = kd vpNA ≡ kdn (5.29) time × part. vpNA

where kd is the mass transfer coeﬃcient of the radicals exiting the particles. Note that this is usually associated with a chain transfer to monomer event, which, if the monomer is water soluble, produces a soluble radical.

• Radical termination in polymer particles:

events n (n − 1) 1 = kt vpNA ≡ ct(n − 1)n (5.30) time × part. vpNA vpNA 2

where ct is the inverse of the termination characteristic time in the polymer particles.

Now we consider a population balance for polymer particles that at time t contain n active radicals: dN n = ρN + k (n + 1)N + c (n + 2)(n + 1)N dt n−1 d n+1 t n+2 −ρNn − kdnNn − ctn(n − 1)Nn (5.31)

63 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

dNn dt n(n-1)ct

ρ ρ

n-2 n-1 n n+1 n+2

kd n kd(n+1)

(n+2)(n+1)ct

Let us introduce the PSSA for Nn and two new parameters: k ρ m = d and α = (5.32) ct ct so we get:

αNn−1 + m(n + 1)Nn+1 + (n + 2)(n + 1)Nn+2

= (α + mn + n(n − 1)) Nn (5.33) The solution has been found in terms of modiﬁed Bessel functions (Stockmayer, 1957): √ Im+n−1 a/ 2 n (m−1−3n)/2 Nn = Npa 2 (5.34) n!Im−1 (a) √ with a = 8α, and the average number of radicals per particle:

P∞ n=0 nNn n = P∞ (5.35) n=0 Nn

Let us ﬁrst consider the case with no desorption, i.e., m = 0. We see that as α → 0 or ρ ct

(which is equivalent to τe τt in section 5.2) we have n → 0.5. From the PBE above for m = α = 0 we have: n(n − 1) N = N (5.36) n+2 (n + 2)(n + 1) n

64 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION

log n

log a

which implies, for n = 0, 1, 2 ... that N2 = N3 = ... = 0. For computing N0 and N1 we use the closure equation: If a radical enters a particle with the maximum number of radicals, then it terminates imme- diately. dN 0 = −ρN + ρN dt 0 1 1 ⇒ N0 = N1 = Np (5.37) dN 2 1 = ρN − ρN dt 0 1 that is n = 0.5. In this case we have a so-called 0-1 system, that is one where half of the particles have zero radicals and the other half one. In order to appreciate the inﬂuence of radical segregation on its average number, let us consider a bulk model, where we assume n 1, and then n(n − 1) ≈ n2. In this case the balance of the radicals in a particle reduces to:

dn = ρ − 2c n2 − k n (5.38) dt t d and using the PSSA for n and introducing the above dimensionless parameters we obtain:

α − 2n2 − mn = 0 (5.39) which in turn leads to: √ −m ± m2 + 8α n = (5.40) 4

65 CHAPTER 5. HETEROGENEOUS FREE-RADICAL POLYMERIZATION where the negative root is meaningless. The bulk model approximation above is valid when termination is low, so that we can have radical accumulation in the particle. In this case: √ √ −m + m2 + 8α → 8α (5.41) and therefore p n → α/2 (5.42) which is independent of the desorption rate and approaches the straight line emerging for α → ∞ appearing in the plot above, computed in the case of radical segregation. We conclude that for n ≥ 3 the polymer particles behave like a bulk (non segregated) system. Thus depending on the value of α the system can approach a segregated behavior (α 1) or a bulk one (α 1). The ﬁrst one occurs because, even if termination is very fast (ct → ∞), as a single radical in a particle cannot terminate. Accordingly, the limit for α → 0 is n = 0.5 and not n = 0. However, this is not true when desorption is present, since even a radical which is alone in the particle can desorb. Desorption becomes important when m > α, as it is indicated in the ﬁgure where it is seen that straight lines indicating n deviate from the segregated value n = 0.5 at α values below the speciﬁc m under examination. Note that since in these conditions bimolecular termination cannot occur we can use the bulk model: dn = ρ − k n ≈ 0 (5.43) dt d which leads to α n = (5.44) m which justiﬁes the straight lines with slope equal to one in the ﬁgure above which describe the system behavior in the region dominated by radical desorption.

66 Chapter 6 Stability of Colloidal Suspensions

6.1 Kinetic Stability of Colloidal Suspensions

DgDo G=fslsl A

interfacial surface 2 tension (sol/liq) [J/m2 ] sol/liq surface change [m ]

γsl > 0 ⇒ colloid state is unstable, i.e., lyophobic (in water: hydrophobic); you need work to create a dispersion (⇒ mixing)

γsl < 0 ⇒ colloid state is stable, i.e., lyophilic (in water: hydrophilic) Lyophobic colloids can be made kinetically stable by building an energy barrier suﬃciently large with respect to the thermal energy of the particles, kT. Two stabilization mechanisms are possible: • electrostatic: the particles are electrically charged

• steric: the particles are coated with some material (e.g. polymer) which prevents their close approach.

Concept of Kinetic Stability

Thermal energy provides kinetic energy to the colloidal particles which collide with energy (kT). The charges on the particle surface provide an energy barrier to be overcome in order to have aggregation.

67 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

kinetically G stable

colloid unstable

bulk

aggregation coordinate

6.2 Interaction between two Charged Bodies

The interaction between two bodies is dominated by two forces, an attractive van der Waals force and a repulsive electrostatic force.

6.2.1 van der Waals Forces

The origin of these forces is the attraction between a temporary dipole and the correspond- ing induced dipoles (London theory). The following semi-quantitative argument provides a reasonably accurate picture of the physics underlying these interactions. Let us use the Bohr model for a hydrogen atom, where electrons are regarded as traveling in well deﬁned orbits around nuclei. As a result of the electrons motion, every atom has an instantaneous dipole moment p approximately equal to p = a0 ∗ e, where e is the electron charge and a0 is the Bohr radius, which is a good estimate of the radius of a hydrogen atom. Let us consider two hydrogen atoms, referred to as atom 1 and atom 2, positioned at a distance R. The electric ﬁeld E generated by the instantaneous dipole 1 at distance R is given by:

p E 1 = 3 (6.1) 4π0R where 0 is the vacuum dielectric permeability. Atom 2, will be polarized by the electric ﬁeld generated by atom 1, which generates an induced dipole of strength:

αp p αE 1 2 = = 3 (6.2) 4π0R

68 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

3 where α is the polarizability of the second atom, and is approximately equal to α = 4π0a0. Since the energy of interaction of two dipoles equals:

2 2 p1 p2 αa0e C Vint = − = − = − (6.3) 3 2 6 6 4π0R (4π0) R R Equation (6.3) shows that van der Waals interactions between pairs of particles in vacuum are always attractive, and decay very strongly with the distance. However, they become consider- able at short distances. When the overall van der Waals interactions between macroscopic objects needs to be com- puted, one assumes that equation (6.3) holds for all pairs of molecules contained in the two objects. This theory has been developed by Hamaker. In this case, the van der Waals interac- tion between macroscopic object 1 and macroscopic object 2 is given by: Z Z dV dV V −C 1 2 A = 6 (6.4) V1 V2 R where the two integrations run over the entire volumes V1 and V2 of the two bodies, and R is the distance between two arbitrary points, one located within the ﬁrst object, the other one within the second object. Generally, the two integrals are diﬃcult to compute, and explicit formulas are available only for very simple geometries. As an example, let us perform the integration for the case of a semi-inﬁnite solid and a point. Equation (6.4) reduces in this case to one single volume integral, over the semi-inﬁnite body. If we indicate with d the distance between the point (named 1) and the surface of the semi-inﬁnite body, and we deﬁne a coordinate system with the x-axis along the direction of the distance d, with the zero on the surface of the body and pointing inwards the body and both other axes parallel to its surface, one can immediately recognize that the system has a rotational symmetry around the x-axis. It is therefore convenient to perform the volume integration using cylindrical coordinates. The distance R in equation (6.4) is equal to the distance between point 1 and an arbitrary point having coordinates x and z inside the body, as shown in the next Figure. By making use of Pitagora’s theorem, the volume integral in equation (6.4) reduces to: Z ∞ Z ∞ 2πz dz πC Z ∞ dx πC V = −C dx = − = − (6.5) A 3 4 3 0 0 z2 + (d + x)2 2 0 (d + x) 6d From equation (6.5) one can observe that the dependence of the van der Waals interactions between a point and an inﬁnite solid decreases as the reverse third power or the distance. The simple calculation shows the eﬀect of summing in a pair additive manner the inter- actions of all pairs of molecules belonging to two macroscopic objects. Even though the

69 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

interactions of two molecules are very weak, the overall interactions between the bodies can become signiﬁcant at short distances, for example at distances comparable to the size of the two objects. There are two important cases where the integrations in equation (6.4) can be performed analytically: (1) two inﬁnite slabs and (2) two spheres having arbitrary size and distance. The corresponding interaction potentials can be computed as follows:

• For two inﬁnite slabs at distance D: A V (D) = − (6.6) A 12πD2

• For two spheres of radius a1 and a2 at distance R: " !# A 2a a 2a a R2 − (a + a )2 V R − 1 2 1 2 1 2 A( ) = 2 2 + 2 2 + ln 2 2 (6.7) 6 R − (a1 + a2) R − (a1 − a2) R − (a1 − a2) where A is the Hamaker constant which depends on the physical characteristics, e.g., polar- izability and density, of the materials involved. In the case of two spheres, one can perform Taylor expansions of this last equation and observe that at distances much smaller than the particle radius, the interactions decay with the ﬁrst power of the distance. On the other hand, for distances much larger than the particle radius the interaction energy decays with the sixth power of the distance, as one could expect. The Hamaker constant depends not only on the physical properties of the materials the macroscopic objects are made of, but also on the dielectric properties of the medium sur- rounding the particles. The eﬀect of this medium can be extremely important in some cases.

70 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

In fact, even though Hamaker constants are usually positive, there are some cases where neg- ative values can be found for some speciﬁc types of materials/medium pairs. A negative value of Hamaker constant implies that van der Waals interactions are repulsive. One ﬁnal caveat about Hamaker’s treatment of van der Waals interactions. A much more rigorous approach of dispersion forces and van der Waals forces is available in the literature, which has been pioneered by Lifshitz. It is based on rigorous quantum mechanical calcula- tions, but the ﬁnal equations are far more complex than the Hamaker theory. However, some general features can be quickly discussed, which are necessary to point out the limitations of the simpler Hamaker theory. First of all, Lifshitz’ theory shows that the pairwise addition of interactions is a not rigorously correct, as van der Waals interactions a truly many-body prob- lem. This eﬀect can be simply accounted for by adjusting the values of the Hamaker constant. The second limitation is given by the so-called retardation eﬀect. Since atoms are ﬂuctuating dipoles, as the distance between two molecules increases beyond a certain threshold, the time required for a molecule to feel the eﬀect of the electric ﬁeld produced by another dipole be- comes signiﬁcant. This implies that the interactions of the diﬀerent dipoles are retarded, and the energy of interaction decays even stronger with the distance, i.e., with the seventh power of the distance, and not anymore with the sixth power. This eﬀect weakens van der Waals interactions for large bodies as their distance increases, compared to the predictions of the Hamaker theory. However, due to its simplicity and good accuracy, Hamaker constants are still commonly used in colloidal science.

Concept of Surface Tension

A

A

WAA = work per unit area needed to separate up to ∞ two parts of liquid column

71 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

WAA = 2γAv (6.8) where γAv is the surface tension of A in contact with vapor (vacuum). We compute WAA as the interaction energy between two ﬂat bodies and get (for hydrocarbons):

1 1 A γ = W = · (6.9) Av 2 AA 2 12πL2

Since it is diﬃcult to postulate L, we compute it from experimental values of γAv and calculated A.

Alkane CnH2n+2

20 3 2 −3 3 n 10 × A (J) 10 × γAv (J/m ) 10 × ρ (kg/m ) L (nm)

5 3.75 16.05 0.626 0.176 6 4.07 18.40 0.660 0.171 8 4.50 21.62 0.702 0.166 10 4.82 23.83 0.730 0.164 12 5.03 25.35 0.749 0.162 14 5.05 26.56 0.763 0.159 16 5.23 24.47 0.773 0.159

We observe that L:

i) has dimension of molecular radius √ ii) L ∝ 1/ ρ.

6.2.2 Electrostatic Forces Electrical Double Layer

• Outside of the outer Helmholtz plane, the ions move freely, therefore this is the plane of closest approach of (hydrated) ions (≈ 0.5 nm).

• The inner Helmholtz plane constitutes the locus of the centers of adsorbed (dehydrated) ions (≈ 0.1 nm).

72 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

IHP = inner Helmholtz plane OHP = outer Helmholtz plane

aqueous solution, eW diffusive layer

0i d x

For x > 0: ) ! ρ = div (εE) ρ Poisson ⇒ ∇2 (ψ) = − (6.10) E = −grad (ψ) ε equation P where ρ = all ions nizie, with ni = number ion concentration, zi = valance, e = electron charge; E = electric ﬁeld ε = permittivity ψ = potential referred to bulk, i.e., ψ = 0 at x = ∞.

For x > d:

The ions are free to diﬀuse and are inﬂuenced by the local electrostatic potential, so that: ! z eψ Boltzmann n = n0 exp − i (6.11) i i kT equation

0 where ni is ni in the bulk. In the diﬀusive layer, x > d, we have ε = εw and: ! 2 1 X 0 zieψ Poisson-Boltzmann ∇ (ψ) = − ni zie exp − (6.12) εw kT equation with B.C.: ψ = 0 at x = ∞, ψ = ψd at x = d. Let us consider a few speciﬁc cases for which we have analytical solutions.

• The Debye-Huckel¨ approximation:

Applies when the electrical energy is small compared to the thermal energy: |zieψ| < kT. Then, z eψ z eψ exp − i ≈ 1 − i (6.13) kT kT

73 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

which leads to P 0 2 2 ! 2 1 X 0 ni zi e ∇ ψ = − ni zie − ψ (6.14) εw kT P 0 According to the principle of electroneutrality for the bulk ni zi = 0 and, therefore, we get ∇2ψ = κ2ψ (6.15)

where P 1 n0z2e2 κ2 = i i (6.16) εw kT is the Debye-Huckel¨ parameter. The solution has the form

ψ = A1 exp (κx) + A2 exp (−κx) (6.17)

but since ψ = 0 as x → ∞, ⇒ A1 = 0 and imposing ψ = ψd at x = d ⇒ A2 = ψd exp(κd), so that

ψ = ψd exp [−κ(x − d)] , for x > d (6.18)

The distance 1/κ where ψ = ψd exp(−1) is deﬁned as the thickness of the diﬀusive layer. At 25◦C in water √ κ = 3.29 I [nm−1] (6.19)

P 2 −3 with I = 1/2 cizi is the ionic strength and ci is in mol/L. For example, for a 10 M, 1:1 electrolyte is 1/κ = 9.6 nm.

• Flat surface:

0 0 0 We consider a symmetric electrolyte, z+ = −z− = z and n+ = n− = n , so that the Poisson-Boltzmann equation becomes 1 zeψ 1 zeψ ∇2ψ = − n0ze exp − + n0ze exp + εw kT εw kT 2n0ze zeψ = sinh (6.20) εw kT and then for a ﬂat geometry d2ψ 2n0ze zeψ 2 = sinh (6.21) dx εw kT Multiplying both sides by (2dψ/dx) and integrating in x: Z dψ d2ψ 4n0ze Z zeψ dψ x x 2 2 d = sinh d (6.22) dx dx εw kT dx

74 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

y

yd

yd/e

0 d d+1/k x

!2 Z x d dψ 4n0ze Z ψ zeψ dx = sinh dψ (6.23) ∞ dx dx εw 0 kT where we account for the B.C.: ψ = 0 and dψ/dx = 0 at x = ∞

!2 dψ 4n0ze kT zeψ ψ = cosh (6.24) dx εw ze kT 0

!2 dψ 4n0kT zeψ = cosh − 1 (6.25) dx εw kT p √ Recalling that cosh(aψ) − 1 = − 2 sinh(aψ/2), we get

! 1 dψ 8n0kT 2 zeψ = − sinh (6.26) dx εw 2kT This can be integrated by variable separation as follows: Z ψ dψ 2κkT Z x = − dx (6.27) ψd sinh (zeψ/2kT) ze d

zeψ zeψ ⇒ tanh = tanh d exp [−κ (x − d)] (6.28) 4kT 4kT In the case where zeψ < kT, we can approximate tanh (zeψ/4kT) ≈ zeψ/4kT, and the solution above becomes

ψ = ψd exp [−κ (x − d)] (6.29) which is the Debye-Huckel¨ approximate solution.

75 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

A couple of comments on the results above: a) Approximate behavior:

y y 2kT ze

y 4kT d yd ze

d x d x

kT for ψ < 2 ⇒ ψ ≈ ψ exp [−κ(x − d)] d ze d kT zeψ for ψ > 4 ⇒ tanh ≈ exp [−κ(x − d)] d ze 4kT

(since tanh (y) → 1 as y → ∞) which suﬃciently away from the surface, where ψ is small, leads to 4kT ψ = exp [−κ (x − d)] (6.30) ze

that is away from the surface the potential behaves like in the case where ψd =

4kT/ze, although ψd is much larger. b) If we take d = 0, and ignore the IHP and OHP, this treatment corresponds to the Gouy and Chapman model. The ﬁgures show the eﬀect of electrolyte charge and concentration on the potential behavior predicted by Debye-Huckel.¨ The points

indicate the value ψ/ψd = exp(−1) and the corresponding Debye thickness 1/κ.

1/κ Celectrolyte

9.60 nm 0.001 M 3.00 nm 0.01 M 0.96 nm 0.1 M It is seen that both the electrolyte concentration and its charge can strongly aﬀect the thickness of the double layer. This is known as double layer compression and is widely

76 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

used in applications to destabilize colloids. However, the predictions of this model on

a quantitative basis are often unrealistic. For example in the case of ψd = 100 mV with 0 0 n = 0.001 M, a surface concentration value nd = n exp (zeψd/kT) = 0.001 exp(12) = 160 M is obtained. This result can be corrected introducing the Stern layer, where some counterions are strongly associated with the surface, thus also neutralizing some of the surface ions.

Simple Example for a Boltzmann Distribution

Let us consider the molecules in the atmosphere which are free to move according to Brownian motion but are also subject to the gravitational ﬁeld.

h P

dh

P+dP

77 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

By applying Newton law to a thin slice of atmosphere dh we get:

dP = −ρg dh (6.31) where ρ is the mass density which using the ideal gas law can be expressed as follows: PM ρ = nM = (6.32) RT where M is the molecular weight and n is the number molecule concentration. Substituting in the previous equation this leads to: dP Mg = − dh (6.33) P RT which integrated with I.C.: P = P0 at h = 0 yields: Mg P = P exp − h (6.34) 0 RT

Recalling that M = mNA, where m is the molecule mass and NA the Avogadro number, while

R = kNA and pressure is proportional to the number molecule concentration the above equation leads to: ! mgh n = n exp − (6.35) 0 kT which, since (mgh) is the gravitational potential, coincides with the Boltzmann equation (6.6).

A More Rigorous Derivation of the Boltzmann Distribution

In order to fully justify the use of the Boltzmann distribution to describe the dependence of the concentration of ions on the electrostatic potential, let us consider the following thermo- dynamic argument. In the presence of a charged surface, which generates an electric ﬁeld, the thermodynamic function which determines the equilibrium condition of the ions is the electrochemical potential eµ, deﬁned as:

eµ = µ + zeψ (6.36) where z is the valence of the ion, ψ is the electrostatic potential at the location considered and µ is the chemical potential. The signiﬁcance of the electrochemical potential is that of free en- ergy per molecule in the presence of electric ﬁeld. For every ion, the electrochemical potential has to be constant in the entire space in order to guarantee the thermodynamic equilibrium. Therefore, by considering two diﬀerent locations, one at distance x from the surface, where the

78 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS electrostatic potential is ψ(x), and the other one in the bulk of the solution, at inﬁnite distance from the surface, where the electrostatic potential is equal to zero, the equilibrium conditions reads: eµ(x) = µ(x) + zeψ(x) = eµ(x = ∞) = µ(x = ∞) (6.37) By using the deﬁnition of chemical potential:

µ(x) = µ0 + kT ln (a(x)) (6.38) where a(x) is the activity of the species at a distance x from the surface and µ0 is a reference chemical potential. By neglecting concentration eﬀects, we can replace the activity by the number concentration, i.e., a(x) ≈ n(x). Therefore, by calling n0 the number concentration of the ion in the bulk of the solution, equation (6.37) becomes:

kT ln (n(x)) + zeψ = kT ln(n0) (6.39) which leads to the Boltzmann distribution of the ion: zeψ n(x) = n exp − (6.40) 0 kT Therefore, the Boltzmann distribution arises naturally (at least for dilute electrolyte solutions) as a consequence of thermodynamic equilibrium in the presence of an electric ﬁeld.

Electrostatic Potential of Interaction

When two charged bodies approach each other the corresponding double layers overlap, the local ion concentration increases compared to the bulk, thus creating an osmotic pressure and therefore a corresponding repulsive force.

y0 y0 y( x )

x 0 D

79 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

Depending on the kinetics of the approach we can have that the ions may have or not time enough to equilibrate. We distinguish three limiting situations:

• constant surface potential, ψ0 ⇒ slow approach;

• constant surface charge, σ0 ⇒ fast approach or ions covalently bound to the surface;

• charge regulation ⇒ the surface groups can dissociate to an extent which depends on the interaction, as for example: −eκ N − + ⇒ − − d s SH S + H σ0 = eS s = +0 (6.41) κd + H exp (−eψ0/kT)

In order to compute the repulsive force between two charged inﬁnite planar surfaces at a distance h, let us consider the following simple argument. At equilibrium, all forces acting on a volume element located between the two plates must balance. The only two forces acting are the electrostatic forces and the osmotic pressure. The osmotic pressure force per unit volume is equal to: dp F = − (6.42) p dx where x is the coordinate perpendicular to the two surfaces. On the other hand, the electrostatic force per unit volume equals the product of the charge density with the electric ﬁeld, and can be written as: dψ F = −ρ (6.43) el dx By using the Poisson equation, this force balance can be recast in the following form:

dp d2ψ dψ − = 0 (6.44) dx dx2 dx The integration of this equation gives:

!2 dψ p − = const. (6.45) 2 dx

This last equation implies that the sum of the osmotic pressure and the so-called Maxwell pressure, /2 · (dψ/dx)2, are constant in the whole domain. Due to the symmetry of the sys- tem considered here, at the midplane the electrostatic potential proﬁle has to have an ex- tremum (minimum if the surface are positively charged, maximum otherwise). Therefore

(dψ/dx)x=h/2 = 0, and the constant in equation (6.45) is equal to the osmotic pressure at the

80 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS midplane. Therefore, once the pressure at midplane is known, the force acting on the planes can be computed, and by integrating the force, the energy of interaction can be derived. In order to determine the pressure at midplane, we can once again use the force balance written as: dp = −ρ dψ (6.46)

In order to simplify the calculations, let us assume to have a solution containing just a symmet- ric z–z electrolyte. By making use of the Boltzmann distribution for the ions concentration, one obtains: zeψ dp = 2zen sinh − dψ (6.47) 0 kT

This equation can be easily integrated between the following limits: p = p0 in the bulk (when

ψ = 0), and p = ph/2 at ψ = ψh/2. The result is the following: " zeψ ! # p − p = 2kTn cosh − h/2 − 1 = F (6.48) h/2 0 0 kT R

The conclusion is that the repulsive force between the planes can be computed if the potential at midplane is known. This can be obtained by integrating the Poisson-Boltzmann equation. One should then notice that the electrostatic repulsive energy (per unit surface) is obtained from the repulsive force per unit surface as follows:

dVel = −FR dh (6.49)

The physical interpretation is that the potential energy per unit surface of two plates at a distance h is equal to minus the work done to bring the plates from inﬁnite distance to the current distance h. Several approximate relations have been developed to compute the electrostatic repulsive potentials between two bodies.

• For small degree of double layer overlap (any geometry), D 1/κ:

64n0kTZ2 Vψ = exp (−κD) (6.50) R κ

zeψ Z = tanh 0 (6.51) 4kT σ ψ In this case VR ≈ VR since the discharge remains anyway small due to the small overlap. This corresponds to the case where the potential at midplane is approximated by the sum

81 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

y0 y0

y m y( x )

x 0 D

of the potentials of two isolated charged inﬁnite planes. This approximation is only valid for small overlapping.

• For small potentials of the two surfaces, zeψ0 kT:

In this case we can apply the Debye-Huckel¨ approximation 2n0kT zeψ 2 κD Vψ = 0 1 − tanh (6.52) R κ kT 2 • Most convenient in applications are: 32n0kT κD Vψ = z2 1 − tanh (6.53) R κ 2

0 " # σ 2n kT B + y0 coth (κD/2) VR = 2y0 ln (6.54) κ 1 + y0 ! h 2 i − ln y0 + cosh (κD) + B sinh (κD) + κD (6.55)

1/2 h 2 2 i where y0 = zeψ0/kT and B = 1 + y0 cosh (κD/2)

• Illustrations:

The next ﬁgure shows a comparison of the three repulsive potentials. The one for con- stant charge is clearly the largest, while the charge regulation solution is somehow inter- ψ mediate. The next ﬁgure shows that VR decreases with distance and with y0 = zeψ0/kT. The approximate expression for D 1/κ (dotted) is compared with exact solution (solid).

82 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

83 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

6.2.3 Total Interaction Energy

The total potential energy of interaction is given by the sum of the attractive and the repulsive contributions derived earlier:

VT = VA + VR (6.56)

Using expressions developed for ﬂat surfaces and symmetric electrolyte, we get:

A 32n0kT κD V = − + z2 1 − tanh (6.57) T 12πD2 κ 2 which is illustrated in the ﬁgure on the next page. It is seen that the van der Waals forces dominate at low distances, where however VT does not go to −∞, but contrary increases due to the occurrence of Born repulsion forces, which are very short-range and come into play when the atom of the two surfaces come in contact. This leads to the very deep attractive well, referred to as primary minimum. At high distances, the van der Waals forces prevail again, often leading to the formation of a secondary minimum.

84 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

Note

Because of the large depth of the primary minimum the energy barrier for separating two particles is much larger, often substantially inﬁnite, compared to that corresponding to the reverse process.

6.2.4 Simple Manifestation of Electrical Double Layers: Soap Films

The ﬁgure shows a soap ﬁlm, where the water molecules are kept in the ﬁlm by the repulsive forces between the layers of surfactant molecules adsorbed at the air-liquid interface.

double layers repulsion

gravity on water molecules

For the ﬁlm formed with a wire frame in the ﬁgure, at each height, H the hydrostatic pres- sure (Hρg) which tends to drain the water molecules have to be balanced by the double-layer pressure, which corresponds to a certain thickness of the ﬁlm, D that can be measured. For example at height of about H = 10 cm, the repulsive double-layer pressure has to be of the order of 103 N/m2. Soap ﬁlm thickness of about 20 nm were stabilized by the overlapping diﬀusive double layers with ψ0 ≈ 30 mV.

85 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

6.3 Coagulation of Colloidal Suspensions

From the shape of the total interaction potential curve as a function of particle distance we can deﬁne the stability of a colloid or a latex. This is illustrated in the ﬁgure below, where we have: a = kinetically stable or meta-stable colloid; b = marginally unstable (critical condition) c = unstable

The loss of stability, or particle aggregation, can be induced in two ways as described in the following.

6.3.1 Aggregation by Potential Control

We can change the particle charge, and then its potential, as shown by the curves in the previ- ous ﬁgure. The most common way to bring charges on the surface of particles is to adsorb ionic surfac- tants. These can be salts which are fully dissociated (e.g. sodium dodecylsulfonate) or weak acids (e.g. carboxylic acids) that dissociate to an extent which depends upon the solution pH.

86 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

Another possibility is to act on the concentration of the so-called potential determining ions, as we discuss next. When considering a dispersion of solid AgI particles in water, since the solution is saturated we have: e e aAg+ aI− = KS (6.58) where KS is the solubility product. In addition, due to the solid-liquid equilibrium we have that the activities of each ion are equal in the two phases:

e s aAg+ = aAg+ (6.59)

e s aI− = aI− (6.60) This in general implies that, since the aﬃnity of Ag+ and I− to the solid and solution is diﬀerent, the particle acquires a charge. We can aﬀect such particle charge by acting on the activity of the ions in the solution. If we add AgNO3, then aAg+ in solution increases and aI− has to decrease, thus increasing the positive particle charge. In this case Ag+ and I− are the potential-determining ions, and we can use them to control the particle charge and potential.

87 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

The ﬁgure below shows the potential proﬁle and the counterion distribution around a charged particle: they have to follow the potential distribution but thermal diﬀusion tends to uniformize them, the result is the diﬀusive electrical double layer.

6.3.2 Aggregation by Electrolyte Addition

Even if the concentrations of the potential determining ions are such as to give a good sur- face charge, and therefore stability to the particles, we can induce aggregation acting on the indiﬀerent ions, that is causing the double layer compression. This is shown in ﬁgure 6.3.1 as well as in ﬁgure 6.3.2, where we see that as the concentration of the indiﬀerent electrolyte increases, the energy barrier decreases and eventually becomes zero. At this point there is no opposition to aggregation, which becomes very fast and controlled by Brownian diﬀusion. The smallest electrolyte concentration leading to such a fast coagulation is called critical coagu- lation concentration. Typical values for three diﬀerent colloids are reported in the table below:

88 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

Valency of Sol of As2S3 Sol of Au Sol of Fe(OH)3 counterions negatively charged negatively charged positively charged

Monovalent LiCl 58 NaCl 9.25 NaCl 51 NaCl 24 1/2BaCl2 9.65 KNO3 50 KNO3 23 KNO3 12

Divalent MgCl2 0.72 CaCl2 0.41 K2SO4 0.205 MgSO4 0.81 BaCl2 0.35 MgSO4 0.22 ZnCl2 0.69 K2Cr2O7 0.195

Trivalent AlCl3 0.093 1/2Al2(SO4)3 0.096 1/2Al2(SO4)3 0.009 Ce(NO3)3 0.080 Ce(NO3)3 0.003

It is seen that the ccc values seem to be independent of the electrolyte type but strongly af- fected by the charge of the counterion. The value of the ccc can be computed from a suitable expression of VT(D) by imposing the two conditions for criticality: dV V = 0 and T = 0 (6.61) T dD

89 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

Let us consider the case of ﬂat surfaces with small overlapping (κD > 1):

A 64n0kTZ2 V = − + exp (−κD) (6.62) T 12πD2 κ By setting 2A 64n0kTZ2 V0 = − κ exp (−κD) = 0 (6.63) T 12πD3 κ and substituting in the equation VT = 0, we get

2A A 2 − κ = 0 ⇒ − κ = 0 ⇒ κD = 2 (6.64) 12πD3 12πD2 D

Substituting in the relation VT = 0, we get the critical κ:

(4 · 12 · 64)πn0kTZ2 exp (−2) κ3 = (6.65) A and recalling for symmetrical electrolytes z = z+ = z−

P 0 2 2 2 2 2 ni zi e 2NAz e κ = = Cs (6.66) εwkT εwkT

0 where Cs = ni /NA is the molar electrolyte concentration, it follows

2 2 3 5 4 (384) (4π) εw(kT) Z ccc[mol/L] = 2 6 (6.67) 2 exp (4) NAA (ze) which at 25◦C in water for relatively high potential so that Z ≈ 1, reduces to

87 · 10−40 ccc = [mol/L] (6.68) z6A2 This relation, although approximated, correctly predicts that the ccc value depends only on the charge of the electrolyte and in a rather strong way. This is known as the Schultz-Hardy rule. Its reliability is clearly demonstrated by the data shown in the table, where for the colloid

As2S3 we have that the ccc values for mono, di and trivalent electrolytes can be scaled as follows: 50 : 0.7 : 0.09 ≈ 1 : 0.014 : 0.0018 (6.69) which compare well with the equation prediction 1 : 2−6 : 3−6 = 1 : 0.016 : 0.0014. It is conﬁrmed that the type of electrolyte, if the valency is the same, plays a minor role.

90 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

Note

Since the stability behavior of colloids is dominated by the concentration of the counterion, we can restrict our attention to symmetric electrolytes. Then, MgCl2 would behave like a 2:2 electrolyte in the presence of negatively charged surfaces, and like a 1:1 electrolyte in the presence of positively charged surfaces. This is conﬁrmed by the ccc data reported in the previous table.

6.4 Steric Interactions

Steric interactions are the third important type of interactions between colloidal particles. Steric interactions are commonly used to stabilize particles when long term stability is re- quired. The most common way to achieve steric stabilization is to graft some polymer on the particle surface. The grafting can be achieved in various ways. The most common is to add polymer to a solution of particles and let it attach onto the particle surface. However, the amount of polymer to be added has to be accurately chosen, otherwise unwanted desta- bilization eﬀects (instead of stabilization) such as depletion induced ﬂocculation or bridging ﬂocculation can arise. Recently, another method has been developed, which consists in grow- ing a polymer brush directly from the particle surface. The physical mechanism underlying steric stabilization is strongly related to the thermody- namic behavior of polymers in solutions. The simplest theory used to explain this mechanism is the Flory-Krigbaum theory. As two particles coated with a polymer layer approach each other, when the center-to-center distance is small enough there is an overlap between the poly- mer layers. This overlap generates an change in the free energy of the polymer layers. There are two contribution of the free energy of the solution: the ﬁrst one is a mixing contribution, the second one is an elastic contribution to the free energy. For the ﬁrst case, if the polymer volume fraction in an isolated layer is equal to φ, then the overlapping leads to a concentration of 2φ in the lens region, as depicted in the ﬁgure. Polymer chains, if soluble in a solvent, occupy a large amount of volume, and their confor- mation is that of a random coil. If the degree of polymerization of the coil is equal to n, the size of the coil scales as R ∼ n0.5. Therefore, if a chain is trying to occupy the same volume already occupied by another chain, there is usually an increase in the free energy of the sys- tem. The change in free energy resulting from the overlap of two sterically stabilized particles

91 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

is equal to:

∆G = ∆GovVlens (6.70)

The ﬁrst term on the right hand side is the free energy change per unit volume, while the second term is the volume of the lens where the overlap occurs. The volume of the lens is a pure geometrical term, and is equal to:

!2 ! 2π d d V = δR − 3R + 2 ∗ δR + (6.71) lens 3 s 2 s s 2 where d is the surface to surface distance between the cores of the particles, δRs is the outer radius of the shell and Rs is the radius of the core (see the previous Figure). The free energy of overlap per unit volume is equal to:

2 ! V2 1 ∆Hov = 2kT − χ (6.72) 2 2 V1Vd where Vd is the volume occupied by a polymer coil, V1 is the solvent molar volume, and V2 is the polymer molar volume. It is important to note that the sign of the free energy of mixing per unit volume depends on the parameter χ. In units of kT, the parameter χ is a measure of

92 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS the energy change between solvent-monomer interactions and solvent-solvent and monomer- monomer interactions. Mathematically this is expressed as follows: z χ = (2w − w − w ) (6.73) 2kT 12 11 22 where z is the coordination number of a monomer (or solvent) molecule, and wi j is the energy of interaction between molecule i and molecule j. Here 1 are solvent molecules and 2 are monomer molecules. Therefore, depending on whether the monomer units like more solvent molecules rather than other monomer units, the χ parameter can become smaller or larger than 1/2. When χ > 1/2 we are in the presence of a bad solvent, i.e., the monomer units prefer to stay close to each other because the polymer is not soluble under those conditions in that solvent. This means that the free energy given by equation (6.72) is negative. In this case, interpenetration of polymer shells is favored, and the polymer does not provide a good stabilization. If instead χ < 1/2 the free energy given by equation (6.72) is positive, and interpenetration is unfavorable. In that case, steric stabilization is eﬀective. It is quite common that the quality of solvent can be changed for many polymers by simply playing with the temperature. In fact, the following temperature dependence of the χ parameter on the temperature is usually observed: ! 1 Θ − χ = ψ 1 − (6.74) 2 T where Θ is the famous Theta temperature. T > Θ implies a good solvent, while T < Θ implies a poor solvent. T = Θ is the critical solubility temperature for many solvents. The second contribution to steric stabilization, arising when two polymer shells try to in- terpenetrate, is the elastic contribution. This mechanism underlying elastic stabilization is actually an entropic one, since polymer coils tend to assume in absence of any constraint a rather swollen conﬁguration. By compressing a polymer, one limits their degrees of freedom and this reduction in conﬁgurational entropy generates a force that for small compressions can be approximated as obeying Hook’s law, with an elastic constant equal to:

3kT ∆S ∝ k d, where k = (6.75) ov H H nl2 where n is the degree of polymerization of a chain and l is approximately the length of a monomer unit. The contribution to the total free energy given by this mechanism is always positive, which means that compression of a polymer coil is always an unfavorable process.

93 CHAPTER 6. STABILITY OF COLLOIDAL SUSPENSIONS

When both contributions to steric stabilization are considered together, it turns out that in the case of a good solvent, steric interactions are always strongly repulsive. In the case of bad solvents, instead, attractive interactions dominate initially, but when the distance between the particle surface is further reduced, repulsion due to elastic compression eventually prevails.

94 Chapter 7 Kinetics and Structure of Colloidal Aggregates

7.1 Diffusion Limited Cluster Aggregation – DLCA

7.1.1 Aggregation Rate Constant – DLCA

In the case where no repulsive barrier exists between the particles, i.e., VT(D) is a monotonously increasing function with no maximum, the rate of particle aggregation is entirely controlled by Brownian motion. Let us compute the ﬂow rate F of particles aggregating on a single ref- erence particle. For this, we note that the ﬂow rate, F of identical particles diﬀusing through a sphere centered around a given particle, is given by:

dN F = 4πr2 D with N = N at r = ∞ (bulk) (7.1) 11 dr 0 where N is the particle concentration, r the sphere radius and D11 the mutual diﬀusion coeﬃ- cient, which since both colliding particles undergo Brownian motion is equal to twice the self diﬀusion coeﬃcient, i.e., D11 = 2D. At steady state, i.e., F = const., the particle concentration proﬁle is given by: F 1 N = N0 − (7.2) 4πD11 r If we now assume that upon contact the second particle disappears (because of coagulation), that is N = 0 at r = R11 where R11 = 2a is the collision radius, we have:

F = 4πD11R11N0 (7.3) which is the ﬂow rate of particles aggregating on the single particle under consideration. If we now consider only the beginning of the aggregation process, we can compute the rate of

95 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

N

N0

r

2a

0 decrease of the particle concentration in bulk due to the aggregation process, Ragg as follows:

1 1 1 R0 = − N F = − 4πDR N2 = − β N2 (7.4) agg 2 0 2 11 0 2 11 0 where the factor 1/2 is needed to count each event only once. In the above expression we have introduced the aggregation rate constant β11 = 4πD11R11, which plays the same role as the reaction rate constant in a second order kinetics. In the case of two particles of equal size, a this reduces to:

β11 = 16πDa (7.5) and using the Stokes-Einstein equation to compute D = kT/(6πηa), where η is the dynamic viscosity of the medium, we obtain:

8 kT β = (7.6) 11 3 η which is size independent. In the case of two particles of diﬀerent radius, Ri and R j, we have:

βi j = 4π Di + D j Ri + R j ! 2 kT 1 1 = Ri + R j + (7.7) 3 η Ri R j

It is interesting to investigate the behavior of the aggregation rate constants for particles of diﬀerent sizes.

96 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

β a a i j i j 4πDa

a a 4 ⇒ β is size independent 1 2 a · 3 a a/2 a + a a + 2 = 3 2 = 4.5 1 4 a · 5 a a/4 a + a a + 4 = 5 4 = 6.25 1 n a (n+1) (n+1)2 a a/n a + a a + n = (n + 1) n = n (n+1)2 limn→∞ n = ∞

From the values in the table above it is seen that small/large collisions are more eﬀective than small/small or large/large ones.

7.1.2 Cluster Mass Distribution – DLCA

In order to derive the Cluster Mass Distribution (CMD) of the aggregates containing k primary particles (or of mass k) we need to consider the following population balance equation, also referred to as Smoluchowski equation:

dN 1 Xk−1 X∞ k = β N N − N β N (7.8) dt 2 i,k−i i k−i k ik i i=1 i=1 where Nk is the number concentration of aggregates of size k, and the ﬁrst term on the r.h.s. rep- resents all possible collisions leading to the formation of an aggregate of mass k, while the second is the rate of disappearance of the aggregates of mass k due to aggregation with ag- gregates of any mass. If we now assume that the aggregation rate constant is constant with size, i.e., βi j = β11 and we sum both sides of the equation above to compute the total aggregate concentration of any mass, that is X∞ N = Nk (7.9) k=1 we obtain: dN 1 1 = β N2 − β N2 = − β N2 (7.10) dt 2 11 11 2 11 which integrated with the I.C.: N(t = 0) = N0 leads to: 1 1 1 = + β11t (7.11) N N0 2

97 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

If we deﬁne the characteristic time of coagulation or of rapid coagulation, tRC the time needed to half the initial value of aggregates we have:

2 1 tRC = = (7.12) β11N0 2πD11R11N0 which for particles of equal size reduces to:

3η 2 × 1011 tRC = ≈ [s] (7.13) 4kT N0 N0 where a water suspension at room temperature has been considered in the latter equation, −3 with N0 in cm . As an example, for concentrated colloids of a few percent in solid volume, 14 −3 N0 = 2 × 10 cm the tRC is in the range of milliseconds. The CMD computed from the Smoluchowski equation is given by:

k−1 N0 (t/τ) Nk = (7.14) (1 + t/τ)k+1 where time has been made dimensionless using the rapid coagulation time, i.e., τ = tRC.

7.1.3 Role of Aggregate Morphology – DLCA

In order to solve the Smoluchowski equation in the general case where the aggregation rate constant is size dependent, that is: ! 2 kT 1 1 βi j = Ri + R j + (7.15) 3 η Ri R j

98 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

we need to correlate βi j directly to the masses i and j of the two colloiding clusters. Accord- ingly, we need to derive a relation between the size Ri of an aggregate and its mass i, that is to say something about the structure of the aggregate. If we consider a solid sphere this relation is simple: 4 i = ρ πR3 , ρ = density (7.16) 3 i which reported on a log-log plot leads to a straight line with slope 1/3. This expression can be used in the case of coalescence, where smaller droplets (e.g. of a liquid) aggregate to form a larger drop. In this case, by substituting it in the above equation we get the following expression for the coalescence rate constant: 2 kT β = i1/3 + j1/3 i−1/3 + j−1/3 (7.17) i j 3 η

Using Monte Carlo simulations and light scattering measurements it has been shown that a similar straight line is obtained also for the polymer aggregates if we deﬁne as aggregate size,

Ri the radius of the smallest sphere enveloping the entire cluster. This is the size that we have tacitely used above in computing the self diﬀusion coeﬃcient of the fractal using Stokes- Einstein equation. The diﬀerence with respect to the solid sphere is that in this case the slope of the straight line is much larger due to the many voids present in the fractal structure, and equal to 1/df, where df is deﬁned as the fractal dimension.

99 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

ln Ri

1/df

1/3

ln i

Ri

In typical applications df ranges from 1.5 to 3.0. If we now accept that our aggregates have a fractal structure, then we use the following scaling of their size with mass

1/df Ri ∝ i (7.18) which leads to the following expression for the aggregation rate constant: 2 kT β = i1/df + j1/df i−1/df + j−1/df (7.19) i j 3 η which can be used to solve numerically the Smoluchowski equation in diﬀusion limited con- ditions.

7.2 Reaction Limited Cluster Aggregation – RLCA

7.2.1 Aggregation Rate Constant – RLCA

In the case where a repulsive energy barrier is present between particles, i.e., VT(D) exhibits a maximum value, then the aggregation process becomes slower than the diﬀusion limited described above and becomes controlled by the presence of the interparticle potential. This is often referred to as reaction limited cluster aggregation, RLCA. In this case, in computing the particle ﬂow rate, F entering a sphere of radius, r centered on a given particle, we have

100 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES to consider not only the particle concentration gradient, i.e., brownian diﬀusion, but also the potential gradient. The particules are diﬀusing toward each other while interacting in the potential ﬁeld VT(r) whose gradient is producing a force: dV F = − T (7.20) T dr which is contrasted by the friction force given by Stokes law, Ff = Bu, where B = 6πηa represents the friction coeﬃcient for a sphere of radius, a in a medium with dynamic viscosity, η. The two forces equilibrate each other once the particle reaches the relative terminal velocity, ud so that FT = Ff. This implies a convective ﬂux of particles given by: N dV J = u N = − T (7.21) c d B dr which superimposes to the diﬀusion ﬂux: dN J = −(D ) (7.22) d 11 dr

where D11 is the mutual diﬀusion coeﬃcient of the particles. The ﬂow rate of particles aggregating on one single particle, F, which at steady state conditions is constant, is given by: ! dN N dV F = − 4πr2 (J + J ) = 4πr2 D + T (7.23) c d 11 dr kT dr where using the Stokes-Einstein equation the friction factor can be represented in terms of the diﬀusion coeﬃcient by B = kT/D11. Using the B.C.: VT = 0, N = N0 at r → ∞, and N VT VT dN/dr + kT dVT/dr = exp − kT d N exp kT /dr, this equation can be integrated leading to: V F exp (−V /kT) Z ∞ V dr N N − T T T = 0 exp + exp 2 (7.24) kT 4πD11 r kT r from which, considering N = 0 at r = 2a and D11=2D, we compute:

8πDN0 F = −R ∞ (7.25) exp (V /kT) dr/r2 2a T

Note that for VT = 0 we obtain F = 8πDN0(2a), which is the same value computed earlier for diﬀusion limited aggregation. Considering the deﬁnition of aggregation rate constant, β = F/N, we can conclude that FDLCA/F = βDLCA/β. This is a very important parameter in colloidal science and is usually referred to as the Fuchs or stability ratio, W deﬁned as: βDLCA Z ∞ V dr W a T = = 2 exp 2 (7.26) β 2a kT r

101 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

which gives the value of the ratio between the rates of rapid (diﬀusion limited) and slow 2 (reaction limited) aggregation. By looking at the function (a/r) exp [VT/(kT)] shown in the ﬁgure above, it is apparent that the value of its integral can be related to the value of only the maximum value of VT, i.e., VT,max. In particular, the following approximate equation for W has been derived: ! 1 V W ≈ exp T,max (7.27) 2κa kT where 1/κ is the thickness of the diﬀusive layer as deﬁned in section 6.2.2. Using this relation we can compute the W values corresponding to typical values of VT,max in applications. From this we can compute the corresponding half coagulation time t1/2 = 2/ (β11N0) following the DLCA same procedure used in section 7.1.2 to compute tRC = 2/ β11 N0 . Considering again the 14 −3 case where N0 = 2 · 10 cm we obtain the results reported in the following table:

VT,max ≤ 0 15kT 25kT W 1 105 109 −3 2 6 t1/2 [s] tRC = 10 10 10

These clearly indicate the meaning of kinetic stabilization, since with a modest energy barrier the coagulation process can be delayed from milliseconds to days or months. Note that the value of W tends to be very sensitive to even small changes of the surface charge or potential. In particular, in these conditions we have that a ten-fold variation of W is obtained with an about 15% change in VT,max and a 7% change in the surface potential, ψ0. This makes it unfeasible to compute W from measurements of ψ0, while it is recommended to measure it

102 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

from direct measurements of the kinetics of particle aggregation, i.e., β11. It can be shown that the relation above for W leads to the plots shown below in the plane log W − log cE, where cE is the concentration of an electrolyte. The region where W > 1 has a negative slope, which depends upon the valency of the electrolyte, and is well conﬁrmed by the experimental value. This loss of stability is due to the double layer compression eﬀect, which appears in the above equation through the eﬀect of the ionic strength on the Debye-Huckel¨ parameter, κ.

The second region corresponds to diﬀusion control, which is unaﬀected by the presence of an electrolyte, i.e., W = 1. The intersection of the two straight lines indicates the ccc, where the energy barrier vanishes.

7.2.2 Role of Cluster Morphology – RLCA

We have seen that in the case of primary particles under RLCA conditions the aggregation rate constant is given by: βDLCA β = 11 (7.28) 11 W We now need to extend this to the aggregation of two clusters of size i and j, respectively. One way to consider this problem is to assume that the aggregation of the two clusters occurs through the interaction between the two primary particles, on each aggregate, which ﬁrst come into contact. This has two relevant consequences:

1. The aggregate-aggregate interaction can be approximated with the interaction between the two colloiding primary particles, which is described by the stability ratio W. The interactions with the other particles can be assumed to be too short range to be relevant.

103 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

2. The rate of aggregation depends upon the probability of collision between the primary particles on the cluster surface, which means the probability of having a primary particle on the external surface of a cluster.

cluster j cluster i

For a given cluster k, the change in the number of primary particles in the cluster with its size, ak, is given by: df df −1 ak dk df ak df k = ⇒ = = k(df −1)/df (7.29) a dak a a a If we multiply this by the primary particle radius, a we get the number of primary particles added on the last layer of the aggregate:

dk (df −1)/df a = dfk (7.30) dak

This means that the aggregation rate constant should be augmented by a factor k(df −1)/df when we consider the probability of collision of the primary particles instead of that of collision of the clusters. With this result we can derive the ﬁnal expression for the aggregation rate constant in RLCA conditions: DLCA βi j β = (i j)λ (7.31) i j W where λ = (df − 1) /df, which for df ≈ 2 leads to λ ≈ 0.5, which has received some experi- mental validation. Upon collision the aggregates formed in RLCA conditions have time to probe many possible conﬁgurations for an aggregation event. Due to this, the resulting aggregates are denser than their counterparts in DLCA, and can also penetrate deeper into each other without immediately aggregating. This results in aggregates which are generally denser with fractal dimensions of about 2.1.

104 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

7.2.3 Cluster Mass Distribution – RLCA

In RLCA detailed calculations of the CMD using equation 7.8 with the aggregation rate con- stant shown in equation 7.31 can only be obtained from numerical solutions to the PBE. How- ever, for many aggregation problems in non-sheared colloidal dispersions it has been found that the resulting CMD exhibits some general features. Therefore it is possible to develop scaling solutions of the PBE, which are often suﬃcient for approximate purposes. A general form of the solution for a wide range of aggregation rate constants is given by

−τ Nk (t) = Ak exp (−k/kc) , (7.32) where A is a normalization constant determined from the conservation of total mass in the system and is given by N kτ−2 A = 0 c (7.33) Γ(2 − τ) where Γ(x) is the gamma function. kc is the time dependent cutoﬀ-mass of the distribution which grows with time and determines the kinetics. In RLCA, this growth is exponential, as kc(t) = p exp(t/t0), where t0 is a sample dependent time constant. τ is a power-law exponent of the CMD describing the shape of the CMD. In RLCA τ = 1.5 has been found to be a reasonable value.

7.3 Comparison of Aggregation Regimes – DLCA vs. RLCA

7.3.1 Aggregation Rate Constant – DLCA vs. RLCA

We now compare the aggregation rate constants of the two aggregation regimes, DLCA and RLCA. The general kernel valid for the two regimes can be written as

DLCA −1 βi j = β11 W Bi jPi j with DLCA β11 = 8kT/(3η) DLCA β11 W = (7.34) β11 1 B = i−1/df + j−1/df i1/df + j1/df i j 4 λ Pi j = (i j) , with λ = 0 in DLCA and λ ∼ 0.5 in RLCA,

105 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

Most important for the aggregation kinetics is the aggregation rate of equal sized aggregates

βii as a function of aggregate mass i. Therefore the parameter λ is extremely important for the kinetics as it dominates this function, as is displayed below.

In DLCA, as discussed before, W ≈ 1 and λ = 0. On the other hand, in RLCA W is large and λ ≈ 0.5, therefore exhibiting a strong mass dependence of βi j. In summary, in DLCA the aggregation of big with small aggregates is favored and the aggregation rate of equal sized aggregates is independent of the aggregate mass, whereas in RLCA big clusters preferably aggregate with big ones such that the aggregation rate of equal sized aggregates strongly in- creases with the aggregate mass. This is reﬂected by the aggregation rate constant values βi j, shown in ﬁgure 7.1 as a function of the aggregate masses i and j in ﬁgure 7.1 for the aggrega- tion regimes DLCA and RLCA.

7.3.2 Cluster Mass Distribution – DLCA vs. RLCA

The mathematical formulation of the cluster mass distributions in DLCA and RLCA has been presented above. The equations were for DLCA

k−1 N0 (t/τ) Nk = (7.35) (1 + t/τ)k+1 and for RLCA N kτ−2 N (t) = 0 c k−τ exp (−k/k ) , (7.36) k Γ(2 − τ) c The last equation can be shown to give identical results to the CMD for DLCA (equation 7.35) if τ = 0 is chosen. The diﬀerent shapes of CMD that are obtained during the aggregation

106 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

(a) −15 10

−16 ij 10 β

−17 10 4 10 3 10 2 2 10 10 1 10 0 0 j 10 10 i

(b) −18 10

−20 10 ij β −22 10

−24 10 4 10 3 10 2 2 10 10 1 10 0 0 j 10 10 i

Figure 7.1: (a) DLCA; (b) RLCA

process are plotted in ﬁgure 7.2. There we see that the distribution for DLCA is ﬂat when computed with the constant kernel (equation 7.35) or the scaling solution with τ = 0. When using the full DLCA kernel, a bell-shaped CMD is obtained. It is seen that as time is passing by the CMD moves towards larger sizes and its area decreases, as a consequence of the increase in size and decrease in number of the aggregates. After a short transient time, the CMD exhibits the typical self-preserving behaviour due to the fact that the rear of the distribution moves at the same speed as the front. Typical RLCA distributions are shown in ﬁgure 7.3 where we compare a scaling solution with τ = 1.5 and the full numerical solution using the RLCA kernel in equation 7.34. Obviously, in this case the scaling solution is a very powerful tool to obtain good estimates of the CMD without going through the procedure of numerically solving the PBE. In the case of RLCA,

107 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

1015

3

1010

105

number density / 1/m

100 100 102 104 106 108 dimensionless aggregate mass / -

Figure 7.2: The CMDs computed with the DLCA kernel. Constant, not size dependent kernel (dashed line) and full size dependent ”fractal” kernel (solid line).

15

3 10

1010

105

number density / 1/m 100 100 102 104 106 108 dimensionless aggregate mass / -

Figure 7.3: Cluster mass distribution (CMD) computed using the aggregation kernel is Eq. (7.34) for RLCA with W = 2.8×104 (continuous lines). The scaling solution for RLCA in Eq. (7.36) with τ = 1.5 is also plotted for comparison (×).

the time evolution of the CMD exhibits a fundamental diﬀerence with respect to DLCA. Since large-large aggregations dominate in this case, the CMD becomes wider in time, and actually

108 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES primary particles remain present in the system up to large aggregation times. The CMD does not exhibit the typical bell shape which causes often problems in the technology.

7.3.3 Aggregate Morphology – DLCA vs. RLCA

We have seen that the kernel and the CMD in the two regimes are rather diﬀerent. This is also apparent in the aggregate structure that often can be described by the aforementioned fractal dimension df. There are several ways to measure the fractal dimension, either by sedimenta- tion experiments, light scattering or image analysis. Such direct images can be obtained, for example, by transmission electron microscopy (TEM) and one example is shown in the picture below. Aggregates of diﬀerent materials and from computer simulations (the lowest set) are

Figure 7.4: left panel: DLCA; right panel: RLCA shown in ﬁgure 7.4 for the two regimes, DLCA and RLCA. Obviously, the clusters for DLCA are much more tenuous and open than the ones formed in RLCA. In summary, the fractal dimensions for each of the regimes are

109 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

Fractal relation: R ∼ i1/df

Regime Fractal dimension df

DLCA 1.6 − 1.9 RLCA 2.0 − 2.2

7.3.4 Comparison to Experimental Data

As has been shown in the TEM images in the previous section the agreement between ex- perimental images and those generated from computer models are very satisfactory and sup- port the fractal concept. However, direct comparison between the CMD computed with the Smoluchowski or PBE equations and experimental data is not straightforward, because direct experimental measurements of the CMD are not or hardly possible. Therefore light scattering techniques are often used, where averages (certain moments of the distribution) are measured. These moments can, with the proper theory, be computed from the CMD and compared to experimental data. This allows to validate the aggregation models presented in this chapter. In ﬁgure 7.5 we show two examples of such validation, one for each of the two aggregation regimes. The lines are model calculations and points are the experiments data.

3 3 10 10 ) / nm ) / nm θ θ ( ( 〉 〉 2 10 2 h,eff 10h,eff R R 〈 〈

1 10 1 10 −1 0 1 2 0 2 4 6 8 10 10 time / min 10 10 time / hr

Figure 7.5: Left panel: DLCA regime, comparing the real time evolution of the experimen- tal light scattering data and the model calculations. Right panel: RLCA regime, comparing experimental data and model calculations.

A further experimental support to the models discussed above can be obtained by making

110 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES the PBE (Eq. 7.8) dimensionless using the following deﬁnition for the dimensionless concen- tration of the clusters of mass k and the dimensionless time:

Nk φk = (7.37) N0 t τ = N βDLCA (7.38) 0 11 W

DLCA where N0 is the initial number of primary particles, W the Fuchs stability ratio and β11 the primary particle aggregation rate constant in DLCA conditions as deﬁned by equation 7.34. Thus, the following dimensionless PBE is obtained from equations 7.8 and 7.34.

dφ 1 Xk−1 X∞ k = B P φ φ − φ B P φ (7.39) dτ 2 i,k−i i,k−i i k−i k i,k i,k i i=1 i=1

with initial conditions: φ0 = 1, φk = 0 for k ≥ 0 . It is remarkable that in this form, the PBEs depend only on two parameters: the fractal di- mension d f and the parameter λ in equation 7.34. Since these two parameters do not depend on many physical parameters such as ionic strength or primary particle concentration, the above equation can be regarded as a master equation describing some kind of universal behavior of aggregating systems under DLCA and RLCA conditions. Some experimental veriﬁcation of these conclusions are reported in ﬁgure 7.6.

7.4 Cluster Coalescence

Let us consider the case where the particles constituting a cluster can coalesce by polymer interdiﬀusion, as it is the case for polymers close or above their glass transition temperature. Figure 7.7 shows cryo-SEM images of elastomer clusters for two limiting cases. If the coalescence process is fast with respect to aggregation, i.e., the characteristic time for par- ticle fusion is much smaller than the characteristic aggregation time, τfus τagg (e.g., with τfus ∝ ηR1/γ, and τagg ∝ 1/ β1,1N0 ), the newly formed clusters relax to spherical geometry (Figure 7.7a) before being involved in the next aggregation event. On the other hand, if the coalescence process is very slow compared to aggregation, i.e., τfus τagg, coalescence is suppressed and ramiﬁed, fractal clusters are prevailing (Figure 7.7b). The inﬂuence of the cluster structure on the aggregation kinetics can be well demonstrated DLCA under DLCA conditions where the aggregation kernel, βi j , has only one free parameter,

111 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

500

PS, Rp=33 nm

400 ) / nm o

,90 R o g 300 =30 θ ( 〉 Rh (30°) 200 h,eff R 〈 , 〉

g 100 R 〈 Rh (90°)

0 0 2 4 6 8 10 τ / − D E Figure 7.6: Average gyration and hydrodynamic radii, Rg and hRhi , as a function of the di- mensionless time, τ , computed from PBE simulations (curves), compared with experimental data, where diﬀerent symbols indicate data from diﬀerent salt con- centrations and particle volume fractions.

(a) (b)

1 µm

1 µm 1 µm

Figure 7.7: Cryo-SEM images of the clusters formed by (a) soft and (b) rigid elastomer latex particles in DLCA at 25 ◦C.

the fractal dimension df. In particulary, we can use the result (not shown) that in DLCA the average particle size or radius scales with time as:

hRi ∝ t1/df (7.40)

Accordingly, when we measure for example the average hydrodynamic radius hRhi for an aggregating system, we can use the scaling at large times to extract information about the

112 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES cluster structure. As shown in Figure 7.8, for fully coalescing clusters the time evolution 1/3 of hRhi follows hRhi ∝ t , which is clear from the spherical shape, i.e., df = 3.0. On the 1/1.7 other hand, for the cluster growth of rigid particles the scaling is: hRhi ∝ t , i.e., df = 1.7, as typical for fractal clusters grown in DLCA. It is worth noting that the dimensionless scaling of experimental data obtained under diﬀerent conditions (e.g., temperature, particle concentration, or coagulant type) leads to unique master-curves characterized in their scaling by the df value, as can be taken from Figure 7.8.

Figure 7.8: Dimensionless scaling of the average hydrodynamic radius hRhi with time under DLCA conditions. Circles are experimental data of coalescing clusters where df = 3.0. Squares are experimental data of fractal clusters latices with df = 1.7. Solid curves are the corresponding simulation results.

Cluster coalescence and colloidal interaction. In contrast to DLCA, where particle repul- sion is completely screened, under RLCA conditions the fate of surface charges during coa- lescence is important for the aggregation kinetics. To account for partial repulsion of spherical clusters of diﬀerent sizes i and j, one can use the following PBE kernel:

1/3 1/3 −1/3 −1/3 2kT i + j i + j βi, j = (7.41) 3η Wi, j where the fractal dimension is ﬁxed because of the spherical cluster shape, i.e., df = 3.0. In addition, the colloidal stability is not anymore determined by the interaction of primary par- ticles as in the case of non coalescing aggregates. The reason is that upon the coalescence

113 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES process on one hand the total polymer surface decreases, thus leading to more stable disper- sions, but on the other hand some of the surface changes may be entrapped inside the newly formed particles thus having a destabilizing eﬀect. Using a simple particle sintering model, we can envision the coalescence process in Fig- ure 7.9 as given by a ﬁrst deformation of the two attached spheres at the point of contact (a), leading to a circular region (b) where a surface area of 2πy2 is lost. All surface charges lo- cated in this region are entrapped. Next, the process proceeds to the ﬁnal spherical geometry (c) where charge redistribution without further entrapment takes place.

Figure 7.9: Schematic shape evolution of a coalescing doublet.

In this model we can take the neck radius, y to characterize the extent of particle fusion and then the number of charged sites left at the end of the coalescence process. For example, in the case of two coalescing primary particles with radius R1, the neck radius y is constrained 1/3 between zero and R2 (= 2 R1). Thus, for a given y value, the balance of initial, lost, and re- maining surface charges returns the value of the surface charge density σs,2 after full doublet coalescence. This calculation can be easily extended to the coalescence of any equal sized clusters with radius Ri/2 and ﬁnal radius Ri (i ≥ 2). The obtained results are shown in Fig- ure 7.10a (open circles) in terms of the relative surface charge density, σs,i/σs,1, as a function of the resulting cluster mass i. The solid line represents a power-law ﬁt to these data, i.e., n σs,i/σs,1 = i , where n is an adjustable parameter that depends on the y value. The only pos- sibility to estimate y and n is by ﬁtting experimental coalescence data such as those shown in

Figure 7.10b. With the obtained y = 1.005Ri/2, it is seen from Figure 7.10a that as clusters increase in size i their surface charge density σs,i decreases due to the charge entrapment dur- ing coalescence. However, we ﬁnd that at least in this case Wi, j is nevertheless increasing with cluster size (due to the increase of the particle size), which causes the slow down in the hRhi and hRgi time evolutions, shown in Figure 7.10b, if we compare the RLCA to the DLCA data

114 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

Figure 7.10: (a) Relative surface charge density of clusters of mass i, σs,i/σs,1. Discrete val- ues (circles) are calculated assuming entrapment of ﬁxed charges from the area 2 2πy whith y = 1.005Ri/2 (i = 2, 4, 8, 16, etc.). The solid line is a power-law ﬁt, −0.0865 σs,i/σs,1 = i , to predict σs,i for clusters of arbitrary size. (b) Dimensionless time evolutions of average hydrodynamic and gyration radii, hRhi (ﬁlled symbols) and hRgi (open symbols), in RLCA for three diﬀerent coag- ulant concentrations (ionic strength). Solid and broken curves are results of the respective PBE simulations.

(see Figure 7.8 for comparison). A further feature of the RLCA–coalescence process as shown in ﬁgure 7.10b is that not all the experimental data collapse onto master-curves for hRhi and hRgi as we discussed in section 7.3.4 for non-calescing systems. This is, despite having equal charge loss, i.e., using the same value of y, because of the diﬀerent evolution of Wi, j with ionic strength for the three diﬀerent coagulant concentrations used in the experiments. Let us compare the case of coalescing elastomer clusters having ﬁxed surface charges dis- cussed above to the case of mobile charges. This is for example the case of ionic surfactants that are typically only physically adsorbed on the particle surface. In this case the charged groups are squeezed out from the neck region during particle fusion and they relocate accord- ing to their adsorption equilibrium. Thus, assuming that no charge is entrapped, the surface charge density σs becomes a function of the available colloidal surface S , i.e., σs(S ). If the ad- sorption equilibrium of the surfactant is known, one can compute σs from the actual colloidal surface given by the CMD at time t. For the experimental system considered in Figure 7.11a, it is shown that the charge density increases as the particle surface decreases during aggregation and cluster coalescence. Accordingly, the colloidal interactions, change in time and in partic- ular the stability ratio Wi j increases during aggregation. Figure 7.11b shows the time evolution

115 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

Figure 7.11: (a) Relative surface charge density σs/σs,0 as a function of the available colloidal surface, S/S 0. (b) Dimensionless time evolutions of average hydrodynamic and gyration radii, hRhi (ﬁlled symbols) and hRgi (open symbols), in RLCA for three diﬀerent coag- ulant concentrations (ionic strengths). Solid and broken curves are results of the respective PBE simulations.

of the average cluster sizes of three colloidal systems under these conditions. It is seen that the process is much slower, particularly when compared to the case of ﬁxed charges shown in ﬁgure 7.10. Finally note that again the experimental data do not collapse onto master-curves, manifesting that RLCA under coalescence conditions is a non-universal process. In the case of the mobile surfactant charges, their relocation depends on the dissociation state of the ionic groups and therefore on the ionic strength of the solution, which is diﬀerent for the three coagulant concentrations employed in ﬁgure 7.11.

7.5 Solid Suspensions under Shear

7.5.1 Shear induced Aggregation

In all previous chapters we considered the aggregation kinetics of colloidal suspensions in stagnant conditions, where particle collisions are driven by Brownian motions, i.e., Brownian- induced aggregation. This is relevant in many applications such as the estimation of the shelf stability of a solid dispersion. However, in most industrial processes suspensions are subject to stirring and then the aggregation process is driven by the velocity gradient induced in the suspension by the stirrer. This is referred to as shear-induced aggregation and it is discussed

116 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES in the following.

Purely shear-induced aggregation kinetics

2(RRij )cos y

vx Gy

Rj

dy yR=( R )sin ij

Ri x

Figure 7.12: Schematic of the geometry of the problem for purely shear-induced aggregation.

We consider the stationary test particle, of radius Ri , located at the origin of the Cartesian frame, and a particle of radius R j moving toward the test particle along the streamline of the shear ﬂow, x. From the geometry of the problem, schematically depicted in ﬁgure 7.13 below, it is evident that the two particles can collide and aggregate only if the relative distance between the two particles centers is y ≤ Ri + R j which implies that the y-axis coordinate of the center of the second particle must be y ≤ Ri + R j sin θ. The velocity of the second particle along the x direction be denoted by vx = Gy , where G is the constant shear-rate. If we denote by n j the number of particles j per unit volume, the number of particles j that enter the element of collision surface in the upper-left quadrant per unit time is given by: h i 2 Ri + R j cos θ Gyn jdy (7.42) Given the symmetry of the problem, an equal number of collisions arises in the lower- right quadrant. Introducing a factor two and the number concentration of test particles, ni and integrating over the spatial coordinate, gives the total number of collisions with the test particle per unit time and per unit volume:

Z Ri+R j h i 4 Ri + R j cos θ Gynin jdy (7.43) 0 Substituting for y and changing the integration coordinate to θ leads to :

Z π/2 3 2 4nin j Ri + R j G cos θ sin θdθ (7.44) 0

117 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

from which the collision frequency per unit volume follows as:

32R3G β = (7.45) 11 3 This result, which was derived for the ﬁrst time by M. von Smoluchowski in the eventful year 1917, shows that the rate of shear-induced aggregation is proportional to the shear rate and to third power of the sum of the particle radii. This strong dependence on the particle size is what renders shear aggregation faster than Brownian aggregation for suﬃciently large particles.

The above β11 expression is valid under laminar conditions, seldom encountered in indus- trial units that typically operate under turbulent conditions. In the presence of turbulence, such dependency is still valid, provided that G is replaced by an average shear rate that can be cal- culated from the average energy dissipation rate of the turbulent ﬂow, . This approximation is valid in the case where the aggregates are smaller than the Kolmogorof vortexes, within which the laminar ﬂow prevails with shear equal to G = (/ν)0.5 , where ν is the kinematic viscosity of the disperse medium.

Generalization to DLVO-interacting Brownian particles in shear ﬂow

The Smoluchowski result for purely shear-induced aggregation kinetics is valid under the restrictive hypotheses that the particles are non-Brownian and non-interacting. The latter hy- pothesis means that the particles are treated as hard spheres which stick upon collision. The shear-induced aggregation kinetics of Brownian particles which do interact (typically with a superposition of van der Waals attraction and electric double layer repulsion) is a more com- plicated problem. The interplay between shear and interactions in this case gives rise to an interesting phenomenology: a colloidal suspension which is completely stable under stagnant conditions (owing to charge-stabilization) can be made to aggregate under the imposition of shear ﬂow, with the result that the rheological properties of the suspension may change dramat- ically. A typical situation is depicted in the Figure below, where, after a lag-time or induction period within which it remains constant, the viscosity suddenly undergoes a very sharp upturn and eventually results in the overload of the shearing device, and the system turns into solid- like upon cessation of ﬂow. Furthermore, the duration of the lag-time correlates exponentially with the applied shear-rate, in the sense that the lag-time before the viscosity upturn decreases exponentially upon increasing the shear rate. The diﬃculty of treating this general case is related to the mathematical complexity of the

118 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

8 -1 6 7 1: 1600 s 4 5 1 2 3 (c) 2: 1700 s-1 -1 -1 3: 1500 s 10 4: 1400 s-1 ] 5: 1300 s-1 6: 1200 s-1

Pa s -1

[ 7: 1100 s -1 8: 1000 s 10-2

10-3 0 5000 10000 15000 t [s]

Figure 7.13: Typical time-evolution of the suspension viscosity for charge-stabilized latex par- ticles in laminar shear ﬂow at a varying imposed shear-rate (see legend).

governing equation. This, in the presence of shear, is the convective diﬀusion equation with an interparticle interaction potential, U(r) , which reads: " # D ∇ (−∇U + bv) − D∇ c = 0 (7.46) kBT where b is the hydrodynamic drag acting on a particle, v is the particle velocity due to the ﬂow and c is the concentration of particles. This equation is a partial diﬀerential equation in three-dimensional space and cannot be solved analytically. Further problems are due to the ﬂow velocity term (linear in the radial distance r) which diverges at inﬁnity. However, since our problem is to determine the collision frequency, this equation can be reduced to an ordi- nary diﬀerential equation in the radial distance as the independent variable. The underlying simplifying assumption is that one neglects the spatial correlation between the concentration and velocity ﬁelds. Integration under the proper boundary conditions for the problem leads to the following generalized kinetic constant for aggregation :

16πD R β 0 11 = R δ/R R x h i (7.47) 2 dx exp( dx d(U/k T)/dx + Pev˜ ) 0 ℘(x)(x+2)2 δ/R B r,e f f

where x is the surface-to-surface radial distance between the particles,v ˜r,e f f is the relative velocity between two particles due to the ﬂow normalized by GR, Pe is the Peclet number (i.e. the ratio between the shear and the Brownian forces) and ℘(x) is a hydrodynamic function accounting for the resistance of the solvent being squeezed when the two particles approach each other. δ is the thickness of the hydrodynamic boundary-layer (a function of the Peclet

119 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES number and of the interaction range). This expression is still suﬃciently complicated, where the integrals need be evaluated numerically. A further simpliﬁcation can be done by consider- ing the limits of a high interaction potential barrier and moderate Peclet number. Under these conditions, the previous expression reduces to the following simple relationship:

q 00 β11 = Pe − (Um/kBT) exp (−Um/kBT + 2Pe/3π) (7.48)

00 where Um is the value of the interaction potential at the maximum of the barrier and Um is the second derivative evaluated at the maximum. Since the Peclet is proportional to the shear 3 rate (Pe = 3πµGR /kBT , where µ is the solvent viscosity,kB is Boltzmann’s constant, and T is the absolute temperature) this formula explains the observed exponential dependence of the lag-time preceding the viscosity upturn upon the shear-rate in terms of the attempt time (activation delay) for the shear-induced aggregation of particles with a potential barrier. The exponential scaling with the shear-rate predicted by this formula is in fairly good agreement with experimental observations.

105

4

10 Characteristic Characteristic aggregation time [s] time aggregation

103 800 1200 1600 -1 G[s ]

Figure 7.14: Characteristic aggregation time as a function of the applied shear-rate.

To better illustrate the physical meaning of the above expression the right panel of the following ﬁgure shows the aggregation rate constant, β11 as a function of the Peclet number Pe, for four values of the surface potential, ψs, which are typical for DLVO-interacting colloidal systems. It is seen that there are two regimes separated by the broken line: on the left hand side (small Pe values), the aggregation rate is very small and sensitive to the surface potential, while on the right hand side (large Pe values) it is substantially larger and practically independent

120 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES of the surface potential. This deﬁnes the critical Pe value separating Brownian- from shear- induced aggregation.

1E+50 Particle radius=282 nm -8 1E+00 Debye length=1×10 m =-30 mV Under shear 1E‐50 s

Energy 1E‐100 -40 mV Shear- barrier induced 1E‐150 -50 mV Interparticle distance 1E‐200 1E‐250 Interaction energy -60 mV Doublet formation Rate 1E‐300 1.0E‐41.0E‐2 1.0E+0 1.0E+2 1.0E+4 1.0E+6 Peclet Number, Pe

7.5.2 Shear induced Breakage

In the presence of strong shear rates, another phenomenon arises which is usually not present under stagnant conditions: cluster breakage. Fluid velocity gradients are not only capable of accelerating the rate of aggregation, but also to break clusters into two or more fragments and also to restructure them, i.e., to increase the primary particles packing density inside a cluster. Both phenomena are strongly coupled, since a more open cluster will be easier to break than a denser one. In addition, cluster breakage also depends on the strength of inter-particle bonds, on cluster size and on the shear rate. Up to know, no complete theory exist which is capable of fully capturing the details of breakage. A typical semi-empirical expression for the breakage rate constant of a cluster with mass i is the one proposed by Delichatsios and Probstein in 1976 and later modiﬁed by Kusters in 1991: ! 4 B βbreak G − i = exp 2 (7.49) 15π G Ri

Equation (7.49) shows that the rate of breakage increases as the shear rate increases (in a non linear fashion for small shear rates, linearly for large shear rates) and increases as the cluster size Ri increases following a sigmoidal trend. The constant B empirically accounts for all dependencies upon structure, material and particle-particle interactions. It is noteworthy that equation (7.49) is just one of the many available expressions proposed to model the rate of breakage, even though it is probably the most commonly used one.

121 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

One of the major diﬃculties related in the modelling of breakage events is that the rate of breakage is not the only piece of information required to construct a mathematical model for coagulation in the presence of shear. In fact, it is necessary to also know the distribution of fragments generated in a breakage event. Unfortunately, it is very diﬃcult to obtain the fragment distribution function both theoretically and experimentally. Usually, either simple binary breakage or fragmentation of a cluster into a speciﬁc number of equal size fragments are assumed. One signiﬁcant diﬀerence between a breakage event and an aggregation event is that break- age is a ﬁrst order kinetic process, i.e., the rate of breakage is proportional to the ﬁrst power to the cluster concentration, while all aggregation mechanisms discussed so far are second order kinetic processes, because they require the collision of two clusters. This implies that the formulation of population balance equations (PBE) changes substantially when breakage is present. The PBE (equation (7.8)) in the presence of shear can be formulated as follows:

dN 1 Xk−1 X∞ X∞ k = β N N − N β N − βbreakN + Γ βbreakN (7.50) dt 2 i,k−i i k−i k ik i k k k,i i i i=1 i=1 i=k+1 The last two terms of equation (7.50) provide the contribution due to breakage to the mass bal- ances. The second last term is a mass loss, due to the breakage of clusters with mass k, while the last term is a positive contribution due to formation of clusters with mass k generated by the fragmentation of all clusters with mass i > k. The function Γk,i is the fragment distribution function, which is deﬁned as the number of fragments with mass k generated by breaking a cluster with mass i.

7.6 Gelation of Colloidal Suspensions

7.6.1 The Gelation Process

During aggregation clusters continuously grow in size. Taking the radius of the smallest sphere enveloping the cluster of mass i as the cluster dimension, Ri, we can compute the cumulative volume fraction occupied by all clusters, as follows:

X 4 φ(t) = πR3N (7.51) 3 i i i

where Ni is the CMD, for example computed through the PBE (Eq. 7.8). As shown in ﬁg- ure 7.15, φ(t) increases in time reaching values larger than one. This indicates that the system

122 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES is becoming increasingly crowded, so that the clusters are not anymore able to diﬀuse ran- domly but begin to interact strongly with each other. The consequence is that the liquid-like colloidal dispersion can dynamically arrest or jam to form a solid-like gel, whose properties can be substantially diﬀerent from their original disperse state, leading to wide applications in many areas such as in producing ceramics, food, medicine, controlled porous materials, drug delivery devices, etc. In particular, during the diﬀusion-limited cluster aggregation (DLCA) and reaction-limited cluster aggregation (RLCA), the solid-like transition results from inter- connections of the fractal clusters when they grow and ﬁll the entire available space. This process, which transforms the original liquid dispersion in a solid-like gel, is referred to as gelation and can be conceptually divided in two steps:

• cluster formation: this is the aggregation process described by the PBE (Eq. 7.8) which continues until the so called arrest time, which is time where the clusters have occupied so much of the space that their movement is seriously hindered. At this point the cumu- lative volume fraction occupied by all clusters, φ(t) is of the order of unity. This time can be measured using dynamic light scattering technique;

• cluster interconnection: the substantially arrested clusters interact with each other form- ing a percolating structure which span the entire available volume. This process is com- pleted at the so called gelation time.

Ф

1 ume l vo

clusters

ve of

ti a l fractal clusters primary doublet 0 fraction particles formation clusters interconnection cumu Time (t)

Figure 7.15: Schematic overview on the gelation process

There are various methods to deﬁne the critical conditions (time, tc) for the gelation to occur. The simplest method is through visual observation, i.e., by tilting the aggregation system to see if it ceases ﬂowing. There are more rigorous methods based on measurements of variations in the system physicochemical properties. One of the most commonly used

123 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES methods is monitoring elastic modulus (G0) of the system, which is near zero in the liquid- like state and sharply increases when the clusters start to interconnect forming the solid-like gel. Another technique that can be well used to deﬁne the occurrence of gelation is cross- correlation dynamic light scattering, whose intensity indicates the transition of the system from ergodic (liquid-like) to non-ergodic (solid-like). The three methods mentioned above to deﬁne the critical gelation time (tc) are depicted in the following ﬁgure.

1E+5 Non‐ergodic 1E+4

1E+3

1E+2 G', Pa tc 1E+1 Arrest tc

1E+0 time 1E+1 1E+2 1E+3 1E+4 t, sec The sample ceases Sharp increase in elastic Transition from ergodic to flowing modulus non‐ergodic

Figure 7.16: Schematic overview on the gleation process

7.6.2 Brownian-Induced Gelation

When a colloidal system is fully or partially destabilized by adding electrolytes, the Brownian- induced aggregation (i.e., DLCA or RLCA) of the particles can lead to gelation if the initial particle volume fraction is large enough (e.g., φ > 0.01 ). Under DLCA conditions, once the system is in close vicinity to gelation, the interconnection process among the clusters is very fast, due to two main reasons: The ﬁrst is because every collision between particles and clusters results in a new cluster, i.e., the reactivity is independent of cluster size. The second arises due to the fact that the characteristic CMD of DLCA is rather monodisperse, and all clusters experience approximately the same environment and are on average separated by the same short distance. This view is conﬁrmed by experiments performed on polystyrene colloids, where the gelation time and the arrest time have been measured as a function of solid volume fraction, as shown in the following ﬁgure (left panel). It is seen from the ﬁgure that the gelation time and the arrest time basically overlap within the experimental error. It should be mentioned that from practical application viewpoint, gelation under DLCA

124 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

3 gelation time from non-ergodic 10 transition3D DLS: NE−transition arrest time from DLS gelation time from G’ gelation time from G’ Rheology: gelation time

2 10 time / min 1 10 Arrest time: DLS

0 10 0.012 0.013 0.014 0.015 0.016 0.017 0.018 salt concentration [NaCl] / mol/l DLCA gelation at different solid RLCA gelation at different salt volume fractions;Figure R 7.17:p=35 Schematic nm overview onconcentrations; the gleation process =0.05; Rp=40 nm

conditions is not the ﬁrst choice because the process is too fast to obtain homogeneous gels at large solid volume fractions. Instead, gelation under RLCA conditions is more commonly used (e.g. in food and ceramic industry), because the aggregation and gelation rate can be well tuned by the amount of salt added into the system. In this way, gelation can be carried out in a large range of solid volume fractions. In the above ﬁgure (right panel), the gelation time and the arrest time measured experimentally are shown as a function of salt concentration for polystyrene particles at a ﬁxed solid volume fraction. One can see that under RLCA conditions, the arrest time is substantially smaller than the gelation time. This is likely due to the broad CMD and diﬀerent reactivity of the clusters in RLCA. With the wide CMD, although a gel network would be formed by the ﬁrst few largest clusters, it is rather weak due to the small bonding number, and the system is still dominated by small clusters, which have low reactivity and thus need substantially long time to form a standing gel network.

7.6.3 Shear-Induced Gelation

To form a gel under DLCA and RLCA conditions, one needs to use electrolytes to screen the repulsive energy barrier and then destabilize the colloidal system. Using electrolytes may be undesired because they cannot be fully eliminated after gelation, leading to contamination of the ﬁnal products. Thus, without adding any electrolytes, one may impose a high shear stress to a colloidal system through ﬂuid motion to force the particle to overtake the energy barrier so as to aggregate and subsequently gelate. Recalling the characteristics of the shear aggrega-

125 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES tion process discussed in section 7.5.1 and in particular the dependence of the corresponding aggregation rate constant on the Pe number, we can conclude that once the imposed shear is high enough, leading to a Pe value in the shear-induced regime, the aggregation will be ex- tremely fast and independent of the DLVO interactions. This occurs for Pe values larger than the critical value leading to shear-induced aggregation. In practical applications, shear-induced gelation can be realized by forcing a colloidal sys- tem to pass through a microchannel (MC) without adding any electrolyte to screen the DLVO interactions. The left panel of the following ﬁgure shows an example of such a device where the capillary exhibits a z-shape with retention times in the order of tens of microseconds and pressure in the range of 20 to 120 bar. The intense shear is generated by forcing the col- loidal system to pass through the z-MC under pressure. In general, right after passing through the z-MC, the system can be either a Newtonian liquid or a viscous non-Newtonian liquid or solid-like gel, depending on how many clusters have been generated, which in turn depends on the shear rate, the particle volume fraction and size. One can speculate that if a suﬃcient amount of clusters is formed in the capillary, gelation occurs and at the MC outlet we have a solid gel having diameter similar to that of the connecting tube. If the conditions for gelation are not reached then the exiting liquid suspension is composed of two distinct classes of clus- ters: Class 1, constituted mainly of primary particles, and at most some dimers and trimers, and Class 2, constituted of large clusters (or gels) with sizes at least two orders of magnitude larger than that of the primary particles. It is remarkable that clusters with intermediate size are negligible. These two classes can in fact be easily isolated using a 5 µm-opening ﬁlter. Such a bimodal CMD is rather diﬀerent from the CMDs which are typically obtained under DLCA or RLCA conditions, and it is indeed diﬃcult to be explained on physical ground. On the other hand, when one thinks to the formation of macroscopic pieces of coagulum which is often observed in suspension/emulsion reactors and coagulators, this can certainly not be regarded as an academic curiosity. One possible explanation can be oﬀered by referring again to the critical transition from Brownian to shear induced aggregation (Pe is already above the critical Pe!). Since the Pe number depends upon the third power of the aggregate size, one can speculate that if in an otherwise stable suspension (i.e., under very slow Brownian aggregation) a very few doublets or triplets are formed (for whatever reason) they might enter the shear-induced aggregation regime and grow very fast, following some kind of runaway behavior, leading to the formation of macroscopic pieces of coagulum. In the case of the shear-induced aggregation in the MC, it is quite reasonable to expect that also breakage plays a role. As a matter of fact, since in general the Pe number is in the order of

126 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

103-104, we should expect the system to be always controlled by shear-induced aggregation. Whether a liquid-like or a solid-like system is obtained at the outlet of the MC should then be related to the competition between the shear generated in the MC and the strength of the aggregates. This is well represented by the Breakage number, Br deﬁned by:

3 3 µGRp µGRp Br = = (7.52) Umin hkBT 3 Which is the ratio between the shearing energy acting on a particle (µGRp ) and the inter- particle bonding energy (or the energy required to breakup a doublet bond) (hkBT, where h is a coeﬃcient, signiﬁcantly larger than unity, representing units of kBT between the primary minimum and the energy barrier on the interparticle interaction curve). This vision is conﬁrmed by a series of experiments where the critical conditions for the solid-like system (gel) formation have been measured using a z-MC unit for various values of the imposed shear, G and the primary particle radius, Rp. The obtained results expressed in terms of the eﬀective particle volume fraction, φg,e, are found to perfectly correlate with the Breakage number as shown in the right panel of the ﬁgure below. It is seen that the critical particle volume fraction φg,e for the shear-induced gelation to occur increases as Br increases. These values form a boundary separating the plane into two regimes: the solid-like gel above the boundary and the liquid-like state below.

As a ﬁnal remark we note that although the shear-induced gelation is signiﬁcantly diﬀerent from the Brownian-induced gelation, they share one feature: the clusters formed in the intense

127 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES shear ﬂow within the MC exhibit fractal scaling with fractal dimension equal to 2.4 ± 0.04, independent of Br, (i.e., of the shear stress, the particle size and the interparticle bonding energy). This is similar to the case of the Brownian-induced aggregations under DLCA and RLCA conditions, which lead to clusters with fractal dimension equal to 1.8 ± 0.05 and 2.1 ± 0.05, respectively, independent of the particle type and size and the electrolyte concentration.

7.7 Experimental Characterization of Colloidal Suspensions

7.7.1 Light Scattering

Scattering of light, x-rays, and neutrons is probably the most important experimental tech- nique used in the investigation of colloidal systems and aggregation phenomena, because it allows one to gain information about the size of particles and aggregates, the structure of ag- gregates and gels, and the kinetics of the aggregation process, in a non-invasive way. Of course several other experimental tools have also been used in the investigation of colloidal systems: microscopy (optical, electron, and X-ray) to study size and morphology; rheology to follow the gel formation and to investigate the mechanical properties of the gel phase; ultrasound spectroscopy to monitor particle size in on-line applications. In this chapter we will focus our discussion on light scattering, but most of the results could be almost immediately be applied to both neutrons and x-ray scattering. In order to better understand the features of light scattering, it is necessary to have an overview of the physical principles and the main results of scattering theory. Among the three sources: light, neutron and x-rays, light is the most used one for scattering experiments, due to the relatively low cost of lasers which are good quality monochromatic light sources and due to the development in detectors (photomultipliers and ﬁber optics) and computer-controlled correlators. Another advantage is that light scattering enables one to perform two diﬀerent kinds of measurements: dynamic light-scattering measurements and static light scattering measurements. In the following, we will brieﬂy review the main concepts of both kinds of measurements. It should be pointed out that most of the static light scattering theory can be also applied to neutron and x-rays scattering experiments. Light scattering is due to the interactions of electromagnetic waves with matter. When an incident electromagnetic wave shines on a molecule, the electrons feel the interaction and, as a results, the center of mass of the negative charges in the molecule is shifted from its original

128 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES position. Then, a dipole is formed, which oscillates with the same frequency as the incident radiation. One of the major results of the electromagnetic theory is that an oscillating dipole emits electromagnetic radiation in all directions. This radiation is the scattered radiation. When a sample is illuminated by an incident electromagnetic wave, the sum of the radiations scattered by all the elements of the sample constitute the scattered radiation. The intensity of the scattered light depends strongly on the optical contrast of the scattering object, which is the diﬀerence in refractive index between the object and the surrounding medium. Another way of understanding the scattering problem is the quantum mechanics perspective, where the incident radiation can be viewed as made of photons traveling in a given direction, and due to the collisions with atoms of the sample, these photons are deviated, or scattered, keeping however their frequency constant. According to this picture, multiple scattering cor- responds to the situation where photons are scattered more than once. Multiple scattering is likely to occur in system with a high concentration of material or in systems with a high optical contrast, when the probability of a photon to be scattered more than once is very high. The general treatment of light scattering is quite complex, especially for the most general case where multiple scattering is considered. It requires the full solution of Maxwell equations, which is feasible only for very simple geometries like spheres, cylinders, ellipsoids etc. This arises because the multiple scattering problem is a typical many-body problem: the scattering behavior of one part of the sample has an eﬀect on, and is aﬀected by, all the other parts of the sample. For complex, but always small, systems, where no analytical solutions of Maxwell equations is available, only heavy numerical methods can be used. Therefore, for most of the applications in the colloidal domain, the interpretation of scat- tering data is unfortunately limited to those conditions where multiple scattering is absent or can be safely neglected. From an experimental point of view, the conditions where multiple scattering can be neglected are those of low concentration and low optical contrast, where the number of incident photons scattered is a small fraction of the total. An alternative to lowering the concentration of scatterers is the so-called refractive index matching, i.e., ﬁnding a solvent that matches as much as possible the refractive index of the scatterer, so that a very low optical contrast can be obtained.

7.7.2 Static Light Scattering

The theory of scattering that neglects multiple scattering is called Rayleigh-Debye-Gans (RDG) theory. The basic assumption is that in every part of the sample, the radiation that illuminates

129 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES the sample is only the incident radiation. In this way, the scattering of every part of the system is independent of the others. The theory allows one to compute the proﬁle of the scattered in- tensity I as a function of the scattering angle Θ, deﬁned as the angle between the directions of the incident radiation and the measurement of the scattered radiation, as shown in next ﬁgure.

Incident radiation, I0

Scattering angle, θ

Scattered radiation, I(q)

The existence of an angular dependence of the scattered radiation is because waves scat- tered from diﬀerent parts of a sample have a diﬀerent phases, and that these phase diﬀerences become larger as the scattering angle Θ increases. In general, the modulus of the wave vector q of the scattered radiation, equal to the modulus of the diﬀerence between the propagation vectors of the scattered and incident radiation, is used instead of the angle θ:

4πn θ q = sin , (7.53) λ0 2 where λ0 is the wavelength of the radiation in vacuum and n is the refractive index of the solvent. It should be noted that the modulus of the wave vector q has the dimensions of the inverse of a length. Therefore, the quantity 1/q represents a length scale, and it gives an indication of the typical size of the objects that contribute to the scattering intensity at the given q value. A better illustration of the meaning of q may be given by an analogy between q and the magniﬁcation of a microscope. Looking at the intensity scattered by a sample at diﬀerent q values is analogous to observing the sample by changing the magniﬁcation. Low values of q correspond to low magniﬁcation, while large values of q correspond to large magniﬁcations and better resolutions. It is obvious from equation (7.53) that changing the scattering angle is not the only way to change the magnitude of q. One can also change the wavelength of the incident radiation. This is one of the reasons why other sources, x-rays and neutrons, are chosen to perform the scattering experiments.

130 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

X-rays are probably the ﬁrst source that has been used in the investigation of the structure of materials, particularly crystals. They have been chosen because of their very low wavelength that results in a high resolution. They are usually applied to investigate gels and surfactant solutions. X-rays scattering, particularly small angle x-rays scattering, allows to investigate systems over a broad range of length-scales. Neutron scattering is based on the scattering of neutrons on the nuclei of atoms. Since neutrons can have a high momentum, which is inversely proportional to their wavelength, neutron scattering also provides a very high resolution. Another advantage is that in the case where the system under investigation is an aqueous solution, the appropriate mixing of water and heavy water (D2O) enables the elimination of multiple scattering or to change the contrast in such a way that only some part of a sample can be studied. This method is called contrast variation technique. Static light scattering measurements are to determine the proﬁle of the scattered intensity as a function of the modulus of the wave vector q. To be more quantitative, we consider a sample made of N subunits, having all the same optical properties. In this case, the intensity of the scattered radiation is given by: I XN XN I(q) = 0 b (q)b∗ (q) exp −i q · R − R , (7.54) r2 j m j m j=1 m=1 where I0 is the intensity of the incident radiation, r is the distance of the sample from the detector (assumed to be much larger than the size of the sample), R j is the vector deﬁning the th position of the center of the j subunit with volume V j, i is the imaginary unit, the asterisk deﬁnes the complex conjugate, and the quantity b j(q), called scattering length, is deﬁned as follows: 2 2 2 Z πn np − n b (q) = exp −i q · r d3r , (7.55) j 2 2 j j λ0 n0 V j where np is refractive index of the material, n0 is the average refractive index of the dispersion

(material and dispersant) and r j is the vector deﬁning the coordinate of a point inside the th j subunit at a distance r j from its center of mass. It is important to notice that equation (7.54) is very general, and holds true not only for light scattering but also for neutron and x-rays scattering. The only diﬀerence for diﬀerent radiation sources is the dependence of the scattering length on the physical properties responsible for the scattering behavior of the system, namely the term multiplying the integral in equation (7.55). From equations (7.54) and (7.55) three very important features of intensity of scattered light can be recognized. First of all, the scattered intensity is proportional to the reverse

131 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES fourth power of the wavelength. This explains among others why the sky appears blue: the component of white sun’s light which is diﬀused more heavily by dust particles and water droplets is blue light (low wavelength). The second important feature is that the intensity of scattered light is proportional to the square of the volume of the object. Therefore, in the presence of a population of large and small particles, the amount of light scattered by large particles easily overwhelms that of small particles. The third feature is that the intensity of scattered light strongly depends on the optical contrast between the material and the medium around it. If the optical contrast is reduced to zero, the intensity of scattered light also goes to zero. Since equation (7.54) is quite complex, requiring the knowledge of the relative distances among the various subunits in the sample, it is useful to consider a special case of equation (7.54) that is very important for all colloidal applications. In particular, let us assume that all the subunits are equal and of spherical shape, then equation (7.54) takes the form:

2 I(q) = I0K1NVp P(q)S (q), (7.56) where Vp is the volume of one spherical particle, K1 is a constant that incorporates the de- pendence of equation (7.54) on the optical constants, P(q) is called particle form factor and depends on the geometrical shape and size of a particle, and S (q) is the structure factor, which depends on the correlations among the particles. In the case of spherical particles, the form factor P(q) is given by:

"3(sin(qR ) − qR cos(qR ))#2 P q p p p , ( ) = 3 (7.57) (qRp)

The form factor for a sphere is plotted in the next ﬁgure. This formula is correct usually for particles suﬃciently smaller than the wavelength of the radiation (about 10 times smaller), and with a low optical contrast. If the particles do not fulﬁll these requirements, the RGD theory cannot be applied to interpret the scattering proﬁle of particles. Instead, the full scattering theory, referred to as Mie theory, has to be used. From a Taylor expansion of the particle form factor, one can derive a very useful relation:

1 P(q) = 1 − q2R2 , (7.58) 3 g,p where Rg,p is the primary particle radius of gyration. Equation (7.58) suggests that, from the bending of the form factor, one can estimate the radius of gyration of an object. The radius of

132 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

gyration of an object is deﬁned as the sum of the squares of the distances of all his points from the center of mass: i 1X 2 R2 = r − r , (7.59) g,p i j cm j=1 For a continuous object, the sum in the above equation should be replaced by an integral. In √ the case of a sphere, Rg,p = 3/5Rp. The structure factor, S (q), on the other hand, contains information about the structure of the system, i.e., how the particles are arranged. The relation between the structure factor and relative positions of i spherical particles in the system is given by the following expression: i 1 X sin(qrm j) S (q) = , (7.60) i2 qr m, j=1 m j

th th where rm j is the distance between the centers of the m and the j particles. If the system is dilute enough that no correlations among the particles exist, i.e., the relative distances among the particles are much larger than 1/q, then S (q) = 1 and the scattering intensity depends only on the geometrical properties of the particles. The general procedure to obtain the structure factor of a system from static scattering mea- surements is as follows. One ﬁrst determines the particle form factor P(q) by performing the static scattering measurements for a dilute suspension of particles, where S (q) = 1 and the measured proﬁle is only proportional to the form factor. Then, by dividing the scattering proﬁle of the sample by the obtained form factor, the structure factor can be analyzed. Two kinds of information from the structure factor are crucial in the study of aggregation phenomena. In the case of a dilute suspension of large fractal aggregates, it can be shown that

133 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES the structure factor has typically a power-law behavior within a certain q-range:

S (q) ∼ q−df , (7.61)

so that from the slope of S (q) in a double logarithmic plane the cluster fractal dimension df can be extracted. The validity of this procedure will be subsequently discussed in the case of small clusters and in the case of gels. Another important quantity that can be determined from the scattering proﬁle is the radius of gyration. It can be obtained by using a Taylor expansion similar to what was done for a single particle. This procedure is called Zimm plot analysis:

1 P(q)S (q) = 1 − q2R2, (7.62) 3 g where a linear region can be found when plotting P(q)S (q) versus q2, the slope of which is proportional to the square of the radius of gyration of the system. All the theory summarized above refers to a system in which there is no polydispersity. When a polydisperse system is analyzed, the eﬀect of the polydispersity on the scattered in- tensity has to be taken into account. It can be seen from equation (7.56) that, since the intensity scattered by each particle is proportional to the square of its volume (proportional to the square of the mass), large particles contribute much more to the total scattered intensity than small particles. In particular, in the case of a dilute population of particles with m diﬀerent classes of particles, the total scattered intensity becomes:

m X 2 I(q) = I0K1 NiVp, jP j(q), (7.63) j=1

th where N j, Vp, j and P j(q) are respectively the number, volume and form factor of the j class particles. Moreover, even for a monodisperse colloidal system, when the aggregation of the primary particles occurs, since the population of aggregates is often broad, the expression of the scattered intensity becomes:

imax 2 X 2 I(q) = I0K1Vp P(q) Nii S i(q), (7.64) i=1 where Ni and S i(q) are the number and structure factor of a cluster with mass i and imax is the largest mass of the clusters in the population.

Consistently, the measured radius of gyration will be an average value hRgi, which, can be

134 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES written in the following form:

imax X 2 2 Ni(t)i Rg,i 2 i=1 hRgi = . (7.65) imax X 2 Ni(t)i i=1

Equation (7.65) shows that the average radius of gyration receives a much greater contribution from large clusters than from small clusters. This is again a consequence of the dependence on the square of the volume of the radiation scattered by an object.

7.7.3 Dynamic Light Scattering

The second scattering technique often used in the study of the colloidal systems and aggrega- tion phenomena is dynamic light scattering, which measures, instead of the scattered intensity as a function of the scattering angle, the rapid ﬂuctuations of the intensity at one speciﬁc an- gle. In a colloidal suspension, the conﬁguration of the system changes rapidly with time due to the Brownian motion of the particles, and consequently, so does the pattern of the scattered radiation. Moreover, such random motion of the particles (or clusters) results that the conﬁg- uration of the system at a certain time t loses quickly any correlation with its initial status. An eﬀective way to analyze such irregular change in the scattered intensity induced by the ran- dom motion of particles (or clusters) is to compute the intensity time autocorrelation function hI(q, 0)I(q, τ)i: 1 Z T hI(q, 0)I(q, τ)i = lim I(q, t)I(q, t + τ)dt, (7.66) T→∞ T 0 where I(q, t) is the scattered intensity at time t and τ is the delay time. When the delay time τ = 0, the intensity autocorrelation function is equal to the mean square intensity, and it decays to the square of the average intensity when the delay time τ goes to inﬁnity. For the latter, the system has lost any correlation with its initial conﬁguration. The above analysis is possible only if the system is fully ergodic, i.e., as time goes by, the system has the freedom to probe all the possible conﬁgurations and does not retain memory of previous stages. Dynamic light scattering can be used to investigate even concentrated colloidal suspension, to recover inter- esting information about the mobility of particles at high volume fractions and in the presence of multi-body interactions, but through a very complicated and sophisticated analysis. In this paragraph we will focus our attention only on the case of dilute colloidal suspensions.

135 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

It is useful to introduce the normalized intensity autocorrelation function:

hI(q, 0)I(q, τ)i g(2)(τ) = , (7.67) hI(q)i2 where hI(q)i is the average intensity. It can be shown that g(2)(τ) is related to another autocor- relation function, the electric ﬁeld autocorrelation function g(1)(τ), deﬁned as:

hE(q, 0)E∗(q, τ)i g(1)(τ) = , (7.68) hI(q)i where E(q, τ) is the electric ﬁeld of the scattered wave at delay time τ and wave vector q, and E∗(q, τ) is the complex conjugate. The relation between the two autocorrelation functions is called Siegert relation: 2 g(2)(τ) = 1 + σ g(1)(τ) , (7.69) where σ is a constant that depends on the speciﬁc conﬁguration of the detector used in the experiment, but it is always smaller than unity and approaches 1 with increasing the detector area. It can be shown that in the case of a dilute suspension of equal size, non-interacting spherical particles, the ﬁeld autocorrelation function decays exponentially, and the time con- stant is proportional to the particle diﬀusion coeﬃcient Diﬀ:

(1) 2 g (τ) = exp −Diﬀq τ . (7.70)

From equation (7.70), it can be seen that the faster the particle move, the larger their diﬀu- sion coeﬃcient and the faster is the decay of the exponential. Therefore, by measuring g(2)(τ), g(1)(τ) can be extracted using the Siegert relation, equation (7.69), and from the slope of the logarithm of g(1)(τ), one can determine the diﬀusion coeﬃcient, and consequently the hydro- dynamic radius Rh using the Stokes-Einstein relation: kT Diﬀ = , (7.71) 6πηRh For a sphere, the hydrodynamic radius is equal to the sphere radius. For any other body, equation (7.71) deﬁnes the hydrodynamic radius as the size of the equivalent sphere that ex- periences the same friction as the body. In the case of a polydisperse suspension, equation (7.70) does not hold any longer. The contribution of particles (clusters) of diﬀerent sizes to the total ﬁeld autocorrelation function is proportional to their masses squared and to their scattering form factors (structure factors).

136 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES

In the case of a population of clusters, equation (7.70) becomes:

imax X 2 2 Nii S i(q) exp −Diﬀ,iq τ g(1)(τ) = i=1 . (7.72) imax X 2 Nii S i(q) i=1 It is clear that measurements performed at diﬀerent angles, i.e., at diﬀerent q values, give diﬀerent results. An important consequence of equation (7.72) is that only an average diﬀusion coeﬃcient can be estimated, and therefore an average hydrodynamic radius hRhi:

imax X 2 Ni(t)i S i(q) i=1 hRhi = , (7.73) imax 2 XNi(t)i S i(q) eﬀ i=1 Rh,i

eﬀ where Rh,i is an eﬀective hydrodynamic radius of a single cluster with mass i, accounting also for the rotational diﬀusive motion of the cluster. From Eqs. (7.73) and (7.65), it can be seen that dynamic light scattering and static light scattering alow one to determine two diﬀerent average sizes of the CMD. These sizes are independent moments of the CMD, and contain independent information on the width of the CMD, thus useful information for the CMD analysis. These are also the formulas that allow one to relate measurable quantities to the results of PBE computations.

7.8 Zeta Potential, Electrophoretic Mobility, and Surface Charge Density

When working with electrostatically stabilized particles, it is particularly important to de- termine their surface charge status. This is typically carried out by using a combination of techniques. The ﬁrst step usually consists in measuring the surface charge density, or to be more precise the maximum surface charge density. Potentiometric titration can be used for this purpose. Potentiometric titration consists in using either a concentrated base or a concentrated acid, which are added in small quantities, and simultaneously measuring the conductivity of the suspension. Titration works exactly as in the case of common acids or base solutions. It

137 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES allows one to measure the point of zero charge of a colloidal particles, which corresponds to the point where all of its charges have been neutralized. From a simple material balance, the total amount of base (acid) used to achieve neutralization can be related to the amount of surface charge. However, another physical property is very commonly used to extract information on the surface charge of particles: the electrophoretic mobility. It is well known (and also rather in- tuitive) that a charged particle moves in the presence of an external electric ﬁeld. The velocity at which the particle will move is linearly proportional to the applied electric ﬁeld. The elec- trophoretic mobility is deﬁned as the ratio between the velocity at which the charged particle moves and the applied electric ﬁeld. Developing a comprehensive theory which accounts for all the physics involved in the study of the electrophoretic mobility is a demanding task. In the following, we will therefore restrict us to the case where particles are surrounded by a thin double layer. This occurs in the presence of a suﬃcient amount of electrolytes. Since the thickness of the double layer is small compared to the size of a particles, one can use planar geometry to perform a few simple calculations. The next ﬁgure shows the geometry.

We consider a small slab of ﬂuid parallel to a charged planar surface. In the presence of an electric ﬁeld, there are two forces acting on the small slab of ﬂuid: the electrostatic force and

138 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES the viscous drag force, and the two have to balance each other. The electrostatic force per unit volume is equal to:

Fel = Eρ (7.74) where E is the electric ﬁeld and ρ is the volume charge density. The viscous drag is instead equal to: d2v F = η (7.75) vis dx2 where η is the dynamic viscosity, and v the ﬂuid velocity. By equating the two forces, and making use of Poisson equation to express the charge density as a function of the electrostatic potential, one obtains the following equation:

d2ψ d2v E = −η (7.76) dx2 dx2 A ﬁst integration of this equation leads to: dψ dv E = −η + C (7.77) dx dx where the arbitrary constant C has to be equal to zero since at inﬁnite distance from the surface both dψ/dx and dv/dx have to be equal to zero, meaning that both electric ﬁeld and velocity ﬁeld are constant at inﬁnite distance from the surface. A second integration can be carried out from the so-called shear plane, i.e., the position where the velocity is zero (which is located very close to the surface) and the potential equal to the so-called ζ-potential, and outsize the double layer, where the electrostatic potential equals zero and the velocity equals the particle velocity ν. The ﬁnal expression for the electrophoretic mobility u is: ν ζ u = = (7.78) E η The most remarkable feature of equation (7.78) (originally derived by Smoluchowski) is that the electrophoretic mobility u is independent of the particle size, and only depends on the value of the ζ-potential. The concept of ζ-potential is very important in colloidal science. Since the ζ-potential is the potential at a position very close to the surface (even though it is not the potential at the surface), it provides very useful information about the surface charge status of the particles. This information is complementary to that provided by titration. In fact, the shear plane, where the zeta potential is measured, is located outside the Stern layer. It therefore accounts for the net charge of a particle, i.e., both the surface charge and the counterions located within the inner Helmholtz plane. This net charge enclosed within the

139 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES surface of shear, is smaller than the charge estimated from titration measurements, but more useful in studying colloidal stability of particles. Equation (7.78) is only valid for small double layers compared to the particle size. When instead the double layer is larger than the particle size, Debye proved that the electrophoretic mobility is equal to 2/3 of the values predicted by equation (7.78). A more complete theory, developed by Henry, provides accurate results for all double layer thicknesses, but only for low surface potentials, and shows that the electrophoretic mobility increases monotonically from the Debye limit to the Smoluchowski limit. However, a non-monotonic behavior is observed for high surface potentials, as shown in the next ﬁgure. These curves are obtained using more complex numerical calculations. In addition, a weak dependence on the type of electrolyte present in the system has been also observed.

Nowadays electrophoretic mobility is most often measured through a combination of DLS and electrophoresis. In fact, in the presence of an electric ﬁeld, the ﬁeld autocorrelation func- tion of a particle takes the following form:

(1) 2 g (τ) = exp (±iqEuτ) exp −Diﬀq τ . (7.79) where i is the imaginary unit. Therefore, the autocorrelation function shows a typical oscil- lating pattern in the presence of an electric ﬁeld, the frequency of which equals qEu. The

140 CHAPTER 7. KINETICS AND STRUCTURE OF COLLOIDAL AGGREGATES electrophoretic mobility can then be obtained by ﬁtting the frequency of these oscillations, and from this the particles zeta potential is calculated.

141 Chapter 8 Proteins and Bioprocesses

8.1 Proteins and Biomolecules

This introductory paragraph summarizes a few basic concepts of protein science required for the next paragraphs. The human body is composed of water (60 %) and of a limited number of classes of biomolecules, which include mainly DNA, RNA, lipids and proteins. Proteins account for about 20 % of the mass of the human body, and are involved in essentially all cellular functions, including: - signals and reactions: e.g., enzymes, hormones (insulin), immunosystem (antibodies, cy- tokines) - structure: e.g., actin and myosin (muscle) - transport: e.g., hemoglobin (oxygen), albumin

These biomolecules exhibit a modular architecture which is composed of a limited num- ber of building blocks. DNA from nucleotides, carbohydrates from few monosaccharides (sugars), proteins from aminoacids (20 in the genetic code). Such building blocks are con- nected via covalent bonds (peptide bonds for proteins) to form the biomolecular chain. From this point of view, biomolecules can be seen as biopolymers, where the monomers are rep- resented by the building block (nucleotides, aminoacids, ...). The design of a biomolecule implies a large number of degrees of freedom in terms of both the number and the nature of the building blocks composing the chain (Figure8.1a), which allow to ﬁnely tune the surface chemistry (e.g, modulate surface charge, hydrophillicity, hydrophobicity...).

How do cells produce proteins with a given sequence? The information about the sequence is contained in the DNA, and the production of proteins occurs in cell compartments, called ribosomes, according to a process called protein transcription: during this process the DNA

142 CHAPTERMany biomolecules 8. PROTEINS AND are BIOPROCESSES biopolymers: Proteins

a b

Peptide Bond

Figure 8.1: a) List of aminoacids and chemistry of the peptide bond; b) diﬀerent levels of protein structure 8 sequence is 00read00 by the cell, and 1 codon of DNA (composed of 3 nucleotides) is translated into 1 aminoacid. Proteins are therefore generated as linear chains of a certain number of aminoacids, and after their formation they have to fold to acquire suitable secondary and ter- tiary structures (Figure 8.1b). This important step, called protein folding, is regulated by a bal- ance of non-covalent forces, with a competition between intra-molecular and extra-molecular interactions. In particular, the burying of hydrophobic aminoacis inside the inner part of the protein structure represents a major driving force for protein folding.

The acquisition of the correct tertiary structure is a crucial prerequisite for the proper func- tion of the protein. The connection between protein structure and function dates back to the formulation of the 00lock and key model00 by Emil Fisher in 1894. From a colloidal point of view, such a complex structure as well as the activity of biomolecules is regulated by a large number of non covalent forces: in addition to van der Waals and electrostatic interactions (discussed in Chapter 6), hydrogen bonds, hydrophobic eﬀect, salt bridges and other solvation forces play a relevant role. Interaction potentials are typically complex, and in most cases DLVO theory alone is not suﬃcient to describe the colloidal stability. Although the strength of non-covalent forces is much weaker than covalent bonds (2-7 kcal/mol of hydrogen bond versus 70-110 kcal/mol of covalent bond), a single biomolecule can exhibit a large number of

143 CHAPTER 8. PROTEINS AND BIOPROCESSES

these interactions, making their contribution crucial.

The structure-function paradigm remains a milestone in protein sciences, and applies to the vast majority of the systems. However, in the last decades a large number of proteins have been discovered to be intrinsically disordered and functional in the unfolded state. These pro- teins typically require promiscuity and ﬂexibility for their functions (e.g. binding to multiple targets). Interestingly, from a physicochemical point of view, these proteins are characterized by higher net charge and lower hydrophobicity with respect to natively folded proteins (Figure Intrinsicallly8.2). Disordered Proteins (IDP)

A large number of proteins are “intrinsically disordered” and functional in the unfolded state (promiscuity, flexibility)

Figure 8.2: Intrinsically disordered protein (adapted from Habchi J. et all, Chem. Rev., 2014, 114, 6561-6588 9

The considerations of this introductory paragraph highlight that there is a fundamental con- nection between protein structure, protein-protein interactions and protein functions. Typical examples of protein functions include binding, self-assembly and enzymatic activity.

The understanding of the functional and aberrant behaviours of proteins in biological sys- tems is important in chemical biology and biomedical sciences, for instance to identify thera- peutic strategies to ﬁght against pathological states.

Moreover, the possibility to engineer functionality by playing with structure makes pro-

144 CHAPTER 8. PROTEINS AND BIOPROCESSES teins attractive materials in the biotechnological context. Indeed, the understanding of the molecular and chemical biology underlying cellular functions, as well as the advent of recom- binant DNA technology, allows us to exploit microorganisms as living reactors to produce desired proteins or use proteins in microroganisms to generate speciﬁc chemical molecules. The manipulation of a living organism or a part of it (e.g. enzymes) to produce a chemical or biological material is the core activity of biochemical engineering. This technology is applied in a very broad range of biotechnological applications to produce products for chemical, food and pharmaceutical industries. Important examples of biochemical products include the pro- duction of ethanol from sugar and corn via yeast, of therapeutic proteins by mammalian cells as well as the production of antibiotics and glutamic acid for food applications.

Figure 8.3: Advances in the area of biochemistry and microbiology in the past years have driven the development of numerous novel products and a new industry.

The application of biotechnology on an industrial scale exhibits a series of engineering challenges analogous to the polymer reaction and colloid engineering systems analyzed in Chapters 1-7 (Figure8.4).

145 CHAPTER 8. PROTEINS AND BIOPROCESSES

a Process Kinetics and Reactor Design

- Bulk Polymerization - Solution reaction - Suspension - Emulsion

Product Formulation Chain Length Distribution/ Particle Size Distribution (colloidal stability, PBE)

b Process Kinetics and Reactor Design Enzyme - Batch - Continuos - Sensors - Mass Transfer (Aeration) Microbial growth and product expression

Product Formulation Product recovery (Separation unit)

Figure 8.4: Analogies between a) polymer reaction engineering and b) biochemical engineering.

8.2 Enzyme Kinetics

Enzymes catalyze chemical reactions in biological systems. These biomolecules are typically structured 3-D proteins exhibiting one or more active sites on the surface, where suitable substrates can bind. Enzymes increase reaction rates by a factor of 106-1012 by stabilizing transition states and reducing activation energy barriers. Therefore they assist reactions but are not modiﬁed during the process. Their peculiarity consists in performing this catalytic activity with extremely high selectivity and at mild conditions of temperature.

8.2.1 Michaelis-Menten Equation

In 1913, L. Michaelis and M.L. Menten derived the equations describing enzymatic rates for a single substrate reaction, which were later modiﬁde by Briggs and Haldane in 1925. Their theory describes a kinetic scheme for the enzyme E and its substrate molecule S to form a

146 CHAPTER 8. PROTEINS AND BIOPROCESSES complex before proceeding to the product P:

k1 k2 E + S )−−*−− E · S −→ E + P k−1 The intermediate ES is assumed to be at any given time at steady state with respect to E and S This means that it is possible to apply the PSSA assumption (Chapter 1, paragraph 1.5), and assume that d[ES]/dt = 0:

d[ES ] = k [E][S ] − k [ES ] − k [ES ] = 0 dt 1 2 −1

k1 1 [ES ] = [E0][S ] = [E0][S ] k2 + k−1 KM where KM is the Michaelis Menten constant. Introducing the mass balance equation [E0] =

[E] + [ES ], where [E0] is the total amount of enzyme initially present in the reaction mixture, we can derive: [E ][S ] [ES ] = 0 KM + [S ] The rate of product formation is given by:

[E0][S ] v = k2[ES ] = k2 KM + [S ]

At high substrate concentrations v = vmax = k2[E0]. The rate of product formation is typically expressed in the compact form: v [S ] v = max KM + [S ] It is convenient to re-arrange the last equation by introducing the reciprocal of the rate (1/v) and of the subtrate concentration (1/[S ]), in order to obtain a linear representation known as the Lineweaver-Burk plot.

8.2.2 Engineering of enzyme kinetics

Several possibilities to modulate enzyme kinetics. For instance, inhibition:

• Competitive: the inhibitor competes with the substrate for the active site of the enzyme E.

• Uncompetitive: the inhibitor binds to either a modiﬁed form of the enzyme which arises when substrate is bound, or to the enzyme-bound substrate itself ES .

147 CHAPTER 8. PROTEINS AND BIOPROCESSES

Figure 8.5: Enzymatic reaction rate as a function of substrate concentration and Lineweaver-Burk plot

• Non-competivie: the inhibitor can combine with either the free enzyme (E) or the ezyme-substrate comples (ES ).

Additional considerations:

• Many enzymes are used in immobilized form, in particular for continuous processes;

• Several enzymes require the binding of small molecules (coenzymes) to be active;

• In many cases more complex kinetics are observed.

148 CHAPTER 8. PROTEINS AND BIOPROCESSES

8.3 Bioprocessing

In the following, we will discuss the basic operation units that are required in a bioprocess.

8.3.1 Microbial growth

First, we need to understand the kinetics of cell growth. Typical systems are bacteria (e.g. E.coli), mammalian cells (e.g. Chinese hamster ovary (CHO) cells) or yeast (e.g. Pichia Pastoris). More recently, also plants and insect systems have been used. The growth rate of a cell is related to the cell metabolism, the set of reactions that are employed by a cell to consume a substrate and generate products. In batch cultivations, the growth rate is divided into four characteristic phases: lag-phase, exponential phase, stationary phase and dead phase. It is important to correlate the growth rate with substrate concentration and other parameters. On this purpose, diﬀerent levels of complexity of models can be applied. Most realistic models should consider a) individual metabolic reactions occurring within the cell; b) variations from cell to cell in a population. In practice, simpler models are considered, which can be divided as: • Segregated: individual cells are diﬀerent from one another. Nonsegregated: population is lumped into one biophase which interacts with the external environment (cell concentration is one variable alone). • Structured: models consider individual reactions or groups of reactions occurring within the cell. Unstructured: models view the cell as an entity in solution which interacts with the environment.

The most simple relationships are unstructured models describing the exponential growth. The most simple expression that includes the eﬀect of nutrient concentration is the Monod model. This model assumes that only one substrate (the growth-limiting substrate, S) is im- portant in determining the rate of cell proliferation. Based on the observation that the substrate transport to the cell is limited by the activity of an enzyme (a permease), Jacques Monod pro- posed a cell growth expression that follows the Michaelis-Menten form:

µ S µ = max Ks + S where µmax is the maximum speciﬁc growth rate of the cells, and Ks is the value of the limiting nutrient concentration which results in a growth rate of half the maximum value. The variation

149 CHAPTER 8. PROTEINS AND BIOPROCESSES of the dry cell weight per volume (X) during time is: dX µ SX = max dt Ks + S

Figure 8.6: Typical time evolution of the growth of a microorganism in a bacth reactor.

After determining the kinetics of cell growth, we need to understand how the synthesis of the desired product by the cell is connected to the rate of cell growth. Here we can distinguish between three diﬀerent types of fermentation (Gaden, Biotech. & Bioeng., 67, 6, 2000): - In fermentation of type I the product is generated directly from the primary energy metabolism of the cell (e.g. biomass itself, ethanol, lactic acid); - In fermentation of type II the product is still originated from the primary energy metabolism of the cell but in an indirect way: it can represent the product of a by-side reaction, or of a reaction which follows in series the production of the mean products of the energy metabolism (e.g. citric acid); - In fermentation of type III the product does not arise from the primary energy metabolism but is synthesized from secondary metabolic pathways of the cell (e.g. antibiotics/ vitamins). Depending on the type of fermentation, the rate of product formation follows the kinetics of cell growth according to diﬀerent proﬁles (Figure 8.7).

8.3.2 Reactor design

In the previous paragraphs we have analyzed the kinetics of our reactions, either enzymatic or cellular. Now we have to decide how to operate our reactions on an industrial scale. Also in bioprocessing, the reactor can de designed in diﬀerent conﬁgurations: batch, fed-batch,

150 CHAPTER 8. PROTEINS AND BIOPROCESSES

Figure 8.7: Diﬀerent types of fermentation.

continuous and plug-ﬂow. Bioreactors which use living cells are usually called fermentors. Bioreactors usually handle liquids, since most chemical reactions occur in the liquid phase, and involve also a gas phase, e.g. aerobic fermentors. Colloids, such as immobilized enzymes or cells, are handled too, either suspended or ﬁxed in a liquid phase.

Figure 8.8: Diﬀerent conﬁgurations of a bioreactor.

Batch Mass balance for a reactant A;

dC dx V A = VC A = −r V dt A0 dt A

−3 −1 3 where rA is the reaction rate (mol · m s ), V is the liquid volume (m ), CA is the reactant −3 concentration (mol · m ), and xA is the fractional conversion of the reactant A, deﬁned as

1−CA/CA0, with CA0 the initial reactant concentration in the liquid in the reactor. The material

151 CHAPTER 8. PROTEINS AND BIOPROCESSES balance can be integrated into:

Z CA dC Z xA dx t = A = C A − A0 CA0 rA 0 rA For enzyme-catalyzed reactions following the Michaelis-Menten law, we can derive for the substrate S :

CS 0 xS − Kmln(1 − xS ) = vmaxt In case of batch fermentors, cells are grown during the exponential phase, in conditions where the substrate is not rate-limiting. In this case µ = µmax and dX 0.693 = µmaxX = X dt tD where tD is the doubling time, the time required to double the population of cells. CSTR The material balance for the reactant A at steady state reads:

FCA0 − FCA0(1 − xA) = −rAV

where F is the volumetric feed rate (m3 s−1) and V is the volume of the reactor (m3). An important parameter is the residente time τ (s), which is deﬁned as: V C x τ = = A0 A F −rA The recriprocal of τ is called the dilution rate, D. For Michaelis-Menten type reaction we can derive for the substrate S :

xS vmaxτ = CS 0 xS + Km 1 − xS For cell growth, the balance reads:

F(X − X0) = µXV

and the dilution rate D can be expressed as: F µ S D = = µ = max V Ks + S

152 CHAPTER 8. PROTEINS AND BIOPROCESSES

Additional aspects in reactor design

• Inoculum;

• Aeration and oxygen mass transfer;

• Sterilization;

• Biosensors.

8.3.3 Product recovery, formulation and delivery

After the production of the desired biomolecule from the cells, the product has to be recov- ered from the mixture of thousands of other proteins of the host system. This puriﬁcation step accounts for about 60-80% of the production cost for therapeutic proteins, and about 60% for enzymes. Many diﬀerent separation strategies have been developed: ﬁltration, extraction, crystallization, membrane, chromatography. Typically, more than one operation units are ap- plied within the same process, with polishing steps following initial puriﬁcation units.

8.3.4 Choice of the reactor conﬁguration

Choice of using either the isolated enzyme or the whole cell:

• Advantages isolated enzyme: more homogeneous solutions for the recovery of the prod- uct (still a challenge - see immobilized enzymes); reduced problems of contamination; reaction mechanism is well understood;

• Advantages entire cell: enzymes in native environment (more stable, right co-factors); cheaper

Choice of continuous/batch operation: The decision to run a process in continuous or in batch operation is dictated by several factors.

• Advantages batch: Reduced risk of contamination; ﬂexibility; possibility to control quality of single batch. Disadvantages batch: presence of dead-times; diﬀerences from one batch to another; possible accumulation of inhibitors.

153 CHAPTER 8. PROTEINS AND BIOPROCESSES

• Advantages continuous: reduction of dead-times; possibility to control processes at steady-state; suitable for large scale production, when reaction is inhibited by a product, when organism has high genetic stability. Disadvantages continuous: high risk of contamination; no fermentation type II or III.

8.3.5 Biopharmaceuticals

The pharmaceutical industry is an important industrial sector concerned with the development and the manufacturing of molecules for diagnostic and therapeutic purposes. Very broadly, we can distinguish between drugs generated via chemical synthesis and molecules produced through the biotechnological route involving biological systems (e.g. plant and animal cells, yeast, bacteria). This sector of biotechnology is deﬁned as red biotechnology.

• Chemical synthesis: Small molecules ( MW 180 Da)

• Biological synthesis: complex molecules e.g. proteins ( MW 150000 Da)

Biopharmaceuticals currently represent around 20% of the entire pharmaceutical revenue, and their number is continuously growing at a rate that exceeds small molecules. Major ad- vantages of biopharmaceuticals include higher speciﬁcity, higher eﬃciency and reduced side eﬀects. However, this improved performance is accompanied by drawbacks related to the more complex bioprocess underlying their production. In this ﬁnal paragraph, we re-visit the general concepts described in this Chapter highlighting the speciﬁc needs of this very impor- tant sector. Main biopharmaceuticals are insulin, growth hormones, monoclonal antibodies, vaccines ( e.g. tetanus, hepatitis B). Monoclonal antibodies currently own the largest market share in terms of value in the global biopharmaceutical market and have a number of therapeutic applications in the treatment of asthma, cancers, autoimmune diseases and other pathological conditions.

154 CHAPTER 8. PROTEINS AND BIOPROCESSES

Industrial (white) Biotechnology Biopharmaceutical Industry Host: enzymes mammalian cells microorganism Products:

Aspirin 21 atoms Hormon ~3000 atoms Antibody ~25 000 atoms

Car Plane Bike

Cost of development / complexity

Figure 8.9: Biopharmaceuticals involve higher cost and more complex processes compared to other bioproducts such as ethanol, sugars, enzymes, amino acids, vitamins.

Production of recombinant proteins with medical applications

This chapter mainly focuses on the production and puriﬁcation of proteins produced by a mammalian expression system which are able to perform posttranslational modiﬁcations such as glycosylation. Most recombinant proteins in this category are complex and highly variable molecules that need to possess certain quality attributes for full bioactivity and therapeutic safety. Product quality attributes include:

• Glycosylation ( attachment of sugar moieties to proteins)

– Variations in terms of glycosylation patterns provoke a heterogeneous product mix- ture

– Aﬀects protein folding

– Inﬂuences therapeutic eﬃcacy (ADCC, CDC, life-time)

155 CHAPTER 8. PROTEINS AND BIOPROCESSES

– Immunogenicity

• Charge isoforms ( charge variants of proteins) – Protein charge heterogeneity – Caused by chemical or enzymatic modiﬁcation – Protein charge distribution – Therapeutic eﬃcacy and safety unknown

• Structural changes – Fragmentation and aggregation – Comprises drug eﬃcacy and safety

Example: Herceptin (Trastuzumab) contains multiple isoforms with diﬀerent activities.

It is of prime importance to limit and control the heterogeneity of the ﬁnal product for safety compliance and therapeutic eﬃcacy. Undesired product modiﬁcations can be limited and pre- vented at various stages of the development and manufacturing process.The next paragraph focuses on assessing the impact of diﬀerent operation modes on the critical quality attributes (including product related-impurities).

P (140% activity) S1 W1 W2 W3 W4 (12% activity)

Figure 8.10: Analytical weak cation exchange chromatogram of trastuzumab (commercial name, Herceptin)

156 CHAPTER 8. PROTEINS AND BIOPROCESSES

Figure 8.11: Development strategy

Fed-batch bioreactors

• Most widely used technique in industry for the production of recombinant proteins

• Based on the periodic delivery of fresh feeds (e.g. glucose, amino acids) to support cell growth and prolong the productive culture life time

Figure 8.12: Protein product concentration proﬁle during fed batch cultivation

Upon inoculation the cell density increases and the expressed protein is accumulated in the bioreactor, which is harvested once the cells enter the death phase. Advantages

157 CHAPTER 8. PROTEINS AND BIOPROCESSES

• Simpler operation

• Ease of scale-up

• High titer concentrations at the time of harvest that simpliﬁes downstream processing

Disadvatages

• The accumulation of cellular by-products and the changing cellular environment envi- ronment inhibits cell growth, reduces productivity and quality.

• The expressed product is harvested and puriﬁed after eight to 21 days

Perfusion bioreactors Perfusion cultures are continuously operated systems where the continuous addition of fresh media is coupled with the outﬂow of spent media while cells are retained inside the reactor. In contrast to batch and fed-batch processes, where there is no removal of inhibitory metabolites, in continuous processes medium is perfused at dilution rates exceeding the cellular growth rate. For this, a good separation device is needed to retain cells in the bioreactor. Cells are held within the reactor by sedimentation, ﬁltration or centrifugation (e.g. gravity-based cell settlers, spin ﬁlters, centrifuges, cross ﬂow ﬁlters, alternating tangential- ﬂow ﬁlters...). Example: Perfusion reactor with external ﬁltration device

Perfusion

Figure 8.13: Perfusion set up featuring feed, bleed and harvest stream. The harvest stream is passed through an external ﬁltration device to retain the cell in the bioreactor. Diﬀerent cell density proﬁles are obtained during diﬀerent modes of operations

In this case, the harvest stream is passed through an external ﬁltration device, which physi- cally retains the cell in the bioreactor. The bleed stream, on the other hand, is a cell containing

158 CHAPTER 8. PROTEINS AND BIOPROCESSES outﬂow used to control and maintain a high viable cell density.

Advantages

• Prolonged culture at high viable cell density

• Enhanced volumetric productivity

• Steady state operation resulting in a constant cellular environment which leads to a constant product quality

• The protein product is continuously harvested which minimizes the exposure to degrada- tive enzymes and metabolic by-products ( e.g. lactate ammonia) if directly puriﬁed

• Small equipment footprint

Disadvantages

• More complicated operation ( maintain sterility, more complex process control) result- ing in a higher risk of failure

• Higher media consumption

• Lower protein product concentration at harvest

Comparison fed-batch and perfusion

• Products prone to degradation (e.g. unstable proteins, highly hydrophobic proteins) require perfusion due to the reduced residence time of the product

• Perfusion is preferred for cell lines with growth associated to the product formation (product concentration increases with cell concentration)

• Lower protein product concentration at harvest in case of perfusion

• Fed-batch , on the other hand, may be favoured in the case of high medium costs

• If cells secrete product in a non-proliferative state or the cell line is unstable, so that the production time horizon is limited, fed batches would be the method of choice

159 CHAPTER 8. PROTEINS AND BIOPROCESSES

1.0 Perfusion Fed-batch Residence time distribution: 0.8

0.6

0.4 Perfusion: τmean = 1 day 0.2 Protein fraction / (-) 0.0 0 2 4 6 8 10 12 14 16 18 Time / (days)

Fed-Batch: τmean = 9 days Probability for protein modification

Figure 8.14: Comparison of the residence time distribution of the expressed product cultivated in fed-batch and in a perfusion reactor

The choice is often based on company tradition, existing facilities, infrastructure and ex- perience. Nevertheless there is a growing interest in high density perfusion cultures due to advantages including product quality, steady state operation and high culture viability. Example: Comparison of fed-batch and perfusion operating conditions in terms of product quality.

• Increased product residence times prolong the exposure of the product to proteases and other degradative enzymes which can lead to fragmentation.

• Furthermore the prolonged exposure can also lead to an increased probability of chem- ical and enzymatic protein modiﬁcations which can cause acidic or basic isoforms.

• The steady state operation in perfusion bioreactors and the shorter residence time favour homogenous post-translational modiﬁcations such as glycosylation

• Protein aggregation is shown to depend on protein concentration, process parameters (temperature, pH, aeration) and residence time.

• Glycosylation appears to reduce aggregation, probably due to the corresponding reduc- tion of in hydrophobicity of the protein.

• Especially the constant metabolite composition and by-product formation during perfu- sion cultures favour the desired glycosylation pattern

160 CHAPTER 8. PROTEINS AND BIOPROCESSES

Outlook

Figure 8.15: Future trends in biotechnology

• Continuous processing is attracting attention in most industries

• The continuous production of biopharmaceuticals has evolved in the past years and may eventuall become the preferred technology

• Currently 5 recombinant proteins and mAbs using perfusion bioreactors are on the mar- ket

• Companies also work on an end-to-end continuous production (-upstream and down- stream) production

161 Chapter 9 Protein Aggregation

9.1 Proteins and Colloids

In all biotechnological applications which involve proteins, particular attention must be given to the stability of the complex protein structure to guarantee proper function. Indeed, proteins are exposed to a broad range of chemical and physical instabilities, which can modify their structure and deteriorate their activity.

• Chemical instabilities include oxydation, deamidation, asparic acid isomerization, pep- tide fragmentation, nonreducible cross-linking.

• Physical instabilities are represented mainly by protein aggregation. Aggregation of ther- apeutic proteins is a signiﬁcant hurdle in protein drug development, hindering rapid commer- cialization of potential drug candidates. Aggregation is indeed the major protein instability en- countered in almost all stages of therapeutic protein manufacturing, including expression from the cells, puriﬁcation, storage, shipping and administration to the patient. About 20 − 25% of the approved therapeutic proteins are administred subcutaneously via injections and are for- mulated as solutions at high protein concentrations (50-200 mg/mL) in order to reduce the injection volumes below 1.5-2 mL. Such high concentrations can clearly promote interactions and aggregation. Since the presence of protein aggregates in pharmaceuticals may compro- mise drug safety and drug eﬃcacy, the protein aggregate content must be strictly controlled to assure satisfactory product quality. There is therefore a severe need to increase our un- derstanding of the mechanisms of protein aggregation at a fundamental level with the aim of optimizing the protein primary sequence and/or the operative parameters, e.g. the solution composition in terms of pH, type and concentration of excipients. This challenge is again a colloidal stability problem. Protein sizes are indeed typically in

162 CHAPTER 9. PROTEIN AGGREGATION

Figure 9.1: Key diﬀerences between proteins and polymer colloids

12 + 10 pH 3.0 - 4.0 Unstable

8 Net Charge < Rh >(nm) pH 4.5 - 6.0 6 - Stable 4 0 20 40 60 80 Time (h) pH-induced pH-induced surface charge changes structure changes

Figure 9.2: Example of the aggregation behavior of a monoclonal antibody solution at low pH

the order of a few nanometers, and are thus lying in the colloidal range. Proteins are therefore small enough to be aﬀected by Brownian motion, but suﬃciently large compared to solvent molecules so that the solvent can be considered as a continuum. Several of the concepts and techniques discussed in Chapters 1-7 for polymers apply also to proteins, in particular for globular aggregates formed by folded proteins. For instance, several protein aggregates exhibit fractal morphology, in analogy with polymer clusters. Light scattering techniques are often used to characterize the structure of protein gels in terms of fractal dimension. However, there are crucial diﬀerences between proteins and polymer colloids, mainly because of the complex protein secondary and tertiary structure.

163 CHAPTER 9. PROTEIN AGGREGATION

To explain this diﬀerence, we use as an example the stability of a monoclonal antibody at low pH: the aggregation stability, which is followed by monitoring the increase during time of the average radius of the population, decreases with increases pH value (Figure 9.2). From a colloidal point of view, the net charge of a protein increases with the increase of the diﬀerence between the pH and the pI value. However, the low pH values modify the secondary and tertiary structures of the proteins; following these unfolding events, reactive hydrophobic patches can be exposed to the exterior, and the attractive hydrophobic forces can overcome the electrostatic repulsive interactions. This example explains clearly how for proteins there is the need to characterize simultaneously aggregation and structural stability. As a consequence of this complexity, the DLVO theory has only limited applications.

9.2 Experimental biophysical techniques

In protein science, and in particular in problems dealing with protein aggregation and self- assembly, experimental analytics is a fundamental aspect and represents the ﬁrst step to per- form any mechanistic study. Protein systems typically exhibit a series of challenges including very low and high values of proteins concentrations, presence of dynamic equilibria and very heterogeneous mixtures, with presence of species ranging from few nm to several microns. As discussed before, with respect to colloidal systems, there is the need to characterize not only the size and shape of the aggregates but also potential changes in the structure of the protein species. In addition, more practical limitations of laboratory experiments related to the small volumes and amounts of material which are normally available have also to be considered. Currently, there is not a single technique capable of providing all the required information. Rather, a bactery of diﬀerent approaches has to be applied in parallel (Figure 9.3). Size and Molecular Weight: In analogy with colloidal systems, light scattering (Chapter 7) represents one of the most important techniques to achieve information about the size and the shape of the protein aggregates which are generated during the aggregation reaction. Static Light Scattering (SLS) and Dynamic Light Scattering (DLS) can be used to follow the increase in the average gyration radius (< Rg >) and in the average hydrodynamic radius (< Rh >), respectively, as well to measure the fractal dimension of the aggregates. However, light scattering is challenging to apply for the analysis of the heterogeneous mix- tures typically observed during the aggregation of proteins in solution. In particular, from the average signal recorded in bulk experiments is diﬃcult to de-convolute information about the

164 CHAPTER 9. PROTEIN AGGREGATION

Figure 9.3: Overview of conventional biophysical methods to investigate protein aggregates over dif- ferent length scale. Zoells S. et al., J. Pharm, Sci, 101,3, 914-935 2012

full size distribution.

An attractive strategy to address this limitation consists in performing the fractionation of the protein mixtures before analyzing individually the fractionated species. The most common method is represented by Size Exclusion Chromatography coupled with inline multi angle light scattering. Limit of the size of the aggregates that can be detected, used to quantify the residual monomer and the oligomer distribution (see Figure 9.4 (a)). Secondary and Tertiary Structure: In order to characterize the structure of the protein, circular dichroism and Fourier Transform Infrared Spectroscopy are some of the most common methods. Protein stability: Isothermal Calorimetry and diﬀerential scanning calorimetry.

165 CHAPTER 9. PROTEIN AGGREGATION

8

88 88 88 88 88

Figure 9.4: Typical SEC chromatogram of a mixture of mAb monomer and mAb aggregates. (a) De- termination of the monomer, dimer and trimer content by peak deconvolution (b) Measure of the aggregate molecular weight from Multi Angle Light Scattering.

Microﬂuidics Very recently, microﬂuidics is emerging a very powerful tool to address many of the limitations of conventional biophysical methods. Attractive advantages include not only small volumes and short analysis times, but also the possibility to couple diﬀerent strategies on the same platform, the more accurate control of mass and heat transport and the ability to compartmentalize solutions in droplets.

166 CHAPTER 9. PROTEIN AGGREGATION

9.3 Kinetic Model and PBE

Many possible aggregation mechanisms have been observed. With respect to colloid systems, also structure changes and nucleation events must be considered in addition to growth, which can occur either via monomer addition or cluster-cluster aggregation. In many applications it is importat to discover which mechanism is the one in action.

Figure 9.5: Diﬀerent mechanisms of aggregation of therapeutic proteins (Roberts C.J., Biotechnology and Bioengineering, 98, 5, 2007.)

There are two levels of analysis to achieve this goal. A ﬁrst simpliﬁed description can be captured by monitoring the kinetics of monomer depletion at several protein concentrations

167 CHAPTER 9. PROTEIN AGGREGATION

(Figure 9.4, and evaluating an apparent reaction order n, deﬁned as:

dM = −k Mn, (9.1) dt app

Where M is the monomer concentration followed on a few half-lives and kapp is the apparent reaction rate constant for monomer loss. The value of n, which typically lye between one and two, reports on the step which is rate limiting in the monomer consumption. In particular, n = 1 is indicative that unimolecular conformational changes are rate limiting the kinetics of monomer depletion, whereas n = 2 rather corresponds to the case where monomer consump- tion is rate limited by the aggregation events leading to dimer formation. A second level of analysis implies a more comprehensive mechanistic description of the full aggregation network. On this purpose, a powerful strategy consists in comparing experi- mental data with model simulations obtained from a population balance equation scheme that describes the contribution of several individual microscopic reactions. We illustrate this strat- egy here below, using a case study as a concrete example to guide the explanation. More than the exact content of this very speciﬁc example, the student is invited to learn the diﬀerent steps (here divided in ﬁve points) of this general strategy, which can be applied to the analysis of any other system.

9.3.1 Case Study: aggregation of a monoclonal antibody (mAb-1)

1) Experimental Observations Figure 9.6 shows some experimental observations regarding mAb-1 aggregation. We con- clude from these data that, in the case of mAb-1:

(a) The monomer depletion is rate limited by monomolecular conformational changes

(b) Aggregation is irreversible

(c) Aggregates exhibit fractal morphology, with df = 1.85

168 CHAPTER 9. PROTEIN AGGREGATION

) )) ) ))) ) ))))))

) ) )

) ) )

Figure 9.6: Experimental observations for mAb-1. (a) Linearization of the monomer depletion kinet- ics followed by SEC (b) Dilution experiments to assess aggregates reversibility (c) SLS experiment to measure the fractal dimension of aggregates.

2) Reaction Scheme According to these observations, the reaction scheme shown in Figure 9.7 is proposed.

Figure 9.7: Proposed reaction scheme for mAb-1 aggregation.

First, the monomer in its native form N unfolds to form U, which is a denaturated conformational state of the monomeric protein. This step, denoted as (M1-1) in the kinetic scheme, is regarded as irreversible in this study. Indeed, U can be considered as an intermediate reactive species which is depleted by irreversible aggregation before it can re-fold. Therefore, aggregation is faster with respect to the possible backward reaction of unfolding, and the reversibility of the unfolding step can be ne- glected. It is worth mentioning that the quantity experimentally accessible from SEC experiments is the sum of the concentrations of N and U, since SEC is not sensitive to changes in protein conforma- tion. The aggregation prone form of the protein, U, can then aggregate to form oligomers, according to step (M1-2). Finally, aggregates grow irreversibly either by monomer addition or by cluster-cluster aggregation, as depicted in step (M1-3). The unfolding step is a simple monomolecular reaction, which can be easily described by a single kinetic rate constant kU. Describing the aggregation steps is a bit more challenging, though, as it requires the deﬁnition of an aggregation kernel which provides a relation between aggregate size and aggregate reactivity. Following the approach presented before in the case of polymer colloids, we ﬁrst

169 CHAPTER 9. PROTEIN AGGREGATION compute the characteristic time for rapid coagulation so as to determine whether or not aggregation occurs under diﬀusion limited conditions. At 70 ◦C, with a protein concentration of 1 g/L, we obtain −5 tRC ≈ 10 s. Therefore, we conclude that aggregation is not limited by diﬀusion under these conditions, and we select the traditional RLCA kernel to describe aggregate growth. However, it must be emphasized that this kernel was derived in the case of spheres uniformly charged, while it is known that protein reactivity strongly depends on protein conformation and on the accessibility of aggregation-prone patches. This eﬀect can be accounted for by introducing diﬀer- ent values of the Fuchs stability ratio in order to characterize the stability of diﬀerent sub-populations of species characterized by a similar reactivity. In particular, the unfolded aggregation-prone monomer U is an unstable intermediate which has a very high reactivity compared to other aggregates species. Therefore, three types of aggregation events characterized by species with diﬀerent reactivity can be identiﬁed: monomer-monomer, monomer-aggregate and aggregate-aggregate. Accordingly, three Fuchs stability ratios are deﬁned: W11,W1j and Wij, which describe oligomer formation, aggregate growth by monomer addition and aggregate growth by cluster-cluster aggregation, respectively. 3) Population Balance Equations The kinetic model corresponding to the reaction scheme of Figure 9.7 is given below:

dN − = kU N dt ∞ dU P = kU N − U k1, jU j (9.2) dt j=1 dU i−1 ∞ i≥2 1 P − P = 2 k j,i− jU jUi− j Ui ki, jU j dt j=1 j=1 With: k = k B P W−1 i, j s i, j i, j i, j k = 8k T/3η s B (9.3) 1 −1/df −1/df 1/df 1/df Bi, j = i + j i + j 4 λ Pi, j = (i j)

And W11 , W1j , Wij

It can be observed that the usual Smoluchowski population balance equations were modiﬁed in order to account for two features that are speciﬁc of proteins: (1) an unfolding step was introduced to reﬂect monomolecular changes in protein conformation, (2) several Fuchs ratio values were introduced to describe the diﬀerent reactivities of the various sub-populations present in solution.

170 CHAPTER 9. PROTEIN AGGREGATION

4) Parameter Estimation The implementation of the proposed kinetic scheme requires the estimation of several pa- rameters. Some of these parameters can be evaluated by independent measurements, while others can be estimated by ﬁtting the suitable quantities to those measured experimentally as a function of time. Since the concentration of U is low and nearly constant due to its high reactivity, the unfolding rate constant kU can be approximated to kapp, which is determined from the linearization of the experimental monomer depletion. The fractal dimension has been measured by SLS and the power law factor λ appearing in the aggregation kernel has been estimated as λ ≈ 1 − 1/df . The remaining parameters are the three Fuchs ratios which have been ﬁtted to describe the experimental data at the reference protein concentration of 2 g/L. The parameters used for the simulations are summarized in Table 9.1.

Parameter kU d f λ W11 W1 j Wi j

Value 1 × 10−3 s−1 1.85 0.5 8.5 × 106 4 × 107 8 × 108 Source kapp SLS Exp. 1 − 1/d f Fit Fit Fit

Table 9.1: Parameters used for the simulations of mAb-1 aggregation (without co-solutes). In Figure 9.8 (a-c) it can be seen that the simulations are in excellent agreement with the experiments, indicating that the proposed kinetic model can successfully describe the aggre- gation of mAb-1 under the investigated conditions. The comparison between the diﬀerent Fuchs stability ratios estimated by the ﬁtting to ex- perimental data provides information on the relative reactivity of the various species involved in the aggregation process.Considering the values reported in Table 9.1, it can be noticed thatW1j Wij . This highlights that, for this system, aggregate growth by monomer addition prevails over aggregate growth by cluster-cluster aggregation, probably due to the high reac- tivity of the unfolded monomer.

5) Model Validation To further validate the proposed kinetic scheme, the kinetics of aggregation were simulated at protein concentrations of 1 g/L and 5 g/L using the same set of values reported in Table I, with no additional parameters. In Figure 9.8 (d-i), it can be seen that the model predictions agree very well with all the experimental results, proving that the model is capable of predict- ing the concentration eﬀect on the aggregation kinetics of mAb-1 in the concentration range

171 CHAPTER 9. PROTEIN AGGREGATION

f f f k k

k k k k f f f

k

k

k k k f f f k

k

k k k k k

Figure 9.8: Comparison between experimental data and simulations for mAb-1 at protein concentra- tion of 2 g/L (a-c), 1 g/L (d-f) and 5 g/L (g-i). The experimental concentration of monomer, dimer and trimer were determined by SEC. The aggregate molecular weight was measured by SEC-MALS and the average hydrodynamic radius was followed by DLS. from 1 g/L to 5 g/L. We can therefore conclude that the kinetic scheme of mAb-1 aggregation is the one presented in Figure 9.9.

Figure 9.9: Kinetic scheme for mAb-1 aggregation

172 CHAPTER 9. PROTEIN AGGREGATION

9.4 Protein Misfolding and Aggregation in the Biomedical Context

9.4.1 Functional role of protein self-assembly and aggregation in biology

Several proteins play theri biological roles in a self-assembled state. For instance, under phys- iological conditions insulin is present as an hexamer which is coordinated by a zinc ion. An- other relevant example is represented by molecular chaperones. These proteins are crucial components of the protein homeostasis network, and assist proteins in folding correctly as well as in the removal of degraded species. Relevant chaperones are heat shock proteins, which are over-expressed as an answer to a rise in the temperature, clusterin, alpha-B crys- tallin. The vast majority of molecular chaperones are present as a distribution of oligomers in dynamic equilibrium. Diﬀerent oligomers have diﬀerent reactivity, and this quaternary struc- ture is crucial to allow molecular chaperones to react to diﬀerent situations and interact with diﬀerent protein structures.

In other cases, biology uses larger forms of protein aggregates. A particular type of protein aggregate structure which has been increasingly found in nature is represented by amyloid ﬁbrils. These aggregates exhibit a regular ﬁbrilar geometry, with a diameter of 5-10 nm and a length of 1-10 µm. Peptide and protein hormones in secretory granules of the endocrine system are stored in an amyloid-like cross-beta-sheet-rich conformation (Maji, S.K. et al., Science. 2009; 325(5938):328-32). Thus, functional amyloids in the pituitary and other organs can contribute to normal cell and tissue physiology. This colloidal state guarantees a controlled release of functional monomeric hormones in response to a change of the environment, for instance the pH. Functional amyloids are also fungal prions, which are involved in prion repli- cation, and the amyloid protein Pmel17, which is involved in mammalian skin pigmentation. Functional amyloids have also been observed in many bacteria, where they are associated to host cell adhesion and invasion, and they are potent inducers of the host inﬂammatory response (Barnhart and Chapman, Annual Review of Microbiology, 60, 131-147, 2006).

173 CHAPTER 9. PROTEIN AGGREGATION

9.4.2 Role of aberrant protein aggregation in pathology: amyloid ﬁbrils

(Reference: Knowles, T.P.J. et al., The amyloid state and its association with protein misfold- ing diseases. Nat. Rev. Mol. Cell Biol., 2014, 15 (6), 384-396) Although amyloid ﬁbrils are increasingly associated to biological functions, they were intially discovered in the context of pathological states. In particular, these peculiar protein aggregates are associated with the on- set and development of a large number of neurodegenerative diseaeses, including Alzheimer’s and Parkinson’s disorders, Amyotrophic Lateral Sclerosis and systemic amyloidosis.

Petkova et al. Science 307, 262–265 (2005).

Figure 9.10: TEM images of amyloid ﬁbrils

The medical doctor Aloises Alzheimer was the ﬁrst scientist who associated these structures observed in the brain of people aﬀected by the disease wit the loss of neuron function. Initially, these structures were thought to consist of starch (from which the word amyloid). However, later it was discovered that they were made of proteins. In many cases, the formation of amyloid ﬁbrils follows the incorrect folding of the pro- tein, a process deﬁned as misfolding. If the protein can not form the correct intramolecular bonds require to fold correclty, it can interact with other molecules to form aggregates. A very important observation is that a large variety of proteins can form amyloid ﬁbrils under suitable conditions. Moreover, even if the monomeric proteins have very few or no properties in common, the amyloid ﬁbrils share a large number of features, including in particular the

174 CHAPTER 9. PROTEIN AGGREGATION

Figure 9.11: Protein Misfolding and Amyloid Fibrils

morphology and a high content of secondary beta sheet structures. These observations induce people to consider amyloid ﬁbirls as an alternative form of folding, and some hypothesis con- sider the simple amyloid structure as the primordial form of folding, which has evolved during the years into more complex 3-D structures. An increasing series of evidence, including mutational studies, associate amyloids witht the onset and development of the disorders. However, the connection between the aggregation process and the lost of function is still largely unclear. Small reactive intermediates, which are formed during the aggregation pathway leading to the formation of ﬁbrils, are currently thought to represent the most toxic species. These intermediates, broadly deﬁned as oligomers, could damage neuronal cells via a series of processes, including membrane perforation, acti- vation of a cascade of signal and sequestration of key functional proteins. The problem is clearly very complex and interdisciplinary, involving contributions from clinical doctors, biologists, biochemists and biophysicists. Since amyloid ﬁbrils are colloids, several aspects of this stability problem share physico-chemical features with the systems dis- cussed in this course, as .described in the following paragraphs.

9.4.3 Kinetic and thermodynamic stability of amyloid ﬁbrils

The main driving force for the formation of amyloid ﬁbrils is their high thermodynamic stabil- ity. The beta sheet structures allow the formation of a large number of intermolecular hydrogen bonds, which are energetically very favorable. This explains why so many diﬀerent proteins

175 CHAPTER 9. PROTEIN AGGREGATION can convert into the amyloid state.

Figure 9.12: Thermodynamic stability of amyloid ﬁbrils

Since the aggregation process is concentration dependent, there is a critical concentration (dependent on the thermodynamics of the process) determining the stability or instability of a protein solution. For many proteins under physiological conditions this critical concentration is close to the physiological value: this observation indicates that proteins in biological sys- tems could be thermodyanamic unstable and only kinetically stable

Energy barrier: Intermolecular forces

stability time ∝ E/kBT

Figure 9.13: Kinetic stability of amyloid ﬁbrils

176 CHAPTER 9. PROTEIN AGGREGATION

9.4.4 Aggregation mechanism of amyloid ﬁbrils

The kinetics of the aggregation process plays therefore an important role in amyloids. In analogy with Chapter 7, we can decribe the time evolution of the ﬁbril size distribution by applying a population balance equation, replacing the concentration of particles Ni with the concentration of ﬁbrils containing j monomeric units, f j. There are, however, some diﬀerences in the aggregation mechanism that must be captured in the PBE (Figure 9.14): since aggregation occurs only in one dimesion at the ﬁbril ends, the aggregation step is replaced by elongation, with a rate constant k+ which is independent on the ﬁbril size (in contrast with the aggregation kernels described in Chapter 7) and only f j−1 and f j partecipate in the mass balance of f j. Additionally, we have to consider primary nucleation and secondary nucleation events, which appear in the mass balances of the smallest

ﬁbrils (containing nC and n2 monomeric units). Typical secondary nucleation reactions are: a) surface-induced secondary nucleation, where the surface of the existing ﬁbrils promotes the formation of new ﬁbril. The rate is therefore proportional to the total mass (surface) of the ﬁbrils in the system; b) fragmentation, because a breakage event creates two new ﬁbril reactive ends. In the descriptio of fragmentation (breakage), we have again the problem of the daughter distribution. We can assume the same probability of breakage for each bond within a ﬁbril, which implies that a ﬁbril with j monomeric units has j − 1 positions where brekage can occur. We note that the ﬁbrillar morphology of amyloids can be considered an extreme case of the fractal aggregates discussed in Chapter 7 with d f = 1. The PBE can be expressed as:

∞ d f j X = 2k f m − 2k f m − k ( j − 1) f + 2k f + δ k mnC + δ k Mmn2 (9.4) dt + j−1 + j − j − i j,nC n j,n2 2 i= j+1

P∞ where m(t) is the monomer concentration, M = i=nC i fi is the total ﬁbril mass concentration and the Kronecker delta operators δ j,nC and δ j,n2 are equal to one for j = nC or j = nC, and zero otherwise. The ﬁrst term on the right side of the equation accounts for the generation of ﬁlaments of length j by monomer addition to a shorter ﬁbril; the second term describes the disappearance of the ﬁbrils of length j which grow further to length j + 1; the third and fourth terms are related to fragmentation events and the last terms refer to the generation of new nuclei by primary and secondary nucleation events with reaction orders nC and n2, respectively. Recently available analytical solutions of the master equation led to closed expressions of the time evolution of the principal moments of the ﬁbril distribution, i.e., the ﬁbril number

177 CHAPTER 9. PROTEIN AGGREGATION

P∞ P∞ concentration, M = i=nC fi and the ﬁbril mass concentration, M = i=nC i fi, and provided insights into the relationship between relevant physical quantities of the system. An important application of the PBE is the possibility to extract information about the relative contribution of diﬀerent microscopic events on the total ﬁbril mass formation (the macroscopic experimental observable). This operation is relevant in many contexts, including the discovery of molecules which could block the aggregation process in vivo, as discussed in the next paragraph.

Figure 9.14: Microscopic aggregation mechanism of amyloid ﬁbrils

9.4.5 Role of chemical kinetics in drug discovery

Information about the microscopic processes underlying changes in macroscopic variables are crucial for understanding the mechanism of action of a given drug as well as for identify- ing strategies to change both the thermodynamics and the kinetics of the disease-associated

178 CHAPTER 9. PROTEIN AGGREGATION processes. This general strategy has found widespread applications in enzymology, where chemical kinetics has become a standard tool for testing inhibition mechanisms, including identifying competitive, uncompetitive and non-competitive inhibition mechanisms (Chapter 8). This approach has already resulted in signiﬁcant progress in the understanding of the mechanisms of action of enzymes and has led to the development of anti-cancer drugs target- ing kinases activity. The exact causative relationship between amyloid formation and organ dysfunction remains unclear, but the inhibition of protein aggregation is an attractive candidate for generating dis- ease modifying therapeutic strategies against Alzheimer’s disease and other neurodegenera- tive disorders because in all cases the toxicity has been associated to the soluble forms of the aggregating peptides. In this context, kinetics is not only a tool to investigate the inhibition mechanism but can represent also a therapeutic target per se, since the delay of the aggregation process for a suﬃciently large number of years can be considered as eﬀective as the thermo- dynamic inhibition of the process. However, either a thermodynamic or a kinetic inhibition should not aim at a generic arrest or delay of the formation of the ﬁnal ﬁbril load, but rather at a speciﬁc intervention on the molecular species that mediate cellular toxicity. Indeed, an un- controlled disassembly of higher order aggregates, thought to be relatively inert in a biological context, could lead to the increase in the concentration of soluble toxic oligomers and hence negative outcome in terms of rescuing toxicity. In order to develop eﬀective therapeutic strate- gies, therefore, an understanding is required not only of the protein aggregation process and its connection to pathogenicity, but also of how potential drugs interfere with these processes. We can apply the population balance equation platform to understand the inhibition mech- anism of ﬁbril formation at the molecular level. The key for applying this approach to analyse inhibition of aggregation is to note that the change in diﬀerent microscopic events results in diﬀerent characteristic macroscopic aggregation proﬁles, as shown qualitatively in the model simulations in Figure 9.15. For instance, the decrease of primary nucleation rate increases the lag-time preceding the growth phase. Elongation and secondary nucleation events have diﬀerent eﬀects on both lag-phase and growth, Surface induced secondary nucleation events become relevant at larger conversion values. As a consequence, a reduction of this micro- scopic step does not aﬀect signiﬁcantly the aggregation proﬁle at low conversion values. By contrast, a decrease of the elongation rate constant inhibits the formation of ﬁbrils from the early stages of the process. and therefore we can discriminate the inhibition of these two mi- croscopic processes by considering the macroscopic proﬁle of the kinetics of aggregation at diﬀerent protein and inhibitor concentrations.

179 CHAPTER 9. PROTEIN AGGREGATION

Figure 9.15: Kinetic modelling analysis of aggregation inhibition mechanism. The binding between the inhibitor (for instance, a molecular chaperone) and the diﬀerent species in the system leads to speciﬁc changes in the microscopic steps of the aggregation process, such as pri- mary nucleation, elongation and secondary heterogeneous processes. (a-c) Dot lines rep- resent model simulations of the macroscopic time evolution of ﬁbril formation, showing how changes in single speciﬁc microscopic aggregation events aﬀect in a characteristic way the observed kinetic macroscopic proﬁle (simulations are compared to experimental data, reported in diﬀerent colors). (d-f) Diﬀerent modalities of intervention have dramat- ically diﬀerent consequences on the concentraiton of toxic oligomers generated during the aggregation process.

It is important to observe that the speciﬁc inhibition of heterogeneous processes delays the ﬁbril formation but does not aﬀect the ﬁnal ﬁbril load, since monomers are still consumed by elongation events. To aﬀect the ﬁnal ﬁbril composition, a thermodynamic inhibition which prevents primary nucleation and elongation processes is required. On the other hand, the kinetic inhibition of secondary processes can suppress the generation of toxic intermediates, in contrast to the kinetic inhibition of primary nucleation and elongation processes, which delays but not suppresses the formation of soluble oligomers. For the speciﬁc system under consideration, calculations based on the kinetic model can quantify the qualitative aspects describe above, leading to the identiﬁcation of the inhibition strategy with the best potential therapeutic beneﬁts.

180 References

POLYMER REACTION ENGINEERING

Dotson, N. A., Polymerization process modeling. VCH: New York 1996. Flory, P. J., Principles of polymer chemistry; Cornell University Press, 2006. Hamielec, A. E., Polymerization Processes, 2. Modeling of Processes and Reactors. Ull- mann’s Encyclopedia, Wiley-VCH 2000. Nomura, M., Emulsion polymerization: Kinetic and mechanistic aspects. Polymer Particles 2005, 175, 1-128. Odian, G., Principles of polymerization. 4th ed.; Wiley, 2004

COLLOIDAL ENGINEERING

Berg, J. C., An introduction to interfaces and colloids the bridge to nanoscience. World Sci- entiﬁc 2010. Cosgrove, T., Colloid science principles, methods and applications. 2nd ed.; Wiley 2010. Friedlander, S. K., Smoke, dust, and haze fundamentals of aerosol dynamics. 2nd ed.; Oxford University Press 2000. Israelachvili, J. N., Intermolecular and surface forces. 3rd ed.; Academic Press 2011. Jia, Z. C., A generalized model for the stability of polymer colloids. Journal of Colloid and Interface Science 2006. Lin, M. Y., Universality in Colloid Aggregation. Nature 1989, 339, 360-362. Sandkuhler, P., Modeling structure eﬀects on aggregation kinetics in colloidal dispersions. Aiche Journal 2003, 49, 1542-1555.

181 CHAPTER 9. PROTEIN AGGREGATION

BIOCHEMICAL ENGINEERING

Blanch, H. W., Clark, D. S. Biochemical Engineering; Marcel Dekker , Inc. 1996. Villadsen, J., Nielsen, J., Liden, G. Bioreaction Engineering Principles. 3rd ed.; Springer New York 2011. Wang, W., Protein aggregation and its inhibition in biopharmaceutics. Intenational Journal of Pharmaceutics 2005, 289, 1-30. Nicoud, L. et al., A multiscale view of therapeutic protein aggregation: A colloid science per- spective. Biotechnology J., 2015. Knowles, T.P.J. et al., The amyloid state and its association with protein misfolding diseases. Nat. Rev. Mol. Cell Biol., 2014, 15 (6), 384-396.

182